#------------------------------------------------------------------------------
#$Date: 2016-02-20 02:53:41 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176768 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/58/2105806.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2105806
loop_
_publ_author_name
'Okamoto, Norihiko L.'
'Tanaka, Katsushi'
'Yasuhara, Akira'
'Inui, Haruyuki'
_publ_section_title
;
 Structure refinement of the δ₁ₚ phase in the Fe--Zn system by
 single-crystal X-ray diffraction combined with scanning transmission
 electron microscopy
;
_journal_coeditor_code           DK5020
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              275
_journal_page_last               282
_journal_paper_doi               10.1107/S2052520613034410
_journal_volume                  70
_journal_year                    2014
_chemical_formula_sum            'Fe13 Zn126'
_chemical_formula_weight         8963.89
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            4
_cell_length_a                   12.8297(2)
_cell_length_b                   12.8297(2)
_cell_length_c                   57.2860(10)
_cell_measurement_reflns_used    301081
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      23.215
_cell_measurement_theta_min      0.355
_cell_volume                     8166.1(2)
_computing_cell_refinement       'CrystalClear (Rigaku/MSC Inc., 2006)'
_computing_data_collection       'CrystalClear (Rigaku/MSC Inc., 2006)'
_computing_data_reduction
'CrystalClear (Rigaku/MSC Inc., 2006), SORTAV (Blessing, 1995)'
_computing_molecular_graphics    'Ortep-3 for Windows (Farrugia, 1997)'
_computing_publication_material  'WinGX publication routines (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR92 (Giacovazzo et al, 1993)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'HUBER 4-circle diffractometer'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  'Si(111) double crystal'
_diffrn_radiation_source         'SPring-8 BL02B1'
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.35450
_diffrn_reflns_av_R_equivalents  0.0277
_diffrn_reflns_av_sigmaI/netI    0.0091
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       127
_diffrn_reflns_limit_l_min       -99
_diffrn_reflns_number            203263
_diffrn_reflns_theta_full        23.19
_diffrn_reflns_theta_max         23.19
_diffrn_reflns_theta_min         0.35
_exptl_absorpt_coefficient_mu    20.094
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            metallic_silver
_exptl_crystal_density_diffrn    7.290
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             16472
_exptl_crystal_size_max          0.034
_exptl_crystal_size_mid          0.034
_exptl_crystal_size_min          0.025
_refine_diff_density_max         5.906
_refine_diff_density_min         -4.164
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_matrix_type           full
_refine_ls_number_parameters     308
_refine_ls_number_reflns         16996
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.025
_refine_ls_R_factor_all          0.0387
_refine_ls_R_factor_gt           0.0314
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1197
_refine_ls_wR_factor_ref         0.1272
_reflns_number_gt                14411
_reflns_number_total             16996
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            dk5020sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        8166.0(3)
_cod_database_code               2105806
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, -x, -z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -x+y, -z'
'-y, x-y, z'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x+y, -x, z'
'-x, -y, -z'
'x, y, -z-1/2'
'y, x, z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
'x, x-y, z'
'y, -x+y, -z'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'x-y, x, -z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Fe Fe1 0.0000 0.0000 0.0000 0.00527(7) Uani d S 1 12
Fe Fe2 0.778964(12) 0.55793(2) 0.016364(5) 0.00803(4) Uani d S 1 2
Fe Fe3 0.135983(12) 0.27197(2) 0.068947(5) 0.00691(3) Uani d S 1 2
Fe Fe4 0.6667 0.3333 0.140259(8) 0.00727(6) Uani d S 1 6
Fe Fe5 0.3333 0.6667 0.176805(8) 0.00649(5) Uani d S 1 6
Fe Fe6 0.112908(12) 0.22582(2) 0.203999(5) 0.00797(4) Uani d S 1 2
Fe Fe7 0.467086(16) 0.93417(3) 0.2500 0.00644(4) Uani d S 1 4
Zn Zn1 0.36258(2) 0.0000 0.0000 0.01322(4) Uani d S 1 2
Zn Zn2 0.886968(11) 0.77394(2) 0.008273(5) 0.01032(4) Uani d S 1 2
Zn Zn3 0.409779(17) 0.81956(3) 0.013189(7) 0.01796(5) Uani d S 1 2
Zn Zn4 0.6667 0.3333 0.024338(11) 0.01412(7) Uani d S 1 6
Zn Zn5 0.195007(15) 0.39001(3) 0.027654(5) 0.01408(4) Uani d S 1 2
Zn Zn6 0.547279(16) 0.09456(3) 0.031300(6) 0.01631(5) Uani d S 1 2
Zn Zn7 0.070702(12) 0.14140(2) 0.034645(5) 0.01019(4) Uani d S 1 2
Zn Zn8 0.31463(2) 0.043982(19) 0.045093(4) 0.01400(3) Uani d . 1 1
Zn Zn9 0.3333 0.6667 0.049028(10) 0.01445(7) Uani d S 1 6
Zn Zn10 0.748900(18) 0.49780(4) 0.061364(7) 0.01972(6) Uani d S 1 2
Zn Zn11 0.12927(2) 0.46834(2) 0.065150(5) 0.01773(4) Uani d . 1 1
Zn Zn12 0.926395(14) 0.85279(3) 0.072510(6) 0.01366(4) Uani d S 1 2
Zn Zn13 0.539021(15) 0.07804(3) 0.078016(7) 0.01707(5) Uani d S 1 2
Zn Zn14 0.31767(2) 0.03900(3) 0.092485(5) 0.01927(4) Uani d . 1 1
Zn Zn15 0.3333 0.6667 0.095657(12) 0.01959(9) Uani d S 1 6
Zn Zn16 0.203460(18) 0.40692(4) 0.104581(7) 0.01982(6) Uani d S 1 2
Zn Zn17 0.08343(2) 0.16685(4) 0.109300(6) 0.02174(6) Uani d S 1 2
Zn Zn18 0.450604(15) 0.90121(3) 0.110691(6) 0.01602(5) Uani d S 1 2
Zn Zn19 0.880762(18) 0.76152(4) 0.133888(9) 0.02284(7) Uani d S 1 2
Zn Zn20 0.02467(3) 0.35593(2) 0.137760(5) 0.02100(5) Uani d . 1 1
Zn Zn21 0.0000 0.0000 0.140576(9) 0.01196(6) Uani d S 1 6
Zn Zn22 0.263172(19) 0.52634(4) 0.141423(7) 0.02070(6) Uani d S 1 2
Zn Zn23 0.115585(16) 0.23117(3) 0.156940(7) 0.01743(5) Uani d S 1 2
Zn Zn24 0.450812(16) 0.90162(3) 0.167752(7) 0.01706(5) Uani d S 1 2
Zn Zn25 0.929536(17) 0.85907(3) 0.180384(6) 0.01646(5) Uani d S 1 2
Zn Zn26 0.32347(2) 0.02481(2) 0.183150(5) 0.01877(4) Uani d . 1 1
Zn Zn27 0.217903(13) 0.43581(3) 0.185444(7) 0.01594(5) Uani d S 1 2
Zn Zn28 0.77367(2) 0.54734(4) 0.206781(7) 0.02064(6) Uani d S 1 2
Zn Zn29 0.530806(16) 0.06161(3) 0.209540(6) 0.01621(5) Uani d S 1 2
Zn Zn30 0.406225(13) 0.81245(3) 0.211558(5) 0.01256(4) Uani d S 1 2
Zn Zn31 0.0000 0.0000 0.219762(10) 0.01400(7) Uani d S 1 6
Zn Zn32 0.883244(18) 0.76649(4) 0.224248(9) 0.02180(6) Uani d S 1 2
Zn Zn33 0.06262(2) 0.36123(2) 0.226383(4) 0.01521(4) Uani d . 1 1
Zn Zn34 0.6667 0.3333 0.228077(10) 0.01658(8) Uani d S 1 6
Zn Zn35 0.26171(2) 0.52342(4) 0.2500 0.01364(6) Uani d S 1 4
Zn Zn36 0.09541(2) 0.19081(4) 0.2500 0.01414(6) Uani d S 1 4
Zn Zn37 0.45884(4) 0.13192(3) 0.2500 0.01935(6) Uani d S 1 2
Zn Zn38 0.67731(5) 0.35463(10) 0.094695(15) 0.0182(3) Uani d SP 0.3333333 2
Zn Zn39 0.48205(8) 0.18194(9) 0.115304(17) 0.02807(19) Uani d P 0.3333333 1
Zn Zn40 0.53703(7) 0.12796(7) 0.121980(14) 0.02086(13) Uani d P 0.3333333 1
Zn Zn41 0.77424(5) 0.54849(10) 0.12343(3) 0.0256(2) Uani d SP 0.3333333 2
Zn Zn42 0.55462(5) 0.10925(10) 0.15604(3) 0.0246(2) Uani d SP 0.3333333 2
Zn Zn43 0.44959(6) 0.20792(6) 0.158150(13) 0.01907(16) Uani d P 0.3333333 1
Zn Zn44 0.52508(9) 0.14852(9) 0.165183(16) 0.0316(2) Uani d P 0.3333333 1
Zn Zn45 0.65079(5) 0.30157(10) 0.184156(16) 0.01928(17) Uani d SP 0.333333 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.154 0.227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.213 0.402 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Zn7 Fe1 Zn7 . 16 65.031(10)
Zn7 Fe1 Zn7 . 20 65.031(10)
Zn7 Fe1 Zn7 16 20 65.031(10)
Zn7 Fe1 Zn7 . 13 180.000(10)
Zn7 Fe1 Zn7 16 13 114.969(10)
Zn7 Fe1 Zn7 20 13 114.969(10)
Zn7 Fe1 Zn7 . 4 114.969(10)
Zn7 Fe1 Zn7 16 4 180.000(10)
Zn7 Fe1 Zn7 20 4 114.969(10)
Zn7 Fe1 Zn7 13 4 65.031(10)
Zn7 Fe1 Zn7 . 8 114.969(10)
Zn7 Fe1 Zn7 16 8 114.969(10)
Zn7 Fe1 Zn7 20 8 180.000(7)
Zn7 Fe1 Zn7 13 8 65.031(10)
Zn7 Fe1 Zn7 4 8 65.031(10)
Zn7 Fe1 Zn2 . 4_445 116.765(5)
Zn7 Fe1 Zn2 16 4_445 62.319(9)
Zn7 Fe1 Zn2 20 4_445 116.765(5)
Zn7 Fe1 Zn2 13 4_445 63.235(5)
Zn7 Fe1 Zn2 4 4_445 117.681(9)
Zn7 Fe1 Zn2 8 4_445 63.235(5)
Zn7 Fe1 Zn2 . 13_665 62.319(9)
Zn7 Fe1 Zn2 16 13_665 116.765(5)
Zn7 Fe1 Zn2 20 13_665 116.765(5)
Zn7 Fe1 Zn2 13 13_665 117.681(9)
Zn7 Fe1 Zn2 4 13_665 63.235(5)
Zn7 Fe1 Zn2 8 13_665 63.235(5)
Zn2 Fe1 Zn2 4_445 13_665 116.643(4)
Zn7 Fe1 Zn2 . 16_665 63.235(5)
Zn7 Fe1 Zn2 16 16_665 117.681(9)
Zn7 Fe1 Zn2 20 16_665 63.235(5)
Zn7 Fe1 Zn2 13 16_665 116.765(5)
Zn7 Fe1 Zn2 4 16_665 62.319(9)
Zn7 Fe1 Zn2 8 16_665 116.765(5)
Zn2 Fe1 Zn2 4_445 16_665 180.000(12)
Zn2 Fe1 Zn2 13_665 16_665 63.357(4)
Zn7 Fe1 Zn2 . 8_655 116.765(5)
Zn7 Fe1 Zn2 16 8_655 116.765(5)
Zn7 Fe1 Zn2 20 8_655 62.319(9)
Zn7 Fe1 Zn2 13 8_655 63.235(5)
Zn7 Fe1 Zn2 4 8_655 63.235(5)
Zn7 Fe1 Zn2 8 8_655 117.681(9)
Zn2 Fe1 Zn2 4_445 8_655 116.643(4)
Zn2 Fe1 Zn2 13_665 8_655 116.643(4)
Zn2 Fe1 Zn2 16_665 8_655 63.357(4)
Zn7 Fe1 Zn2 . 1_445 117.681(9)
Zn7 Fe1 Zn2 16 1_445 63.235(5)
Zn7 Fe1 Zn2 20 1_445 63.235(5)
Zn7 Fe1 Zn2 13 1_445 62.319(9)
Zn7 Fe1 Zn2 4 1_445 116.765(5)
Zn7 Fe1 Zn2 8 1_445 116.765(5)
Zn2 Fe1 Zn2 4_445 1_445 63.357(4)
Zn2 Fe1 Zn2 13_665 1_445 180.000(14)
Zn2 Fe1 Zn2 16_665 1_445 116.643(4)
Zn2 Fe1 Zn2 8_655 1_445 63.357(4)
Zn7 Fe1 Zn2 . 20_455 63.235(5)
Zn7 Fe1 Zn2 16 20_455 63.235(5)
Zn7 Fe1 Zn2 20 20_455 117.681(9)
Zn7 Fe1 Zn2 13 20_455 116.765(5)
Zn7 Fe1 Zn2 4 20_455 116.765(5)
Zn7 Fe1 Zn2 8 20_455 62.319(9)
Zn2 Fe1 Zn2 4_445 20_455 63.357(4)
Zn2 Fe1 Zn2 13_665 20_455 63.357(4)
Zn2 Fe1 Zn2 16_665 20_455 116.643(4)
Zn2 Fe1 Zn2 8_655 20_455 180.000(12)
Zn2 Fe1 Zn2 1_445 20_455 116.643(4)
Zn2 Fe2 Zn4 . . 179.44(2)
Zn2 Fe2 Zn5 . 13_665 66.151(12)
Zn4 Fe2 Zn5 . 13_665 113.293(19)
Zn2 Fe2 Zn8 . 16_665 65.630(9)
Zn4 Fe2 Zn8 . 16_665 114.811(15)
Zn5 Fe2 Zn8 13_665 16_665 119.522(12)
Zn2 Fe2 Zn8 . 12_665 65.630(9)
Zn4 Fe2 Zn8 . 12_665 114.811(15)
Zn5 Fe2 Zn8 13_665 12_665 119.522(12)
Zn8 Fe2 Zn8 16_665 12_665 67.623(13)
Zn2 Fe2 Zn1 . 8_665 66.858(9)
Zn4 Fe2 Zn1 . 8_665 112.970(10)
Zn5 Fe2 Zn1 13_665 8_665 65.296(6)
Zn8 Fe2 Zn1 16_665 8_665 121.930(12)
Zn8 Fe2 Zn1 12_665 8_665 63.593(7)
Zn2 Fe2 Zn1 . 16_665 66.858(9)
Zn4 Fe2 Zn1 . 16_665 112.970(10)
Zn5 Fe2 Zn1 13_665 16_665 65.296(6)
Zn8 Fe2 Zn1 16_665 16_665 63.593(7)
Zn8 Fe2 Zn1 12_665 16_665 121.930(12)
Zn1 Fe2 Zn1 8_665 16_665 122.051(15)
Zn2 Fe2 Zn10 . . 115.459(16)
Zn4 Fe2 Zn10 . . 65.098(18)
Zn5 Fe2 Zn10 13_665 . 178.390(17)
Zn8 Fe2 Zn10 16_665 . 61.721(11)
Zn8 Fe2 Zn10 12_665 . 61.721(11)
Zn1 Fe2 Zn10 8_665 . 115.128(7)
Zn1 Fe2 Zn10 16_665 . 115.128(7)
Zn2 Fe2 Zn6 . 16_665 118.835(9)
Zn4 Fe2 Zn6 . 16_665 61.311(9)
Zn5 Fe2 Zn6 13_665 16_665 113.783(11)
Zn8 Fe2 Zn6 16_665 16_665 64.156(9)
Zn8 Fe2 Zn6 12_665 16_665 120.364(14)
Zn1 Fe2 Zn6 8_665 16_665 173.750(14)
Zn1 Fe2 Zn6 16_665 16_665 60.923(9)
Zn10 Fe2 Zn6 . 16_665 65.611(10)
Zn2 Fe2 Zn6 . 20 118.835(9)
Zn4 Fe2 Zn6 . 20 61.311(9)
Zn5 Fe2 Zn6 13_665 20 113.783(11)
Zn8 Fe2 Zn6 16_665 20 120.364(14)
Zn8 Fe2 Zn6 12_665 20 64.156(9)
Zn1 Fe2 Zn6 8_665 20 60.923(9)
Zn1 Fe2 Zn6 16_665 20 173.750(14)
Zn10 Fe2 Zn6 . 20 65.612(10)
Zn6 Fe2 Zn6 16_665 20 115.536(18)
Zn2 Fe2 Zn3 . 4 117.745(13)
Zn4 Fe2 Zn3 . 4 61.809(14)
Zn5 Fe2 Zn3 13_665 4 62.558(11)
Zn8 Fe2 Zn3 16_665 4 114.182(9)
Zn8 Fe2 Zn3 12_665 4 176.516(14)
Zn1 Fe2 Zn3 8_665 4 116.397(12)
Zn1 Fe2 Zn3 16_665 4 61.273(10)
Zn10 Fe2 Zn3 . 4 116.145(13)
Zn6 Fe2 Zn3 16_665 4 59.321(10)
Zn6 Fe2 Zn3 20 4 112.606(13)
Zn2 Fe2 Zn3 . 8_655 117.745(13)
Zn4 Fe2 Zn3 . 8_655 61.809(14)
Zn5 Fe2 Zn3 13_665 8_655 62.558(11)
Zn8 Fe2 Zn3 16_665 8_655 176.516(14)
Zn8 Fe2 Zn3 12_665 8_655 114.182(9)
Zn1 Fe2 Zn3 8_665 8_655 61.273(10)
Zn1 Fe2 Zn3 16_665 8_655 116.397(12)
Zn10 Fe2 Zn3 . 8_655 116.145(13)
Zn6 Fe2 Zn3 16_665 8_655 112.606(13)
Zn6 Fe2 Zn3 20 8_655 59.321(10)
Zn3 Fe2 Zn3 4 8_655 63.849(16)
Zn7 Fe3 Zn16 . . 179.863(19)
Zn7 Fe3 Zn11 . 17 115.828(12)
Zn16 Fe3 Zn11 . 17 64.284(12)
Zn7 Fe3 Zn11 . . 115.828(12)
Zn16 Fe3 Zn11 . . 64.284(12)
Zn11 Fe3 Zn11 17 . 63.079(13)
Zn7 Fe3 Zn17 . . 116.760(16)
Zn16 Fe3 Zn17 . . 63.103(16)
Zn11 Fe3 Zn17 17 . 117.252(14)
Zn11 Fe3 Zn17 . . 117.252(14)
Zn7 Fe3 Zn12 . 16_665 64.174(10)
Zn16 Fe3 Zn12 . 16_665 115.716(14)
Zn11 Fe3 Zn12 17 16_665 115.841(9)
Zn11 Fe3 Zn12 . 16_665 178.869(13)
Zn17 Fe3 Zn12 . 16_665 63.415(13)
Zn7 Fe3 Zn12 . 20_455 64.174(10)
Zn16 Fe3 Zn12 . 20_455 115.716(14)
Zn11 Fe3 Zn12 17 20_455 178.869(13)
Zn11 Fe3 Zn12 . 20_455 115.841(9)
Zn17 Fe3 Zn12 . 20_455 63.415(13)
Zn12 Fe3 Zn12 16_665 20_455 65.236(15)
Zn7 Fe3 Zn14 . 20 115.148(9)
Zn16 Fe3 Zn14 . 20 64.810(9)
Zn11 Fe3 Zn14 17 20 64.448(9)
Zn11 Fe3 Zn14 . 20 118.010(13)
Zn17 Fe3 Zn14 . 20 63.873(8)
Zn12 Fe3 Zn14 16_665 20 61.307(10)
Zn12 Fe3 Zn14 20_455 20 116.634(13)
Zn7 Fe3 Zn14 . 9 115.148(9)
Zn16 Fe3 Zn14 . 9 64.810(9)
Zn11 Fe3 Zn14 17 9 118.010(13)
Zn11 Fe3 Zn14 . 9 64.448(9)
Zn17 Fe3 Zn14 . 9 63.873(8)
Zn12 Fe3 Zn14 16_665 9 116.634(13)
Zn12 Fe3 Zn14 20_455 9 61.307(10)
Zn14 Fe3 Zn14 20 9 118.899(15)
Zn7 Fe3 Zn8 . 9 65.537(8)
Zn16 Fe3 Zn8 . 9 114.508(8)
Zn11 Fe3 Zn8 17 9 114.279(12)
Zn11 Fe3 Zn8 . 9 60.773(9)
Zn17 Fe3 Zn8 . 9 116.959(8)
Zn12 Fe3 Zn8 16_665 9 119.902(13)
Zn12 Fe3 Zn8 20_455 9 64.637(9)
Zn14 Fe3 Zn8 20 9 178.692(14)
Zn14 Fe3 Zn8 9 9 61.246(8)
Zn7 Fe3 Zn8 . 20 65.537(8)
Zn16 Fe3 Zn8 . 20 114.508(8)
Zn11 Fe3 Zn8 17 20 60.773(9)
Zn11 Fe3 Zn8 . 20 114.279(12)
Zn17 Fe3 Zn8 . 20 116.959(8)
Zn12 Fe3 Zn8 16_665 20 64.637(9)
Zn12 Fe3 Zn8 20_455 20 119.902(13)
Zn14 Fe3 Zn8 20 20 61.246(8)
Zn14 Fe3 Zn8 9 20 178.692(14)
Zn8 Fe3 Zn8 9 20 118.576(14)
Zn7 Fe3 Zn5 . . 65.443(11)
Zn16 Fe3 Zn5 . . 114.694(16)
Zn11 Fe3 Zn5 17 . 60.975(10)
Zn11 Fe3 Zn5 . . 60.975(10)
Zn17 Fe3 Zn5 . . 177.797(17)
Zn12 Fe3 Zn5 16_665 . 118.335(12)
Zn12 Fe3 Zn5 20_455 . 118.335(12)
Zn14 Fe3 Zn5 20 . 115.485(8)
Zn14 Fe3 Zn5 9 . 115.485(8)
Zn8 Fe3 Zn5 9 . 63.642(8)
Zn8 Fe3 Zn5 20 . 63.642(8)
Zn40 Fe4 Zn40 17_655 . 15.69(4)
Zn40 Fe4 Zn40 17_655 9_655 90.72(4)
Zn40 Fe4 Zn40 . 9_655 104.12(3)
Zn40 Fe4 Zn40 17_655 16_665 104.12(3)
Zn40 Fe4 Zn40 . 16_665 115.98(4)
Zn40 Fe4 Zn40 9_655 16_665 15.69(4)
Zn40 Fe4 Zn40 17_655 20 104.12(3)
Zn40 Fe4 Zn40 . 20 90.72(4)
Zn40 Fe4 Zn40 9_655 20 115.98(4)
Zn40 Fe4 Zn40 16_665 20 104.12(3)
Zn40 Fe4 Zn40 17_655 12_665 115.98(4)
Zn40 Fe4 Zn40 . 12_665 104.12(3)
Zn40 Fe4 Zn40 9_655 12_665 104.12(3)
Zn40 Fe4 Zn40 16_665 12_665 90.72(4)
Zn40 Fe4 Zn40 20 12_665 15.69(4)
Zn40 Fe4 Zn45 17_655 16_665 117.09(2)
Zn40 Fe4 Zn45 . 16_665 119.22(3)
Zn40 Fe4 Zn45 9_655 16_665 106.50(3)
Zn40 Fe4 Zn45 16_665 16_665 106.50(3)
Zn40 Fe4 Zn45 20 16_665 119.22(3)
Zn40 Fe4 Zn45 12_665 16_665 117.09(2)
Zn40 Fe4 Zn45 17_655 . 106.50(3)
Zn40 Fe4 Zn45 . . 106.50(3)
Zn40 Fe4 Zn45 9_655 . 117.09(2)
Zn40 Fe4 Zn45 16_665 . 119.22(3)
Zn40 Fe4 Zn45 20 . 117.09(2)
Zn40 Fe4 Zn45 12_665 . 119.22(3)
Zn45 Fe4 Zn45 16_665 . 13.82(4)
Zn40 Fe4 Zn45 17_655 20 119.22(3)
Zn40 Fe4 Zn45 . 20 117.09(2)
Zn40 Fe4 Zn45 9_655 20 119.22(3)
Zn40 Fe4 Zn45 16_665 20 117.09(2)
Zn40 Fe4 Zn45 20 20 106.50(3)
Zn40 Fe4 Zn45 12_665 20 106.50(3)
Zn45 Fe4 Zn45 16_665 20 13.82(4)
Zn45 Fe4 Zn45 . 20 13.82(4)
Zn40 Fe4 Zn41 17_655 20 47.03(2)
Zn40 Fe4 Zn41 . 20 62.46(2)
Zn40 Fe4 Zn41 9_655 20 47.03(2)
Zn40 Fe4 Zn41 16_665 20 62.46(2)
Zn40 Fe4 Zn41 20 20 132.88(5)
Zn40 Fe4 Zn41 12_665 20 132.88(5)
Zn45 Fe4 Zn41 16_665 20 107.81(4)
Zn45 Fe4 Zn41 . 20 107.81(4)
Zn45 Fe4 Zn41 20 20 119.95(5)
Zn40 Fe4 Zn41 17_655 16_665 62.46(2)
Zn40 Fe4 Zn41 . 16_665 47.03(2)
Zn40 Fe4 Zn41 9_655 16_665 132.88(5)
Zn40 Fe4 Zn41 16_665 16_665 132.88(5)
Zn40 Fe4 Zn41 20 16_665 47.03(2)
Zn40 Fe4 Zn41 12_665 16_665 62.46(2)
Zn45 Fe4 Zn41 16_665 16_665 119.95(5)
Zn45 Fe4 Zn41 . 16_665 107.81(4)
Zn45 Fe4 Zn41 20 16_665 107.81(4)
Zn41 Fe4 Zn41 20 16_665 106.87(4)
Zn40 Fe4 Zn41 17_655 . 132.88(5)
Zn40 Fe4 Zn41 . . 132.88(5)
Zn40 Fe4 Zn41 9_655 . 62.46(2)
Zn40 Fe4 Zn41 16_665 . 47.03(2)
Zn40 Fe4 Zn41 20 . 62.46(2)
Zn40 Fe4 Zn41 12_665 . 47.03(2)
Zn45 Fe4 Zn41 16_665 . 107.81(4)
Zn45 Fe4 Zn41 . . 119.95(5)
Zn45 Fe4 Zn41 20 . 107.81(4)
Zn41 Fe4 Zn41 20 . 106.87(4)
Zn41 Fe4 Zn41 16_665 . 106.87(4)
Zn22 Fe5 Zn22 20_565 . 63.742(19)
Zn22 Fe5 Zn22 20_565 16_665 63.742(19)
Zn22 Fe5 Zn22 . 16_665 63.742(19)
Zn22 Fe5 Zn30 20_565 . 114.990(10)
Zn22 Fe5 Zn30 . . 178.435(18)
Zn22 Fe5 Zn30 16_665 . 114.990(10)
Zn22 Fe5 Zn30 20_565 16_665 114.990(10)
Zn22 Fe5 Zn30 . 16_665 114.990(10)
Zn22 Fe5 Zn30 16_665 16_665 178.435(17)
Zn30 Fe5 Zn30 . 16_665 66.262(15)
Zn22 Fe5 Zn30 20_565 20_565 178.435(18)
Zn22 Fe5 Zn30 . 20_565 114.990(10)
Zn22 Fe5 Zn30 16_665 20_565 114.990(10)
Zn30 Fe5 Zn30 . 20_565 66.262(15)
Zn30 Fe5 Zn30 16_665 20_565 66.262(15)
Zn22 Fe5 Zn27 20_565 20_565 63.353(14)
Zn22 Fe5 Zn27 . 20_565 116.710(13)
Zn22 Fe5 Zn27 16_665 20_565 116.711(13)
Zn30 Fe5 Zn27 . 20_565 62.820(9)
Zn30 Fe5 Zn27 16_665 20_565 62.820(9)
Zn30 Fe5 Zn27 20_565 20_565 118.21(2)
Zn22 Fe5 Zn27 20_565 16_665 116.711(13)
Zn22 Fe5 Zn27 . 16_665 116.711(13)
Zn22 Fe5 Zn27 16_665 16_665 63.353(14)
Zn30 Fe5 Zn27 . 16_665 62.820(9)
Zn30 Fe5 Zn27 16_665 16_665 118.21(2)
Zn30 Fe5 Zn27 20_565 16_665 62.820(9)
Zn27 Fe5 Zn27 20_565 16_665 116.498(8)
Zn22 Fe5 Zn27 20_565 . 116.710(13)
Zn22 Fe5 Zn27 . . 63.353(14)
Zn22 Fe5 Zn27 16_665 . 116.710(13)
Zn30 Fe5 Zn27 . . 118.21(2)
Zn30 Fe5 Zn27 16_665 . 62.820(9)
Zn30 Fe5 Zn27 20_565 . 62.820(9)
Zn27 Fe5 Zn27 20_565 . 116.498(8)
Zn27 Fe5 Zn27 16_665 . 116.498(8)
Zn22 Fe5 Zn24 20_565 16_665 63.034(9)
Zn22 Fe5 Zn24 . 16_665 63.034(9)
Zn22 Fe5 Zn24 16_665 16_665 116.33(2)
Zn30 Fe5 Zn24 . 16_665 117.429(12)
Zn30 Fe5 Zn24 16_665 16_665 62.105(11)
Zn30 Fe5 Zn24 20_565 16_665 117.429(12)
Zn27 Fe5 Zn24 20_565 16_665 63.601(4)
Zn27 Fe5 Zn24 16_665 16_665 179.68(2)
Zn27 Fe5 Zn24 . 16_665 63.601(4)
Zn22 Fe5 Zn24 20_565 . 63.034(9)
Zn22 Fe5 Zn24 . . 116.33(2)
Zn22 Fe5 Zn24 16_665 . 63.034(9)
Zn30 Fe5 Zn24 . . 62.104(11)
Zn30 Fe5 Zn24 16_665 . 117.429(12)
Zn30 Fe5 Zn24 20_565 . 117.429(12)
Zn27 Fe5 Zn24 20_565 . 63.601(4)
Zn27 Fe5 Zn24 16_665 . 63.601(4)
Zn27 Fe5 Zn24 . . 179.68(2)
Zn24 Fe5 Zn24 16_665 . 116.298(8)
Zn22 Fe5 Zn24 20_565 20_565 116.33(2)
Zn22 Fe5 Zn24 . 20_565 63.034(9)
Zn22 Fe5 Zn24 16_665 20_565 63.035(9)
Zn30 Fe5 Zn24 . 20_565 117.429(12)
Zn30 Fe5 Zn24 16_665 20_565 117.429(12)
Zn30 Fe5 Zn24 20_565 20_565 62.105(11)
Zn27 Fe5 Zn24 20_565 20_565 179.68(2)
Zn27 Fe5 Zn24 16_665 20_565 63.601(4)
Zn27 Fe5 Zn24 . 20_565 63.601(4)
Zn24 Fe5 Zn24 16_665 20_565 116.298(8)
Zn24 Fe5 Zn24 . 20_565 116.298(8)
Zn33 Fe6 Zn33 17 . 74.890(15)
Zn33 Fe6 Zn27 17 . 70.344(11)
Zn33 Fe6 Zn27 . . 70.344(11)
Zn33 Fe6 Zn25 17 16_665 110.789(10)
Zn33 Fe6 Zn25 . 16_665 173.966(13)
Zn27 Fe6 Zn25 . 16_665 113.060(14)
Zn33 Fe6 Zn25 17 20_455 173.966(13)
Zn33 Fe6 Zn25 . 20_455 110.790(10)
Zn27 Fe6 Zn25 . 20_455 113.060(14)
Zn25 Fe6 Zn25 16_665 20_455 63.461(18)
Zn33 Fe6 Zn26 17 20 62.395(9)
Zn33 Fe6 Zn26 . 20 123.928(14)
Zn27 Fe6 Zn26 . 20 62.411(9)
Zn25 Fe6 Zn26 16_665 20 61.725(11)
Zn25 Fe6 Zn26 20_455 20 114.200(14)
Zn33 Fe6 Zn26 17 9 123.928(14)
Zn33 Fe6 Zn26 . 9 62.395(9)
Zn27 Fe6 Zn26 . 9 62.411(9)
Zn25 Fe6 Zn26 16_665 9 114.200(14)
Zn25 Fe6 Zn26 20_455 9 61.725(11)
Zn26 Fe6 Zn26 20 9 114.294(16)
Zn33 Fe6 Zn36 17 . 65.086(11)
Zn33 Fe6 Zn36 . . 65.086(11)
Zn27 Fe6 Zn36 . . 122.888(17)
Zn25 Fe6 Zn36 16_665 . 114.916(14)
Zn25 Fe6 Zn36 20_455 . 114.916(14)
Zn26 Fe6 Zn36 20 . 119.255(9)
Zn26 Fe6 Zn36 9 . 119.255(9)
Zn33 Fe6 Zn31 17 . 113.213(14)
Zn33 Fe6 Zn31 . . 113.212(14)
Zn27 Fe6 Zn31 . . 175.302(19)
Zn25 Fe6 Zn31 16_665 . 63.114(13)
Zn25 Fe6 Zn31 20_455 . 63.114(13)
Zn26 Fe6 Zn31 20 . 116.003(10)
Zn26 Fe6 Zn31 9 . 116.003(10)
Zn36 Fe6 Zn31 . . 61.811(16)
Zn33 Fe6 Zn23 17 . 120.102(12)
Zn33 Fe6 Zn23 . . 120.102(11)
Zn27 Fe6 Zn23 . . 64.243(13)
Zn25 Fe6 Zn23 16_665 . 59.353(11)
Zn25 Fe6 Zn23 20_455 . 59.353(11)
Zn26 Fe6 Zn23 20 . 62.891(8)
Zn26 Fe6 Zn23 9 . 62.891(8)
Zn36 Fe6 Zn23 . . 172.869(17)
Zn31 Fe6 Zn23 . . 111.059(17)
Zn33 Fe6 Zn32 17 16_665 63.951(10)
Zn33 Fe6 Zn32 . 16_665 122.362(15)
Zn27 Fe6 Zn32 . 16_665 124.386(9)
Zn25 Fe6 Zn32 16_665 16_665 60.418(12)
Zn25 Fe6 Zn32 20_455 16_665 110.438(14)
Zn26 Fe6 Zn32 20 16_665 69.154(11)
Zn26 Fe6 Zn32 9 16_665 172.077(14)
Zn36 Fe6 Zn32 . 16_665 61.812(11)
Zn31 Fe6 Zn32 . 16_665 56.859(9)
Zn23 Fe6 Zn32 . 16_665 115.033(12)
Zn33 Fe6 Zn32 17 20_455 122.362(15)
Zn33 Fe6 Zn32 . 20_455 63.951(10)
Zn27 Fe6 Zn32 . 20_455 124.386(9)
Zn25 Fe6 Zn32 16_665 20_455 110.438(14)
Zn25 Fe6 Zn32 20_455 20_455 60.418(12)
Zn26 Fe6 Zn32 20 20_455 172.077(14)
Zn26 Fe6 Zn32 9 20_455 69.154(11)
Zn36 Fe6 Zn32 . 20_455 61.812(11)
Zn31 Fe6 Zn32 . 20_455 56.859(9)
Zn23 Fe6 Zn32 . 20_455 115.033(12)
Zn32 Fe6 Zn32 16_665 20_455 106.51(2)
Zn33 Fe7 Zn33 12_565 23_566 63.593(10)
Zn33 Fe7 Zn33 12_565 3_665 178.41(2)
Zn33 Fe7 Zn33 23_566 3_665 116.383(10)
Zn33 Fe7 Zn33 12_565 16_665 116.383(10)
Zn33 Fe7 Zn33 23_566 16_665 178.41(2)
Zn33 Fe7 Zn33 3_665 16_665 63.593(10)
Zn33 Fe7 Zn35 12_565 7_565 63.708(11)
Zn33 Fe7 Zn35 23_566 7_565 63.708(11)
Zn33 Fe7 Zn35 3_665 7_565 117.804(15)
Zn33 Fe7 Zn35 16_665 7_565 117.804(15)
Zn33 Fe7 Zn35 12_565 3_665 117.804(15)
Zn33 Fe7 Zn35 23_566 3_665 117.804(15)
Zn33 Fe7 Zn35 3_665 3_665 63.708(11)
Zn33 Fe7 Zn35 16_665 3_665 63.708(11)
Zn35 Fe7 Zn35 7_565 3_665 64.70(2)
Zn33 Fe7 Zn30 12_565 14_556 117.146(9)
Zn33 Fe7 Zn30 23_566 14_556 63.787(6)
Zn33 Fe7 Zn30 3_665 14_556 63.787(6)
Zn33 Fe7 Zn30 16_665 14_556 117.146(9)
Zn35 Fe7 Zn30 7_565 14_556 63.761(9)
Zn35 Fe7 Zn30 3_665 14_556 63.761(9)
Zn33 Fe7 Zn30 12_565 . 63.787(6)
Zn33 Fe7 Zn30 23_566 . 117.146(9)
Zn33 Fe7 Zn30 3_665 . 117.146(9)
Zn33 Fe7 Zn30 16_665 . 63.787(6)
Zn35 Fe7 Zn30 7_565 . 63.761(9)
Zn35 Fe7 Zn30 3_665 . 63.761(9)
Zn30 Fe7 Zn30 14_556 . 116.889(19)
Zn33 Fe7 Zn37 12_565 17_665 116.033(15)
Zn33 Fe7 Zn37 23_566 17_665 116.033(15)
Zn33 Fe7 Zn37 3_665 17_665 62.454(11)
Zn33 Fe7 Zn37 16_665 17_665 62.454(11)
Zn35 Fe7 Zn37 7_565 17_665 179.679(16)
Zn35 Fe7 Zn37 3_665 17_665 115.625(14)
Zn30 Fe7 Zn37 14_556 17_665 116.338(8)
Zn30 Fe7 Zn37 . 17_665 116.338(8)
Zn33 Fe7 Zn37 12_565 1_565 62.454(10)
Zn33 Fe7 Zn37 23_566 1_565 62.454(10)
Zn33 Fe7 Zn37 3_665 1_565 116.033(15)
Zn33 Fe7 Zn37 16_665 1_565 116.033(15)
Zn35 Fe7 Zn37 7_565 1_565 115.625(14)
Zn35 Fe7 Zn37 3_665 1_565 179.679(17)
Zn30 Fe7 Zn37 14_556 1_565 116.338(7)
Zn30 Fe7 Zn37 . 1_565 116.338(7)
Zn37 Fe7 Zn37 17_665 1_565 64.05(2)
Zn33 Fe7 Zn29 12_565 14_566 116.256(9)
Zn33 Fe7 Zn29 23_566 14_566 62.814(7)
Zn33 Fe7 Zn29 3_665 14_566 62.814(7)
Zn33 Fe7 Zn29 16_665 14_566 116.256(9)
Zn35 Fe7 Zn29 7_565 14_566 116.131(8)
Zn35 Fe7 Zn29 3_665 14_566 116.131(8)
Zn30 Fe7 Zn29 14_556 14_566 62.976(10)
Zn30 Fe7 Zn29 . 14_566 179.87(2)
Zn37 Fe7 Zn29 17_665 14_566 63.770(9)
Zn37 Fe7 Zn29 1_565 14_566 63.770(9)
Zn33 Fe7 Zn29 12_565 1_565 62.814(7)
Zn33 Fe7 Zn29 23_566 1_565 116.256(9)
Zn33 Fe7 Zn29 3_665 1_565 116.256(9)
Zn33 Fe7 Zn29 16_665 1_565 62.814(7)
Zn35 Fe7 Zn29 7_565 1_565 116.131(8)
Zn35 Fe7 Zn29 3_665 1_565 116.131(8)
Zn30 Fe7 Zn29 14_556 1_565 179.87(2)
Zn30 Fe7 Zn29 . 1_565 62.976(10)
Zn37 Fe7 Zn29 17_665 1_565 63.770(9)
Zn37 Fe7 Zn29 1_565 1_565 63.770(9)
Zn29 Fe7 Zn29 14_566 1_565 117.16(2)
Fe2 Zn1 Fe2 16_665 8_655 162.777(17)
Fe2 Zn1 Zn6 16_665 . 60.579(9)
Fe2 Zn1 Zn6 8_655 . 133.232(12)
Fe2 Zn1 Zn6 16_665 13_655 133.232(12)
Fe2 Zn1 Zn6 8_655 13_655 60.579(9)
Zn6 Zn1 Zn6 . 13_655 99.382(14)
Fe2 Zn1 Zn3 16_665 13_665 61.556(10)
Fe2 Zn1 Zn3 8_655 13_665 131.804(12)
Zn6 Zn1 Zn3 . 13_665 59.307(11)
Zn6 Zn1 Zn3 13_655 13_665 71.841(12)
Fe2 Zn1 Zn3 16_665 1_545 131.804(12)
Fe2 Zn1 Zn3 8_655 1_545 61.556(10)
Zn6 Zn1 Zn3 . 1_545 71.841(12)
Zn6 Zn1 Zn3 13_655 1_545 59.307(11)
Zn3 Zn1 Zn3 13_665 1_545 101.100(14)
Fe2 Zn1 Zn8 16_665 . 57.403(8)
Fe2 Zn1 Zn8 8_655 . 116.231(9)
Zn6 Zn1 Zn8 . . 61.922(7)
Zn6 Zn1 Zn8 13_655 . 152.699(12)
Zn3 Zn1 Zn8 13_665 . 109.352(10)
Zn3 Zn1 Zn8 1_545 . 94.539(9)
Fe2 Zn1 Zn8 16_665 5 116.231(9)
Fe2 Zn1 Zn8 8_655 5 57.403(8)
Zn6 Zn1 Zn8 . 5 152.699(12)
Zn6 Zn1 Zn8 13_655 5 61.922(7)
Zn3 Zn1 Zn8 13_665 5 94.539(9)
Zn3 Zn1 Zn8 1_545 5 109.352(10)
Zn8 Zn1 Zn8 . 5 142.308(15)
Fe2 Zn1 Zn2 16_665 8_655 109.846(12)
Fe2 Zn1 Zn2 8_655 8_655 52.931(8)
Zn6 Zn1 Zn2 . 8_655 148.354(10)
Zn6 Zn1 Zn2 13_655 8_655 106.629(8)
Zn3 Zn1 Zn2 13_665 8_655 146.611(9)
Zn3 Zn1 Zn2 1_545 8_655 106.398(7)
Zn8 Zn1 Zn2 . 8_655 87.185(10)
Zn8 Zn1 Zn2 5 8_655 58.744(8)
Fe2 Zn1 Zn2 16_665 16_665 52.931(8)
Fe2 Zn1 Zn2 8_655 16_665 109.846(12)
Zn6 Zn1 Zn2 . 16_665 106.629(8)
Zn6 Zn1 Zn2 13_655 16_665 148.354(10)
Zn3 Zn1 Zn2 13_665 16_665 106.398(7)
Zn3 Zn1 Zn2 1_545 16_665 146.611(9)
Zn8 Zn1 Zn2 . 16_665 58.744(8)
Zn8 Zn1 Zn2 5 16_665 87.185(10)
Zn2 Zn1 Zn2 8_655 16_665 56.916(11)
Fe2 Zn1 Zn5 16_665 20 117.528(10)
Fe2 Zn1 Zn5 8_655 20 56.131(8)
Zn6 Zn1 Zn5 . 20 97.604(9)
Zn6 Zn1 Zn5 13_655 20 106.177(10)
Zn3 Zn1 Zn5 13_665 20 155.135(12)
Zn3 Zn1 Zn5 1_545 20 59.756(8)
Zn8 Zn1 Zn5 . 20 60.767(7)
Zn8 Zn1 Zn5 5 20 106.450(9)
Zn2 Zn1 Zn5 8_655 20 58.242(9)
Zn2 Zn1 Zn5 16_665 20 88.159(11)
Fe2 Zn1 Zn5 16_665 4 56.131(8)
Fe2 Zn1 Zn5 8_655 4 117.528(10)
Zn6 Zn1 Zn5 . 4 106.177(10)
Zn6 Zn1 Zn5 13_655 4 97.604(9)
Zn3 Zn1 Zn5 13_665 4 59.756(8)
Zn3 Zn1 Zn5 1_545 4 155.135(12)
Zn8 Zn1 Zn5 . 4 106.450(9)
Zn8 Zn1 Zn5 5 4 60.767(7)
Zn2 Zn1 Zn5 8_655 4 88.159(11)
Zn2 Zn1 Zn5 16_665 4 58.242(9)
Zn5 Zn1 Zn5 20 4 142.964(18)
Fe2 Zn2 Fe1 . 1_665 179.755(15)
Fe2 Zn2 Zn7 . 13_665 121.867(14)
Fe1 Zn2 Zn7 1_665 13_665 58.378(8)
Fe2 Zn2 Zn7 . 20_665 121.876(12)
Fe1 Zn2 Zn7 1_665 20_665 57.928(7)
Zn7 Zn2 Zn7 13_665 20_665 107.323(11)
Fe2 Zn2 Zn7 . 16_665 121.876(12)
Fe1 Zn2 Zn7 1_665 16_665 57.928(7)
Zn7 Zn2 Zn7 13_665 16_665 107.323(11)
Zn7 Zn2 Zn7 20_665 16_665 61.348(13)
Fe2 Zn2 Zn2 . 4 121.753(3)
Fe1 Zn2 Zn2 1_665 4 58.322(2)
Zn7 Zn2 Zn2 13_665 4 60.204(10)
Zn7 Zn2 Zn2 20_665 4 108.093(9)
Zn7 Zn2 Zn2 16_665 4 58.927(8)
Fe2 Zn2 Zn2 . 8_765 121.753(3)
Fe1 Zn2 Zn2 1_665 8_765 58.322(2)
Zn7 Zn2 Zn2 13_665 8_765 60.204(10)
Zn7 Zn2 Zn2 20_665 8_765 58.927(8)
Zn7 Zn2 Zn2 16_665 8_765 108.093(9)
Zn2 Zn2 Zn2 4 8_765 108.241(12)
Fe2 Zn2 Zn8 . 12_665 60.145(9)
Fe1 Zn2 Zn8 1_665 12_665 119.661(9)
Zn7 Zn2 Zn8 13_665 12_665 147.776(6)
Zn7 Zn2 Zn8 20_665 12_665 93.843(11)
Zn7 Zn2 Zn8 16_665 12_665 61.735(8)
Zn2 Zn2 Zn8 4 12_665 90.562(10)
Zn2 Zn2 Zn8 8_765 12_665 150.272(16)
Fe2 Zn2 Zn8 . 16_665 60.145(9)
Fe1 Zn2 Zn8 1_665 16_665 119.661(9)
Zn7 Zn2 Zn8 13_665 16_665 147.776(6)
Zn7 Zn2 Zn8 20_665 16_665 61.735(8)
Zn7 Zn2 Zn8 16_665 16_665 93.843(11)
Zn2 Zn2 Zn8 4 16_665 150.272(16)
Zn2 Zn2 Zn8 8_765 16_665 90.562(10)
Zn8 Zn2 Zn8 12_665 16_665 63.987(11)
Fe2 Zn2 Zn5 . 13_665 59.418(11)
Fe1 Zn2 Zn5 1_665 13_665 120.827(12)
Zn7 Zn2 Zn5 13_665 13_665 62.449(10)
Zn7 Zn2 Zn5 20_665 13_665 148.553(7)
Zn7 Zn2 Zn5 16_665 13_665 148.553(7)
Zn2 Zn2 Zn5 4 13_665 92.617(12)
Zn2 Zn2 Zn5 8_765 13_665 92.617(12)
Zn8 Zn2 Zn5 12_665 13_665 109.747(10)
Zn8 Zn2 Zn5 16_665 13_665 109.747(10)
Fe2 Zn2 Zn1 . 8_665 60.211(6)
Fe1 Zn2 Zn1 1_665 8_665 119.864(6)
Zn7 Zn2 Zn1 13_665 8_665 92.022(8)
Zn7 Zn2 Zn1 20_665 8_665 149.886(10)
Zn7 Zn2 Zn1 16_665 8_665 91.294(6)
Zn2 Zn2 Zn1 4 8_665 61.542(5)
Zn2 Zn2 Zn1 8_765 8_665 149.486(17)
Zn8 Zn2 Zn1 12_665 8_665 59.918(6)
Zn8 Zn2 Zn1 16_665 8_665 111.943(10)
Zn5 Zn2 Zn1 13_665 8_665 61.127(5)
Fe2 Zn2 Zn1 . 16_665 60.211(6)
Fe1 Zn2 Zn1 1_665 16_665 119.864(6)
Zn7 Zn2 Zn1 13_665 16_665 92.022(8)
Zn7 Zn2 Zn1 20_665 16_665 91.294(6)
Zn7 Zn2 Zn1 16_665 16_665 149.886(10)
Zn2 Zn2 Zn1 4 16_665 149.486(17)
Zn2 Zn2 Zn1 8_765 16_665 61.542(5)
Zn8 Zn2 Zn1 12_665 16_665 111.943(10)
Zn8 Zn2 Zn1 16_665 16_665 59.918(6)
Zn5 Zn2 Zn1 13_665 16_665 61.127(5)
Zn1 Zn2 Zn1 8_665 16_665 111.315(10)
Zn9 Zn3 Zn6 . 13_665 160.92(2)
Zn9 Zn3 Zn4 . 13_665 102.079(17)
Zn6 Zn3 Zn4 13_665 13_665 58.842(14)
Zn9 Zn3 Zn1 . 13_665 132.101(11)
Zn6 Zn3 Zn1 13_665 13_665 59.444(9)
Zn4 Zn3 Zn1 13_665 13_665 103.552(12)
Zn9 Zn3 Zn1 . 1_565 132.101(11)
Zn6 Zn3 Zn1 13_665 1_565 59.444(9)
Zn4 Zn3 Zn1 13_665 1_565 103.552(12)
Zn1 Zn3 Zn1 13_665 1_565 78.900(14)
Zn9 Zn3 Fe2 . 4 111.438(11)
Zn6 Zn3 Fe2 13_665 4 59.133(9)
Zn4 Zn3 Fe2 13_665 4 54.692(9)
Zn1 Zn3 Fe2 13_665 4 57.171(7)
Zn1 Zn3 Fe2 1_565 4 116.424(13)
Zn9 Zn3 Fe2 . 8_665 111.438(11)
Zn6 Zn3 Fe2 13_665 8_665 59.133(9)
Zn4 Zn3 Fe2 13_665 8_665 54.692(9)
Zn1 Zn3 Fe2 13_665 8_665 116.424(13)
Zn1 Zn3 Fe2 1_565 8_665 57.170(7)
Fe2 Zn3 Fe2 4 8_665 101.935(17)
Zn9 Zn3 Zn5 . 16_665 74.601(9)
Zn6 Zn3 Zn5 13_665 16_665 107.349(9)
Zn4 Zn3 Zn5 13_665 16_665 101.354(10)
Zn1 Zn3 Zn5 13_665 16_665 61.119(8)
Zn1 Zn3 Zn5 1_565 16_665 136.748(15)
Fe2 Zn3 Zn5 4 16_665 55.300(9)
Fe2 Zn3 Zn5 8_665 16_665 155.728(17)
Zn9 Zn3 Zn5 . 20_565 74.601(9)
Zn6 Zn3 Zn5 13_665 20_565 107.349(9)
Zn4 Zn3 Zn5 13_665 20_565 101.354(10)
Zn1 Zn3 Zn5 13_665 20_565 136.748(15)
Zn1 Zn3 Zn5 1_565 20_565 61.119(8)
Fe2 Zn3 Zn5 4 20_565 155.728(17)
Fe2 Zn3 Zn5 8_665 20_565 55.300(8)
Zn5 Zn3 Zn5 16_665 20_565 144.807(19)
Zn9 Zn3 Zn3 . 20_565 56.490(9)
Zn6 Zn3 Zn3 13_665 20_565 107.677(10)
Zn4 Zn3 Zn3 13_665 20_565 57.525(9)
Zn1 Zn3 Zn3 13_665 20_565 107.943(7)
Zn1 Zn3 Zn3 1_565 20_565 160.642(8)
Fe2 Zn3 Zn3 4 20_565 58.076(8)
Fe2 Zn3 Zn3 8_665 20_565 104.359(9)
Zn5 Zn3 Zn3 16_665 20_565 58.211(9)
Zn5 Zn3 Zn3 20_565 20_565 115.240(9)
Zn9 Zn3 Zn3 . 16_665 56.490(9)
Zn6 Zn3 Zn3 13_665 16_665 107.677(10)
Zn4 Zn3 Zn3 13_665 16_665 57.525(9)
Zn1 Zn3 Zn3 13_665 16_665 160.642(8)
Zn1 Zn3 Zn3 1_565 16_665 107.942(7)
Fe2 Zn3 Zn3 4 16_665 104.359(9)
Fe2 Zn3 Zn3 8_665 16_665 58.076(8)
Zn5 Zn3 Zn3 16_665 16_665 115.240(9)
Zn5 Zn3 Zn3 20_565 16_665 58.211(9)
Zn3 Zn3 Zn3 20_565 16_665 60.0
Fe2 Zn4 Fe2 20 16_665 116.831(9)
Fe2 Zn4 Fe2 20 . 116.831(9)
Fe2 Zn4 Fe2 16_665 . 116.831(9)
Fe2 Zn4 Zn6 20 16_665 62.639(3)
Fe2 Zn4 Zn6 16_665 16_665 178.18(3)
Fe2 Zn4 Zn6 . 16_665 62.639(3)
Fe2 Zn4 Zn6 20 . 62.639(3)
Fe2 Zn4 Zn6 16_665 . 62.639(3)
Fe2 Zn4 Zn6 . . 178.18(3)
Zn6 Zn4 Zn6 16_665 . 117.830(8)
Fe2 Zn4 Zn6 20 20 178.18(3)
Fe2 Zn4 Zn6 16_665 20 62.639(3)
Fe2 Zn4 Zn6 . 20 62.639(3)
Zn6 Zn4 Zn6 16_665 20 117.830(8)
Zn6 Zn4 Zn6 . 20 117.830(8)
Fe2 Zn4 Zn3 20 13_665 63.499(11)
Fe2 Zn4 Zn3 16_665 13_665 63.499(11)
Fe2 Zn4 Zn3 . 13_665 117.94(2)
Zn6 Zn4 Zn3 16_665 13_665 115.037(15)
Zn6 Zn4 Zn3 . 13_665 60.234(12)
Zn6 Zn4 Zn3 20 13_665 115.037(15)
Fe2 Zn4 Zn3 20 4 63.499(11)
Fe2 Zn4 Zn3 16_665 4 117.94(2)
Fe2 Zn4 Zn3 . 4 63.499(11)
Zn6 Zn4 Zn3 16_665 4 60.234(12)
Zn6 Zn4 Zn3 . 4 115.037(15)
Zn6 Zn4 Zn3 20 4 115.037(15)
Zn3 Zn4 Zn3 13_665 4 64.950(18)
Fe2 Zn4 Zn3 20 8_655 117.94(2)
Fe2 Zn4 Zn3 16_665 8_655 63.499(11)
Fe2 Zn4 Zn3 . 8_655 63.499(11)
Zn6 Zn4 Zn3 16_665 8_655 115.037(15)
Zn6 Zn4 Zn3 . 8_655 115.037(15)
Zn6 Zn4 Zn3 20 8_655 60.234(12)
Zn3 Zn4 Zn3 13_665 8_655 64.950(18)
Zn3 Zn4 Zn3 4 8_655 64.950(18)
Fe2 Zn4 Zn10 20 20 59.628(12)
Fe2 Zn4 Zn10 16_665 20 117.222(15)
Fe2 Zn4 Zn10 . 20 117.222(15)
Zn6 Zn4 Zn10 16_665 20 64.192(10)
Zn6 Zn4 Zn10 . 20 64.192(10)
Zn6 Zn4 Zn10 20 20 122.20(2)
Zn3 Zn4 Zn10 13_665 20 113.085(8)
Zn3 Zn4 Zn10 4 20 113.085(8)
Zn3 Zn4 Zn10 8_655 20 177.57(2)
Fe2 Zn4 Zn10 20 . 117.222(15)
Fe2 Zn4 Zn10 16_665 . 117.222(15)
Fe2 Zn4 Zn10 . . 59.628(12)
Zn6 Zn4 Zn10 16_665 . 64.192(10)
Zn6 Zn4 Zn10 . . 122.20(2)
Zn6 Zn4 Zn10 20 . 64.192(10)
Zn3 Zn4 Zn10 13_665 . 177.57(2)
Zn3 Zn4 Zn10 4 . 113.085(8)
Zn3 Zn4 Zn10 8_655 . 113.085(8)
Zn10 Zn4 Zn10 20 . 68.840(18)
Fe2 Zn4 Zn10 20 16_665 117.222(15)
Fe2 Zn4 Zn10 16_665 16_665 59.628(12)
Fe2 Zn4 Zn10 . 16_665 117.222(15)
Zn6 Zn4 Zn10 16_665 16_665 122.20(2)
Zn6 Zn4 Zn10 . 16_665 64.192(10)
Zn6 Zn4 Zn10 20 16_665 64.192(10)
Zn3 Zn4 Zn10 13_665 16_665 113.085(9)
Zn3 Zn4 Zn10 4 16_665 177.57(2)
Zn3 Zn4 Zn10 8_655 16_665 113.085(8)
Zn10 Zn4 Zn10 20 16_665 68.840(18)
Zn10 Zn4 Zn10 . 16_665 68.840(18)
Fe2 Zn5 Zn11 13_665 17 135.122(12)
Fe2 Zn5 Zn11 13_665 . 135.122(12)
Zn11 Zn5 Zn11 17 . 60.285(13)
Fe2 Zn5 Fe3 13_665 . 163.912(16)
Zn11 Zn5 Fe3 17 . 57.078(9)
Zn11 Zn5 Fe3 . . 57.078(9)
Fe2 Zn5 Zn2 13_665 13_665 54.431(10)
Zn11 Zn5 Zn2 17 13_665 144.626(9)
Zn11 Zn5 Zn2 . 13_665 144.626(9)
Fe3 Zn5 Zn2 . 13_665 109.481(14)
Fe2 Zn5 Zn7 13_665 . 111.168(14)
Zn11 Zn5 Zn7 17 . 101.909(11)
Zn11 Zn5 Zn7 . . 101.909(11)
Fe3 Zn5 Zn7 . . 52.744(10)
Zn2 Zn5 Zn7 13_665 . 56.737(10)
Fe2 Zn5 Zn3 13_665 16_665 62.142(11)
Zn11 Zn5 Zn3 17 16_665 104.105(14)
Zn11 Zn5 Zn3 . 16_665 73.419(12)
Fe3 Zn5 Zn3 . 16_665 130.221(13)
Zn2 Zn5 Zn3 13_665 16_665 107.803(12)
Zn7 Zn5 Zn3 . 16_665 146.187(9)
Fe2 Zn5 Zn3 13_665 20_565 62.142(11)
Zn11 Zn5 Zn3 17 20_565 73.419(12)
Zn11 Zn5 Zn3 . 20_565 104.105(14)
Fe3 Zn5 Zn3 . 20_565 130.221(13)
Zn2 Zn5 Zn3 13_665 20_565 107.803(12)
Zn7 Zn5 Zn3 . 20_565 146.187(9)
Zn3 Zn5 Zn3 16_665 20_565 63.578(18)
Fe2 Zn5 Zn1 13_665 20 58.572(6)
Zn11 Zn5 Zn1 17 20 94.066(7)
Zn11 Zn5 Zn1 . 20 153.656(12)
Fe3 Zn5 Zn1 . 20 115.928(8)
Zn2 Zn5 Zn1 13_665 20 60.630(8)
Zn7 Zn5 Zn1 . 20 88.495(10)
Zn3 Zn5 Zn1 16_665 20 110.645(13)
Zn3 Zn5 Zn1 20_565 20 59.126(10)
Fe2 Zn5 Zn1 13_665 4 58.572(6)
Zn11 Zn5 Zn1 17 4 153.656(12)
Zn11 Zn5 Zn1 . 4 94.066(7)
Fe3 Zn5 Zn1 . 4 115.928(8)
Zn2 Zn5 Zn1 13_665 4 60.630(8)
Zn7 Zn5 Zn1 . 4 88.495(10)
Zn3 Zn5 Zn1 16_665 4 59.126(10)
Zn3 Zn5 Zn1 20_565 4 110.645(13)
Zn1 Zn5 Zn1 20 4 110.511(12)
Fe2 Zn5 Zn8 13_665 20 116.598(9)
Zn11 Zn5 Zn8 17 20 57.479(8)
Zn11 Zn5 Zn8 . 20 106.065(12)
Fe3 Zn5 Zn8 . 20 57.680(7)
Zn2 Zn5 Zn8 13_665 20 87.355(9)
Zn7 Zn5 Zn8 . 20 59.126(7)
Zn3 Zn5 Zn8 16_665 20 154.686(13)
Zn3 Zn5 Zn8 20_565 20 92.847(10)
Zn1 Zn5 Zn8 20 20 58.699(5)
Zn1 Zn5 Zn8 4 20 144.392(15)
Fe2 Zn5 Zn8 13_665 9 116.598(9)
Zn11 Zn5 Zn8 17 9 106.065(12)
Zn11 Zn5 Zn8 . 9 57.479(8)
Fe3 Zn5 Zn8 . 9 57.680(7)
Zn2 Zn5 Zn8 13_665 9 87.355(9)
Zn7 Zn5 Zn8 . 9 59.126(7)
Zn3 Zn5 Zn8 16_665 9 92.847(10)
Zn3 Zn5 Zn8 20_565 9 154.686(13)
Zn1 Zn5 Zn8 20 9 144.392(15)
Zn1 Zn5 Zn8 4 9 58.699(5)
Zn8 Zn5 Zn8 20 9 108.358(13)
Zn13 Zn6 Zn4 . . 102.47(2)
Zn13 Zn6 Fe2 . 16_665 110.468(12)
Zn4 Zn6 Fe2 . 16_665 56.050(9)
Zn13 Zn6 Fe2 . 20 110.468(12)
Zn4 Zn6 Fe2 . 20 56.050(9)
Fe2 Zn6 Fe2 16_665 20 105.434(17)
Zn13 Zn6 Zn3 . 13_665 163.396(19)
Zn4 Zn6 Zn3 . 13_665 60.924(17)
Fe2 Zn6 Zn3 16_665 13_665 61.547(10)
Fe2 Zn6 Zn3 20 13_665 61.547(10)
Zn13 Zn6 Zn1 . . 129.053(11)
Zn4 Zn6 Zn1 . . 106.464(14)
Fe2 Zn6 Zn1 16_665 . 58.498(7)
Fe2 Zn6 Zn1 20 . 120.457(15)
Zn3 Zn6 Zn1 13_665 . 61.249(10)
Zn13 Zn6 Zn1 . 13_655 129.053(11)
Zn4 Zn6 Zn1 . 13_655 106.464(14)
Fe2 Zn6 Zn1 16_665 13_655 120.457(15)
Fe2 Zn6 Zn1 20 13_655 58.498(7)
Zn3 Zn6 Zn1 13_665 13_655 61.249(10)
Zn1 Zn6 Zn1 . 13_655 80.618(14)
Zn13 Zn6 Zn8 . . 73.024(9)
Zn4 Zn6 Zn8 . . 103.753(9)
Fe2 Zn6 Zn8 16_665 . 56.154(7)
Fe2 Zn6 Zn8 20 . 159.742(15)
Zn3 Zn6 Zn8 13_665 . 109.325(8)
Zn1 Zn6 Zn8 . . 59.953(7)
Zn1 Zn6 Zn8 13_655 . 135.634(14)
Zn13 Zn6 Zn8 . 17_655 73.024(9)
Zn4 Zn6 Zn8 . 17_655 103.753(9)
Fe2 Zn6 Zn8 16_665 17_655 159.742(15)
Fe2 Zn6 Zn8 20 17_655 56.154(7)
Zn3 Zn6 Zn8 13_665 17_655 109.325(8)
Zn1 Zn6 Zn8 . 17_655 135.634(14)
Zn1 Zn6 Zn8 13_655 17_655 59.953(7)
Zn8 Zn6 Zn8 . 17_655 139.951(16)
Zn13 Zn6 Zn10 . 20 56.725(11)
Zn4 Zn6 Zn10 . 20 59.851(15)
Fe2 Zn6 Zn10 16_665 20 108.023(15)
Fe2 Zn6 Zn10 20 20 56.317(10)
Zn3 Zn6 Zn10 13_665 20 110.128(14)
Zn1 Zn6 Zn10 . 20 165.939(16)
Zn1 Zn6 Zn10 13_655 20 105.520(9)
Zn8 Zn6 Zn10 . 20 117.624(14)
Zn8 Zn6 Zn10 17_655 20 56.181(10)
Zn13 Zn6 Zn10 . 16_665 56.725(11)
Zn4 Zn6 Zn10 . 16_665 59.851(15)
Fe2 Zn6 Zn10 16_665 16_665 56.317(10)
Fe2 Zn6 Zn10 20 16_665 108.023(15)
Zn3 Zn6 Zn10 13_665 16_665 110.128(14)
Zn1 Zn6 Zn10 . 16_665 105.520(9)
Zn1 Zn6 Zn10 13_655 16_665 165.939(16)
Zn8 Zn6 Zn10 . 16_665 56.181(10)
Zn8 Zn6 Zn10 17_655 16_665 117.624(14)
Zn10 Zn6 Zn10 20 16_665 65.769(17)
Fe3 Zn7 Fe1 . . 178.070(14)
Fe3 Zn7 Zn2 . 13_665 122.627(13)
Fe1 Zn7 Zn2 . 13_665 59.303(8)
Fe3 Zn7 Zn2 . 20_455 121.729(8)
Fe1 Zn7 Zn2 . 20_455 58.837(7)
Zn2 Zn7 Zn2 13_665 20_455 60.870(7)
Fe3 Zn7 Zn2 . 16_665 121.729(8)
Fe1 Zn7 Zn2 . 16_665 58.837(7)
Zn2 Zn7 Zn2 13_665 16_665 60.870(7)
Zn2 Zn7 Zn2 20_455 16_665 109.291(14)
Fe3 Zn7 Zn12 . 16_665 61.250(8)
Fe1 Zn7 Zn12 . 16_665 117.199(9)
Zn2 Zn7 Zn12 13_665 16_665 148.285(8)
Zn2 Zn7 Zn12 20_455 16_665 148.278(12)
Zn2 Zn7 Zn12 16_665 16_665 89.668(9)
Fe3 Zn7 Zn12 . 20_455 61.250(8)
Fe1 Zn7 Zn12 . 20_455 117.199(9)
Zn2 Zn7 Zn12 13_665 20_455 148.285(8)
Zn2 Zn7 Zn12 20_455 20_455 89.668(9)
Zn2 Zn7 Zn12 16_665 20_455 148.278(12)
Zn12 Zn7 Zn12 16_665 20_455 63.339(15)
Fe3 Zn7 Zn7 . 16 120.954(7)
Fe1 Zn7 Zn7 . 16 57.484(5)
Zn2 Zn7 Zn7 13_665 16 108.027(7)
Zn2 Zn7 Zn7 20_455 16 59.326(6)
Zn2 Zn7 Zn7 16_665 16 107.784(7)
Zn12 Zn7 Zn7 16_665 16 91.187(7)
Zn12 Zn7 Zn7 20_455 16 59.714(6)
Fe3 Zn7 Zn7 . 20 120.954(7)
Fe1 Zn7 Zn7 . 20 57.484(5)
Zn2 Zn7 Zn7 13_665 20 108.027(7)
Zn2 Zn7 Zn7 20_455 20 107.784(7)
Zn2 Zn7 Zn7 16_665 20 59.326(6)
Zn12 Zn7 Zn7 16_665 20 59.714(6)
Zn12 Zn7 Zn7 20_455 20 91.187(7)
Zn7 Zn7 Zn7 16 20 60.0
Fe3 Zn7 Zn8 . 9 61.281(7)
Fe1 Zn7 Zn8 . 9 119.336(7)
Zn2 Zn7 Zn8 13_665 9 90.947(9)
Zn2 Zn7 Zn8 20_455 9 60.502(7)
Zn2 Zn7 Zn8 16_665 9 149.181(13)
Zn12 Zn7 Zn8 16_665 9 113.953(11)
Zn12 Zn7 Zn8 20_455 9 62.367(9)
Zn7 Zn7 Zn8 16 9 91.928(6)
Zn7 Zn7 Zn8 20 9 149.541(7)
Fe3 Zn7 Zn8 . 20 61.281(7)
Fe1 Zn7 Zn8 . 20 119.336(7)
Zn2 Zn7 Zn8 13_665 20 90.947(9)
Zn2 Zn7 Zn8 20_455 20 149.181(13)
Zn2 Zn7 Zn8 16_665 20 60.502(7)
Zn12 Zn7 Zn8 16_665 20 62.367(9)
Zn12 Zn7 Zn8 20_455 20 113.953(11)
Zn7 Zn7 Zn8 16 20 149.541(7)
Zn7 Zn7 Zn8 20 20 91.928(6)
Zn8 Zn7 Zn8 9 20 111.859(12)
Fe3 Zn7 Zn5 . . 61.813(11)
Fe1 Zn7 Zn5 . . 120.117(12)
Zn2 Zn7 Zn5 13_665 . 60.814(10)
Zn2 Zn7 Zn5 20_455 . 92.046(8)
Zn2 Zn7 Zn5 16_665 . 92.046(8)
Zn12 Zn7 Zn5 16_665 . 113.059(10)
Zn12 Zn7 Zn5 20_455 . 113.059(10)
Zn7 Zn7 Zn5 16 . 148.989(2)
Zn7 Zn7 Zn5 20 . 148.989(2)
Zn8 Zn7 Zn5 9 . 61.261(7)
Zn8 Zn7 Zn5 20 . 61.261(7)
Fe2 Zn8 Zn11 16_665 12 135.687(11)
Fe2 Zn8 Fe3 16_665 20 164.904(13)
Zn11 Zn8 Fe3 12 20 57.696(9)
Fe2 Zn8 Zn10 16_665 16_665 60.048(11)
Zn11 Zn8 Zn10 12 16_665 104.691(10)
Fe3 Zn8 Zn10 20 16_665 128.960(14)
Fe2 Zn8 Zn14 16_665 . 129.781(12)
Zn11 Zn8 Zn14 12 . 62.544(10)
Fe3 Zn8 Zn14 20 . 59.033(9)
Zn10 Zn8 Zn14 16_665 . 70.291(12)
Fe2 Zn8 Zn2 16_665 16_665 54.225(9)
Zn11 Zn8 Zn2 12 16_665 147.533(11)
Fe3 Zn8 Zn2 20 16_665 110.902(11)
Zn10 Zn8 Zn2 16_665 16_665 104.841(10)
Zn14 Zn8 Zn2 . 16_665 142.080(12)
Fe2 Zn8 Zn7 16_665 20 111.985(11)
Zn11 Zn8 Zn7 12 20 102.890(10)
Fe3 Zn8 Zn7 20 20 53.182(8)
Zn10 Zn8 Zn7 16_665 20 143.858(12)
Zn14 Zn8 Zn7 . 20 103.212(10)
Zn2 Zn8 Zn7 16_665 20 57.764(8)
Fe2 Zn8 Zn1 16_665 . 59.004(7)
Zn11 Zn8 Zn1 12 . 95.823(10)
Fe3 Zn8 Zn1 20 . 118.735(10)
Zn10 Zn8 Zn1 16_665 . 109.947(12)
Zn14 Zn8 Zn1 . . 156.545(12)
Zn2 Zn8 Zn1 16_665 . 61.338(8)
Zn7 Zn8 Zn1 20 . 89.846(10)
Fe2 Zn8 Zn6 16_665 . 59.690(9)
Zn11 Zn8 Zn6 12 . 76.146(11)
Fe3 Zn8 Zn6 20 . 133.650(13)
Zn10 Zn8 Zn6 16_665 . 63.464(12)
Zn14 Zn8 Zn6 . . 104.976(12)
Zn2 Zn8 Zn6 16_665 . 105.706(11)
Zn7 Zn8 Zn6 20 . 147.224(13)
Zn1 Zn8 Zn6 . . 58.125(10)
Fe2 Zn8 Zn12 16_665 16_665 114.771(10)
Zn11 Zn8 Zn12 12 16_665 106.667(10)
Fe3 Zn8 Zn12 20 16_665 56.863(8)
Zn10 Zn8 Zn12 16_665 16_665 92.230(12)
Zn14 Zn8 Zn12 . 16_665 58.017(9)
Zn2 Zn8 Zn12 16_665 16_665 85.342(10)
Zn7 Zn8 Zn12 20 16_665 57.448(9)
Zn1 Zn8 Zn12 . 16_665 143.300(12)
Zn6 Zn8 Zn12 . 16_665 154.980(13)
Fe2 Zn8 Zn5 16_665 20 118.879(11)
Zn11 Zn8 Zn5 12 20 58.288(9)
Fe3 Zn8 Zn5 20 20 58.678(9)
Zn10 Zn8 Zn5 16_665 20 156.527(12)
Zn14 Zn8 Zn5 . 20 109.444(11)
Zn2 Zn8 Zn5 16_665 20 89.465(10)
Zn7 Zn8 Zn5 20 20 59.613(9)
Zn1 Zn8 Zn5 . 20 60.534(7)
Zn6 Zn8 Zn5 . 20 95.051(11)
Zn12 Zn8 Zn5 16_665 20 107.648(10)
Fe2 Zn8 Zn8 16_665 20 56.189(6)
Zn11 Zn8 Zn8 12 20 153.612(8)
Fe3 Zn8 Zn8 20 20 115.760(7)
Zn10 Zn8 Zn8 16_665 20 57.507(6)
Zn14 Zn8 Zn8 . 20 91.759(8)
Zn2 Zn8 Zn8 16_665 20 58.007(6)
Zn7 Zn8 Zn8 20 20 88.072(6)
Zn1 Zn8 Zn8 . 20 108.292(5)
Zn6 Zn8 Zn8 . 20 107.332(8)
Zn12 Zn8 Zn8 16_665 20 59.152(6)
Zn5 Zn8 Zn8 20 20 144.122(8)
Zn3 Zn9 Zn3 16_665 . 67.020(19)
Zn3 Zn9 Zn3 16_665 20_565 67.020(19)
Zn3 Zn9 Zn3 . 20_565 67.020(19)
Zn3 Zn9 Zn15 16_665 . 140.395(12)
Zn3 Zn9 Zn15 . . 140.395(12)
Zn3 Zn9 Zn15 20_565 . 140.395(12)
Zn3 Zn9 Zn11 16_665 20_565 74.478(11)
Zn3 Zn9 Zn11 . 20_565 105.918(9)
Zn3 Zn9 Zn11 20_565 20_565 140.511(16)
Zn15 Zn9 Zn11 . 20_565 70.320(12)
Zn3 Zn9 Zn11 16_665 12_565 105.918(9)
Zn3 Zn9 Zn11 . 12_565 74.478(11)
Zn3 Zn9 Zn11 20_565 12_565 140.511(16)
Zn15 Zn9 Zn11 . 12_565 70.320(12)
Zn11 Zn9 Zn11 20_565 12_565 58.780(11)
Zn3 Zn9 Zn11 16_665 16_665 140.511(16)
Zn3 Zn9 Zn11 . 16_665 74.478(11)
Zn3 Zn9 Zn11 20_565 16_665 105.919(9)
Zn15 Zn9 Zn11 . 16_665 70.319(12)
Zn11 Zn9 Zn11 20_565 16_665 109.261(13)
Zn11 Zn9 Zn11 12_565 16_665 53.557(10)
Zn3 Zn9 Zn11 16_665 . 74.478(11)
Zn3 Zn9 Zn11 . . 140.511(16)
Zn3 Zn9 Zn11 20_565 . 105.918(9)
Zn15 Zn9 Zn11 . . 70.320(13)
Zn11 Zn9 Zn11 20_565 . 53.557(10)
Zn11 Zn9 Zn11 12_565 . 109.261(13)
Zn11 Zn9 Zn11 16_665 . 140.54(2)
Zn3 Zn9 Zn11 16_665 9_665 140.511(16)
Zn3 Zn9 Zn11 . 9_665 105.918(9)
Zn3 Zn9 Zn11 20_565 9_665 74.478(11)
Zn15 Zn9 Zn11 . 9_665 70.319(12)
Zn11 Zn9 Zn11 20_565 9_665 140.54(2)
Zn11 Zn9 Zn11 12_565 9_665 109.261(13)
Zn11 Zn9 Zn11 16_665 9_665 58.780(11)
Zn11 Zn9 Zn11 . 9_665 109.261(13)
Zn3 Zn9 Zn11 16_665 17 105.918(9)
Zn3 Zn9 Zn11 . 17 140.511(16)
Zn3 Zn9 Zn11 20_565 17 74.478(11)
Zn15 Zn9 Zn11 . 17 70.320(12)
Zn11 Zn9 Zn11 20_565 17 109.261(13)
Zn11 Zn9 Zn11 12_565 17 140.54(2)
Zn11 Zn9 Zn11 16_665 17 109.261(13)
Zn11 Zn9 Zn11 . 17 58.780(11)
Zn11 Zn9 Zn11 9_665 17 53.557(10)
Zn38 Zn10 Fe2 . . 154.73(3)
Zn38 Zn10 Zn13 . 20 68.097(11)
Fe2 Zn10 Zn13 . 20 112.629(11)
Zn38 Zn10 Zn13 . 16_665 68.097(11)
Fe2 Zn10 Zn13 . 16_665 112.629(11)
Zn13 Zn10 Zn13 20 16_665 134.19(2)
Zn38 Zn10 Zn8 . 12_665 139.236(18)
Fe2 Zn10 Zn8 . 12_665 58.231(10)
Zn13 Zn10 Zn8 20 12_665 75.313(9)
Zn13 Zn10 Zn8 16_665 12_665 137.404(15)
Zn38 Zn10 Zn8 . 16_665 139.236(18)
Fe2 Zn10 Zn8 . 16_665 58.231(10)
Zn13 Zn10 Zn8 20 16_665 137.404(15)
Zn13 Zn10 Zn8 16_665 16_665 75.313(9)
Zn8 Zn10 Zn8 12_665 16_665 64.987(13)
Zn38 Zn10 Zn38 . 16_665 7.17(3)
Fe2 Zn10 Zn38 . 16_665 148.72(2)
Zn13 Zn10 Zn38 20 16_665 64.65(2)
Zn13 Zn10 Zn38 16_665 16_665 73.14(2)
Zn8 Zn10 Zn38 12_665 16_665 138.439(17)
Zn8 Zn10 Zn38 16_665 16_665 145.97(2)
Zn38 Zn10 Zn38 . 20 7.17(3)
Fe2 Zn10 Zn38 . 20 148.72(2)
Zn13 Zn10 Zn38 20 20 73.14(2)
Zn13 Zn10 Zn38 16_665 20 64.65(2)
Zn8 Zn10 Zn38 12_665 20 145.97(2)
Zn8 Zn10 Zn38 16_665 20 138.439(18)
Zn38 Zn10 Zn38 16_665 20 8.60(4)
Zn38 Zn10 Zn4 . . 99.46(3)
Fe2 Zn10 Zn4 . . 55.275(13)
Zn13 Zn10 Zn4 20 . 99.839(12)
Zn13 Zn10 Zn4 16_665 . 99.839(12)
Zn8 Zn10 Zn4 12_665 . 103.985(14)
Zn8 Zn10 Zn4 16_665 . 103.985(14)
Zn38 Zn10 Zn4 16_665 . 93.71(2)
Zn38 Zn10 Zn4 20 . 93.71(2)
Zn38 Zn10 Zn6 . 20 110.119(17)
Fe2 Zn10 Zn6 . 20 58.071(9)
Zn13 Zn10 Zn6 20 20 57.242(11)
Zn13 Zn10 Zn6 16_665 20 155.658(19)
Zn8 Zn10 Zn6 12_665 20 60.356(8)
Zn8 Zn10 Zn6 16_665 20 110.628(14)
Zn38 Zn10 Zn6 16_665 20 103.37(2)
Zn38 Zn10 Zn6 20 20 110.455(17)
Zn4 Zn10 Zn6 . 20 55.958(10)
Zn38 Zn10 Zn6 . 16_665 110.119(17)
Fe2 Zn10 Zn6 . 16_665 58.071(9)
Zn13 Zn10 Zn6 20 16_665 155.658(19)
Zn13 Zn10 Zn6 16_665 16_665 57.242(11)
Zn8 Zn10 Zn6 12_665 16_665 110.628(14)
Zn8 Zn10 Zn6 16_665 16_665 60.356(8)
Zn38 Zn10 Zn6 16_665 16_665 110.455(17)
Zn38 Zn10 Zn6 20 16_665 103.37(2)
Zn4 Zn10 Zn6 . 16_665 55.958(10)
Zn6 Zn10 Zn6 20 16_665 104.05(2)
Zn38 Zn10 Zn14 . 12_665 88.95(2)
Fe2 Zn10 Zn14 . 12_665 112.834(13)
Zn13 Zn10 Zn14 20 12_665 56.140(9)
Zn13 Zn10 Zn14 16_665 12_665 110.494(16)
Zn8 Zn10 Zn14 12_665 12_665 55.000(9)
Zn8 Zn10 Zn14 16_665 12_665 87.451(13)
Zn38 Zn10 Zn14 16_665 12_665 91.813(16)
Zn38 Zn10 Zn14 20 12_665 96.05(2)
Zn4 Zn10 Zn14 . 12_665 149.466(8)
Zn6 Zn10 Zn14 20 12_665 93.560(10)
Zn6 Zn10 Zn14 16_665 12_665 146.980(14)
Zn11 Zn11 Fe3 20_565 . 174.872(9)
Zn11 Zn11 Zn8 20_565 9 122.439(7)
Fe3 Zn11 Zn8 . 9 61.531(8)
Zn11 Zn11 Zn5 20_565 . 122.160(8)
Fe3 Zn11 Zn5 . . 61.947(10)
Zn8 Zn11 Zn5 9 . 64.234(9)
Zn11 Zn11 Zn11 20_565 17 120.0
Fe3 Zn11 Zn11 . 17 58.460(6)
Zn8 Zn11 Zn11 9 17 111.064(7)
Zn5 Zn11 Zn11 . 17 59.857(7)
Zn11 Zn11 Zn13 20_565 16_565 62.940(6)
Fe3 Zn11 Zn13 . 16_565 117.047(10)
Zn8 Zn11 Zn13 9 16_565 75.330(10)
Zn5 Zn11 Zn13 . 16_565 133.695(14)
Zn11 Zn11 Zn13 17 16_565 164.153(10)
Zn11 Zn11 Zn16 20_565 . 117.727(8)
Fe3 Zn11 Zn16 . . 57.146(11)
Zn8 Zn11 Zn16 9 . 109.269(12)
Zn5 Zn11 Zn16 . . 109.642(10)
Zn11 Zn11 Zn16 17 . 60.304(7)
Zn13 Zn11 Zn16 16_565 . 104.083(13)
Zn11 Zn11 Zn9 20_565 . 63.221(5)
Fe3 Zn11 Zn9 . . 116.953(10)
Zn8 Zn11 Zn9 9 . 134.042(16)
Zn5 Zn11 Zn9 . . 75.201(13)
Zn11 Zn11 Zn9 17 . 60.610(5)
Zn13 Zn11 Zn9 16_565 . 125.994(9)
Zn16 Zn11 Zn9 . . 103.815(15)
Zn11 Zn11 Zn14 20_565 9 119.038(7)
Fe3 Zn11 Zn14 . 9 59.237(8)
Zn8 Zn11 Zn14 9 9 59.782(9)
Zn5 Zn11 Zn14 . 9 111.977(11)
Zn11 Zn11 Zn14 17 9 109.742(8)
Zn13 Zn11 Zn14 16_565 9 59.997(9)
Zn16 Zn11 Zn14 . 9 60.708(11)
Zn9 Zn11 Zn14 . 9 164.138(17)
Zn11 Zn11 Zn18 20_565 16_665 64.844(6)
Fe3 Zn11 Zn18 . 16_665 110.540(12)
Zn8 Zn11 Zn18 9 16_665 122.129(12)
Zn5 Zn11 Zn18 . 16_665 167.814(13)
Zn11 Zn11 Zn18 17 16_665 108.268(8)
Zn13 Zn11 Zn18 16_565 16_665 57.599(11)
Zn16 Zn11 Zn18 . 16_665 59.118(9)
Zn9 Zn11 Zn18 . 16_665 101.954(14)
Zn14 Zn11 Zn18 9 16_665 67.934(10)
Zn11 Zn11 Zn15 20_565 . 66.655(5)
Fe3 Zn11 Zn15 . . 109.039(11)
Zn8 Zn11 Zn15 9 . 169.108(14)
Zn5 Zn11 Zn15 . . 117.517(12)
Zn11 Zn11 Zn15 17 . 64.429(5)
Zn13 Zn11 Zn15 16_565 . 106.521(12)
Zn16 Zn11 Zn15 . . 59.842(13)
Zn9 Zn11 Zn15 . . 53.773(15)
Zn14 Zn11 Zn15 9 . 111.413(15)
Zn18 Zn11 Zn15 16_665 . 54.066(12)
Fe3 Zn12 Fe3 16_665 20_665 169.555(17)
Fe3 Zn12 Zn14 16_665 12_665 59.876(8)
Fe3 Zn12 Zn14 20_665 12_665 129.388(13)
Fe3 Zn12 Zn14 16_665 16_665 129.388(13)
Fe3 Zn12 Zn14 20_665 16_665 59.876(8)
Zn14 Zn12 Zn14 12_665 16_665 69.582(15)
Fe3 Zn12 Zn7 16_665 16_665 54.576(8)
Fe3 Zn12 Zn7 20_665 16_665 115.139(13)
Zn14 Zn12 Zn7 12_665 16_665 105.972(10)
Zn14 Zn12 Zn7 16_665 16_665 148.284(15)
Fe3 Zn12 Zn7 16_665 20_665 115.139(13)
Fe3 Zn12 Zn7 20_665 20_665 54.576(8)
Zn14 Zn12 Zn7 12_665 20_665 148.284(15)
Zn14 Zn12 Zn7 16_665 20_665 105.972(10)
Zn7 Zn12 Zn7 16_665 20_665 60.571(12)
Fe3 Zn12 Zn17 16_665 16_665 57.619(10)
Fe3 Zn12 Zn17 20_665 16_665 129.078(15)
Zn14 Zn12 Zn17 12_665 16_665 61.397(11)
Zn14 Zn12 Zn17 16_665 16_665 100.912(13)
Zn7 Zn12 Zn17 16_665 16_665 103.957(9)
Zn7 Zn12 Zn17 20_665 16_665 146.267(15)
Fe3 Zn12 Zn17 16_665 20_665 129.078(15)
Fe3 Zn12 Zn17 20_665 20_665 57.619(10)
Zn14 Zn12 Zn17 12_665 20_665 100.912(13)
Zn14 Zn12 Zn17 16_665 20_665 61.397(11)
Zn7 Zn12 Zn17 16_665 20_665 146.267(15)
Zn7 Zn12 Zn17 20_665 20_665 103.957(9)
Zn17 Zn12 Zn17 16_665 20_665 71.662(18)
Fe3 Zn12 Zn12 16_665 20_565 57.382(8)
Fe3 Zn12 Zn12 20_665 20_565 117.182(8)
Zn14 Zn12 Zn12 12_665 20_565 108.871(8)
Zn14 Zn12 Zn12 16_665 20_565 153.383(9)
Zn7 Zn12 Zn12 16_665 20_565 58.330(7)
Zn7 Zn12 Zn12 20_665 20_565 88.813(7)
Zn17 Zn12 Zn12 16_665 20_565 58.903(8)
Zn17 Zn12 Zn12 20_665 20_565 93.951(10)
Fe3 Zn12 Zn12 16_665 16_775 117.182(8)
Fe3 Zn12 Zn12 20_665 16_775 57.382(8)
Zn14 Zn12 Zn12 12_665 16_775 153.383(9)
Zn14 Zn12 Zn12 16_665 16_775 108.871(8)
Zn7 Zn12 Zn12 16_665 16_775 88.813(7)
Zn7 Zn12 Zn12 20_665 16_775 58.330(8)
Zn17 Zn12 Zn12 16_665 16_775 93.951(10)
Zn17 Zn12 Zn12 20_665 16_775 58.903(8)
Zn12 Zn12 Zn12 20_565 16_775 60.0
Fe3 Zn12 Zn8 16_665 12_665 58.500(7)
Fe3 Zn12 Zn8 20_665 12_665 119.917(13)
Zn14 Zn12 Zn8 12_665 12_665 58.771(9)
Zn14 Zn12 Zn8 16_665 12_665 93.824(12)
Zn7 Zn12 Zn8 16_665 12_665 60.185(8)
Zn7 Zn12 Zn8 20_665 12_665 91.145(12)
Zn17 Zn12 Zn8 16_665 12_665 107.155(11)
Zn17 Zn12 Zn8 20_665 12_665 153.547(14)
Zn12 Zn12 Zn8 20_565 12_665 108.163(6)
Zn12 Zn12 Zn8 16_775 12_665 145.536(8)
Fe3 Zn12 Zn8 16_665 16_665 119.917(13)
Fe3 Zn12 Zn8 20_665 16_665 58.499(7)
Zn14 Zn12 Zn8 12_665 16_665 93.824(12)
Zn14 Zn12 Zn8 16_665 16_665 58.771(9)
Zn7 Zn12 Zn8 16_665 16_665 91.145(12)
Zn7 Zn12 Zn8 20_665 16_665 60.185(8)
Zn17 Zn12 Zn8 16_665 16_665 153.547(14)
Zn17 Zn12 Zn8 20_665 16_665 107.155(11)
Zn12 Zn12 Zn8 20_565 16_665 145.536(8)
Zn12 Zn12 Zn8 16_775 16_665 108.163(6)
Zn8 Zn12 Zn8 12_665 16_665 61.695(11)
Zn40 Zn13 Zn40 17_655 . 15.28(4)
Zn40 Zn13 Zn10 17_655 20 96.53(2)
Zn40 Zn13 Zn10 . 20 105.75(2)
Zn40 Zn13 Zn10 17_655 16_665 105.75(2)
Zn40 Zn13 Zn10 . 16_665 96.53(2)
Zn10 Zn13 Zn10 20 16_665 72.80(2)
Zn40 Zn13 Zn6 17_655 . 162.00(2)
Zn40 Zn13 Zn6 . . 162.00(2)
Zn10 Zn13 Zn6 20 . 66.034(13)
Zn10 Zn13 Zn6 16_665 . 66.034(13)
Zn40 Zn13 Zn18 17_655 1_545 59.12(2)
Zn40 Zn13 Zn18 . 1_545 59.12(2)
Zn10 Zn13 Zn18 20 1_545 140.245(12)
Zn10 Zn13 Zn18 16_665 1_545 140.245(12)
Zn6 Zn13 Zn18 . 1_545 137.534(18)
Zn40 Zn13 Zn11 17_655 16_655 112.52(2)
Zn40 Zn13 Zn11 . 16_655 120.26(2)
Zn10 Zn13 Zn11 20 16_655 104.152(11)
Zn10 Zn13 Zn11 16_665 16_655 141.668(18)
Zn6 Zn13 Zn11 . 16_655 77.717(14)
Zn18 Zn13 Zn11 1_545 16_655 64.729(12)
Zn40 Zn13 Zn11 17_655 12 120.26(2)
Zn40 Zn13 Zn11 . 12 112.52(2)
Zn10 Zn13 Zn11 20 12 141.668(18)
Zn10 Zn13 Zn11 16_665 12 104.152(11)
Zn6 Zn13 Zn11 . 12 77.717(14)
Zn18 Zn13 Zn11 1_545 12 64.729(12)
Zn11 Zn13 Zn11 16_655 12 54.120(12)
Zn40 Zn13 Zn14 17_655 17_655 67.49(2)
Zn40 Zn13 Zn14 . 17_655 82.37(2)
Zn10 Zn13 Zn14 20 17_655 70.316(12)
Zn10 Zn13 Zn14 16_665 17_655 141.207(16)
Zn6 Zn13 Zn14 . 17_655 108.127(9)
Zn18 Zn13 Zn14 1_545 17_655 71.233(9)
Zn11 Zn13 Zn14 16_655 17_655 61.329(9)
Zn11 Zn13 Zn14 12 17_655 112.082(13)
Zn40 Zn13 Zn14 17_655 . 82.37(2)
Zn40 Zn13 Zn14 . . 67.49(2)
Zn10 Zn13 Zn14 20 . 141.207(16)
Zn10 Zn13 Zn14 16_665 . 70.316(12)
Zn6 Zn13 Zn14 . . 108.127(9)
Zn18 Zn13 Zn14 1_545 . 71.233(9)
Zn11 Zn13 Zn14 16_655 . 112.082(13)
Zn11 Zn13 Zn14 12 . 61.329(9)
Zn14 Zn13 Zn14 17_655 . 140.273(18)
Zn40 Zn13 Zn39 17_655 17_655 26.85(3)
Zn40 Zn13 Zn39 . 17_655 40.57(3)
Zn10 Zn13 Zn39 20 17_655 71.32(3)
Zn10 Zn13 Zn39 16_665 17_655 105.76(2)
Zn6 Zn13 Zn39 . 17_655 137.10(3)
Zn18 Zn13 Zn39 1_545 17_655 76.84(3)
Zn11 Zn13 Zn39 16_655 17_655 109.238(19)
Zn11 Zn13 Zn39 12 17_655 141.57(3)
Zn14 Zn13 Zn39 17_655 17_655 50.671(19)
Zn14 Zn13 Zn39 . 17_655 107.73(3)
Zn40 Zn13 Zn39 17_655 . 40.57(3)
Zn40 Zn13 Zn39 . . 26.85(3)
Zn10 Zn13 Zn39 20 . 105.76(2)
Zn10 Zn13 Zn39 16_665 . 71.32(3)
Zn6 Zn13 Zn39 . . 137.10(3)
Zn18 Zn13 Zn39 1_545 . 76.84(3)
Zn11 Zn13 Zn39 16_655 . 141.57(3)
Zn11 Zn13 Zn39 12 . 109.238(19)
Zn14 Zn13 Zn39 17_655 . 107.73(3)
Zn14 Zn13 Zn39 . . 50.671(19)
Zn39 Zn13 Zn39 17_655 . 59.84(4)
Zn39 Zn14 Fe3 . 20 174.86(3)
Zn39 Zn14 Zn12 . 16_665 125.91(3)
Fe3 Zn14 Zn12 20 16_665 58.817(9)
Zn39 Zn14 Zn8 . . 123.30(3)
Fe3 Zn14 Zn8 20 . 59.721(9)
Zn12 Zn14 Zn8 16_665 . 63.212(10)
Zn39 Zn14 Zn20 . 12 63.07(3)
Fe3 Zn14 Zn20 20 12 112.750(14)
Zn12 Zn14 Zn20 16_665 12 128.795(14)
Zn8 Zn14 Zn20 . 12 162.384(14)
Zn39 Zn14 Zn13 . . 65.71(3)
Fe3 Zn14 Zn13 20 . 112.973(14)
Zn12 Zn14 Zn13 16_665 . 133.670(14)
Zn8 Zn14 Zn13 . . 73.767(11)
Zn20 Zn14 Zn13 12 . 97.186(13)
Zn39 Zn14 Zn17 . 20 122.51(3)
Fe3 Zn14 Zn17 20 20 56.892(10)
Zn12 Zn14 Zn17 16_665 20 60.156(13)
Zn8 Zn14 Zn17 . 20 109.628(13)
Zn20 Zn14 Zn17 12 20 73.516(13)
Zn13 Zn14 Zn17 . 20 159.029(17)
Zn39 Zn14 Zn41 . 16_665 19.35(3)
Fe3 Zn14 Zn41 20 16_665 162.83(3)
Zn12 Zn14 Zn41 16_665 16_665 109.361(18)
Zn8 Zn14 Zn41 . 16_665 128.86(3)
Zn20 Zn14 Zn41 12 16_665 63.31(3)
Zn13 Zn14 Zn41 . 16_665 84.18(3)
Zn17 Zn14 Zn41 20 16_665 107.10(3)
Zn39 Zn14 Zn16 . 20 119.57(3)
Fe3 Zn14 Zn16 20 20 55.441(10)
Zn12 Zn14 Zn16 16_665 20 105.831(12)
Zn8 Zn14 Zn16 . 20 105.629(13)
Zn20 Zn14 Zn16 12 20 60.624(11)
Zn13 Zn14 Zn16 . 20 101.362(14)
Zn17 Zn14 Zn16 20 20 57.668(14)
Zn41 Zn14 Zn16 16_665 20 123.92(3)
Zn39 Zn14 Zn11 . 12 120.87(3)
Fe3 Zn14 Zn11 20 12 56.315(9)
Zn12 Zn14 Zn11 16_665 12 106.928(12)
Zn8 Zn14 Zn11 . 12 57.673(9)
Zn20 Zn14 Zn11 12 12 104.719(13)
Zn13 Zn14 Zn11 . 12 58.674(10)
Zn17 Zn14 Zn11 20 12 104.744(13)
Zn41 Zn14 Zn11 16_665 12 140.19(2)
Zn16 Zn14 Zn11 20 12 58.349(13)
Zn39 Zn14 Zn19 . 16_665 67.51(3)
Fe3 Zn14 Zn19 20 16_665 113.068(13)
Zn12 Zn14 Zn19 16_665 16_665 80.504(12)
Zn8 Zn14 Zn19 . 16_665 141.365(13)
Zn20 Zn14 Zn19 12 16_665 55.360(10)
Zn13 Zn14 Zn19 . 16_665 132.849(15)
Zn17 Zn14 Zn19 20 16_665 57.047(10)
Zn41 Zn14 Zn19 16_665 16_665 50.24(3)
Zn16 Zn14 Zn19 20 16_665 96.243(13)
Zn11 Zn14 Zn19 12 16_665 154.503(14)
Zn39 Zn14 Zn40 . . 24.27(3)
Fe3 Zn14 Zn40 20 . 150.89(2)
Zn12 Zn14 Zn40 16_665 . 150.14(2)
Zn8 Zn14 Zn40 . . 125.455(19)
Zn20 Zn14 Zn40 12 . 52.460(18)
Zn13 Zn14 Zn40 . . 53.832(18)
Zn17 Zn14 Zn40 20 . 124.63(2)
Zn41 Zn14 Zn40 16_665 . 41.33(2)
Zn16 Zn14 Zn40 20 . 98.954(18)
Zn11 Zn14 Zn40 12 . 100.098(18)
Zn19 Zn14 Zn40 16_665 . 80.502(19)
Zn9 Zn15 Zn18 . . 108.288(15)
Zn9 Zn15 Zn18 . 16_665 108.288(15)
Zn18 Zn15 Zn18 . 16_665 110.628(15)
Zn9 Zn15 Zn18 . 20_565 108.288(15)
Zn18 Zn15 Zn18 . 20_565 110.628(15)
Zn18 Zn15 Zn18 16_665 20_565 110.628(15)
Zn9 Zn15 Zn16 . 20_565 100.045(15)
Zn18 Zn15 Zn16 . 20_565 58.520(4)
Zn18 Zn15 Zn16 16_665 20_565 58.520(4)
Zn18 Zn15 Zn16 20_565 20_565 151.67(3)
Zn9 Zn15 Zn16 . 16_665 100.045(15)
Zn18 Zn15 Zn16 . 16_665 58.520(4)
Zn18 Zn15 Zn16 16_665 16_665 151.67(3)
Zn18 Zn15 Zn16 20_565 16_665 58.520(4)
Zn16 Zn15 Zn16 20_565 16_665 117.024(9)
Zn9 Zn15 Zn16 . . 100.045(15)
Zn18 Zn15 Zn16 . . 151.67(3)
Zn18 Zn15 Zn16 16_665 . 58.520(4)
Zn18 Zn15 Zn16 20_565 . 58.520(4)
Zn16 Zn15 Zn16 20_565 . 117.024(9)
Zn16 Zn15 Zn16 16_665 . 117.024(9)
Zn9 Zn15 Zn22 . 20_565 149.261(9)
Zn18 Zn15 Zn22 . 20_565 59.179(12)
Zn18 Zn15 Zn22 16_665 20_565 59.179(12)
Zn18 Zn15 Zn22 20_565 20_565 102.45(2)
Zn16 Zn15 Zn22 20_565 20_565 49.216(12)
Zn16 Zn15 Zn22 16_665 20_565 95.839(17)
Zn16 Zn15 Zn22 . 20_565 95.839(17)
Zn9 Zn15 Zn22 . 16_665 149.261(9)
Zn18 Zn15 Zn22 . 16_665 59.179(12)
Zn18 Zn15 Zn22 16_665 16_665 102.45(2)
Zn18 Zn15 Zn22 20_565 16_665 59.179(12)
Zn16 Zn15 Zn22 20_565 16_665 95.839(17)
Zn16 Zn15 Zn22 16_665 16_665 49.216(12)
Zn16 Zn15 Zn22 . 16_665 95.839(17)
Zn22 Zn15 Zn22 20_565 16_665 52.546(16)
Zn9 Zn15 Zn22 . . 149.261(9)
Zn18 Zn15 Zn22 . . 102.45(2)
Zn18 Zn15 Zn22 16_665 . 59.179(12)
Zn18 Zn15 Zn22 20_565 . 59.179(12)
Zn16 Zn15 Zn22 20_565 . 95.839(17)
Zn16 Zn15 Zn22 16_665 . 95.839(17)
Zn16 Zn15 Zn22 . . 49.216(12)
Zn22 Zn15 Zn22 20_565 . 52.546(16)
Zn22 Zn15 Zn22 16_665 . 52.546(16)
Zn9 Zn15 Zn11 . 20_565 55.908(12)
Zn18 Zn15 Zn11 . 20_565 101.261(7)
Zn18 Zn15 Zn11 16_665 20_565 59.032(9)
Zn18 Zn15 Zn11 20_565 20_565 147.882(13)
Zn16 Zn15 Zn11 20_565 20_565 53.262(8)
Zn16 Zn15 Zn11 16_665 20_565 144.469(17)
Zn16 Zn15 Zn11 . 20_565 94.454(8)
Zn22 Zn15 Zn11 20_565 20_565 96.922(9)
Zn22 Zn15 Zn11 16_665 20_565 148.590(15)
Zn22 Zn15 Zn11 . 20_565 118.121(8)
Zn9 Zn15 Zn11 . . 55.908(12)
Zn18 Zn15 Zn11 . . 147.882(13)
Zn18 Zn15 Zn11 16_665 . 59.032(9)
Zn18 Zn15 Zn11 20_565 . 101.261(7)
Zn16 Zn15 Zn11 20_565 . 94.454(8)
Zn16 Zn15 Zn11 16_665 . 144.469(17)
Zn16 Zn15 Zn11 . . 53.262(8)
Zn22 Zn15 Zn11 20_565 . 118.121(8)
Zn22 Zn15 Zn11 16_665 . 148.590(15)
Zn22 Zn15 Zn11 . . 96.922(9)
Zn11 Zn15 Zn11 20_565 . 46.689(11)
Zn22 Zn16 Fe3 . . 175.86(2)
Zn22 Zn16 Zn17 . . 116.37(2)
Fe3 Zn16 Zn17 . . 59.488(13)
Zn22 Zn16 Zn11 . . 124.769(17)
Fe3 Zn16 Zn11 . . 58.569(10)
Zn17 Zn16 Zn11 . . 109.497(13)
Zn22 Zn16 Zn11 . 17 124.769(17)
Fe3 Zn16 Zn11 . 17 58.570(10)
Zn17 Zn16 Zn11 . 17 109.498(13)
Zn11 Zn16 Zn11 . 17 59.393(13)
Zn22 Zn16 Zn18 . 16_665 65.805(11)
Fe3 Zn16 Zn18 . 16_665 116.025(12)
Zn17 Zn16 Zn18 . 16_665 123.647(11)
Zn11 Zn16 Zn18 . 16_665 63.850(11)
Zn11 Zn16 Zn18 17 16_665 111.344(18)
Zn22 Zn16 Zn18 . 20_565 65.805(11)
Fe3 Zn16 Zn18 . 20_565 116.025(12)
Zn17 Zn16 Zn18 . 20_565 123.647(11)
Zn11 Zn16 Zn18 . 20_565 111.344(18)
Zn11 Zn16 Zn18 17 20_565 63.850(11)
Zn18 Zn16 Zn18 16_665 20_565 108.614(18)
Zn22 Zn16 Zn14 . 9 118.902(10)
Fe3 Zn16 Zn14 . 9 59.750(8)
Zn17 Zn16 Zn14 . 9 61.033(10)
Zn11 Zn16 Zn14 . 9 60.942(9)
Zn11 Zn16 Zn14 17 9 109.199(13)
Zn18 Zn16 Zn14 16_665 9 69.841(9)
Zn18 Zn16 Zn14 20_565 9 172.19(2)
Zn22 Zn16 Zn14 . 20 118.902(10)
Fe3 Zn16 Zn14 . 20 59.750(8)
Zn17 Zn16 Zn14 . 20 61.033(10)
Zn11 Zn16 Zn14 . 20 109.199(13)
Zn11 Zn16 Zn14 17 20 60.942(9)
Zn18 Zn16 Zn14 16_665 20 172.19(2)
Zn18 Zn16 Zn14 20_565 20 69.841(9)
Zn14 Zn16 Zn14 9 20 110.590(16)
Zn22 Zn16 Zn20 . . 62.087(11)
Fe3 Zn16 Zn20 . . 115.363(13)
Zn17 Zn16 Zn20 . . 74.312(13)
Zn11 Zn16 Zn20 . . 105.543(9)
Zn11 Zn16 Zn20 17 . 164.936(13)
Zn18 Zn16 Zn20 16_665 . 57.178(10)
Zn18 Zn16 Zn20 20_565 . 126.992(15)
Zn14 Zn16 Zn20 9 . 59.117(9)
Zn14 Zn16 Zn20 20 . 130.124(19)
Zn22 Zn16 Zn20 . 17 62.087(11)
Fe3 Zn16 Zn20 . 17 115.363(13)
Zn17 Zn16 Zn20 . 17 74.312(13)
Zn11 Zn16 Zn20 . 17 164.936(13)
Zn11 Zn16 Zn20 17 17 105.543(9)
Zn18 Zn16 Zn20 16_665 17 126.992(15)
Zn18 Zn16 Zn20 20_565 17 57.178(10)
Zn14 Zn16 Zn20 9 17 130.124(19)
Zn14 Zn16 Zn20 20 17 59.117(9)
Zn20 Zn16 Zn20 . 17 89.520(18)
Zn22 Zn16 Zn15 . . 67.887(19)
Fe3 Zn16 Zn15 . . 116.25(2)
Zn17 Zn16 Zn15 . . 175.74(2)
Zn11 Zn16 Zn15 . . 66.896(16)
Zn11 Zn16 Zn15 17 . 66.896(16)
Zn18 Zn16 Zn15 16_665 . 57.386(11)
Zn18 Zn16 Zn15 20_565 . 57.386(11)
Zn14 Zn16 Zn15 9 . 117.435(12)
Zn14 Zn16 Zn15 20 . 117.435(12)
Zn20 Zn16 Zn15 . . 108.567(14)
Zn20 Zn16 Zn15 17 . 108.567(14)
Zn21 Zn17 Fe3 . . 160.83(2)
Zn21 Zn17 Zn16 . . 141.76(2)
Fe3 Zn17 Zn16 . . 57.409(13)
Zn21 Zn17 Zn12 . 16_665 105.213(18)
Fe3 Zn17 Zn12 . 16_665 58.966(9)
Zn16 Zn17 Zn12 . 16_665 107.359(14)
Zn21 Zn17 Zn12 . 20_455 105.213(18)
Fe3 Zn17 Zn12 . 20_455 58.966(9)
Zn16 Zn17 Zn12 . 20_455 107.359(14)
Zn12 Zn17 Zn12 16_665 20_455 62.194(16)
Zn21 Zn17 Zn19 . 20_455 60.306(11)
Fe3 Zn17 Zn19 . 20_455 123.033(12)
Zn16 Zn17 Zn19 . 20_455 104.097(14)
Zn12 Zn17 Zn19 16_665 20_455 138.90(2)
Zn12 Zn17 Zn19 20_455 20_455 83.670(13)
Zn21 Zn17 Zn19 . 16_665 60.306(11)
Fe3 Zn17 Zn19 . 16_665 123.033(12)
Zn16 Zn17 Zn19 . 16_665 104.097(14)
Zn12 Zn17 Zn19 16_665 16_665 83.670(13)
Zn12 Zn17 Zn19 20_455 16_665 138.90(2)
Zn19 Zn17 Zn19 20_455 16_665 113.49(2)
Zn21 Zn17 Zn14 . 20 124.260(9)
Fe3 Zn17 Zn14 . 20 59.235(9)
Zn16 Zn17 Zn14 . 20 61.299(11)
Zn12 Zn17 Zn14 16_665 20 58.448(10)
Zn12 Zn17 Zn14 20_455 20 109.153(13)
Zn19 Zn17 Zn14 20_455 20 162.49(2)
Zn19 Zn17 Zn14 16_665 20 64.860(12)
Zn21 Zn17 Zn14 . 9 124.260(9)
Fe3 Zn17 Zn14 . 9 59.235(9)
Zn16 Zn17 Zn14 . 9 61.299(11)
Zn12 Zn17 Zn14 16_665 9 109.153(13)
Zn12 Zn17 Zn14 20_455 9 58.448(9)
Zn19 Zn17 Zn14 20_455 9 64.860(12)
Zn19 Zn17 Zn14 16_665 9 162.49(2)
Zn14 Zn17 Zn14 20 9 111.015(18)
Zn21 Zn17 Zn23 . . 60.651(13)
Fe3 Zn17 Zn23 . . 138.52(2)
Zn16 Zn17 Zn23 . . 81.112(17)
Zn12 Zn17 Zn23 16_665 . 147.045(8)
Zn12 Zn17 Zn23 20_455 . 147.045(8)
Zn19 Zn17 Zn23 20_455 . 63.400(12)
Zn19 Zn17 Zn23 16_665 . 63.400(12)
Zn14 Zn17 Zn23 20 . 102.845(13)
Zn14 Zn17 Zn23 9 . 102.845(13)
Zn40 Zn18 Zn40 17_665 1_565 15.15(4)
Zn40 Zn18 Zn20 17_665 16_665 57.38(2)
Zn40 Zn18 Zn20 1_565 16_665 70.08(2)
Zn40 Zn18 Zn20 17_665 12_565 70.08(2)
Zn40 Zn18 Zn20 1_565 12_565 57.38(2)
Zn20 Zn18 Zn20 16_665 12_565 97.627(18)
Zn40 Zn18 Zn13 17_665 1_565 58.32(2)
Zn40 Zn18 Zn13 1_565 1_565 58.32(2)
Zn20 Zn18 Zn13 16_665 1_565 100.225(12)
Zn20 Zn18 Zn13 12_565 1_565 100.225(12)
Zn40 Zn18 Zn15 17_665 . 171.49(2)
Zn40 Zn18 Zn15 1_565 . 171.49(2)
Zn20 Zn18 Zn15 16_665 . 118.410(13)
Zn20 Zn18 Zn15 12_565 . 118.410(13)
Zn13 Zn18 Zn15 1_565 . 118.10(2)
Zn40 Zn18 Zn16 17_665 16_665 108.32(2)
Zn40 Zn18 Zn16 1_565 16_665 123.46(2)
Zn20 Zn18 Zn16 16_665 16_665 61.682(11)
Zn20 Zn18 Zn16 12_565 16_665 151.571(17)
Zn13 Zn18 Zn16 1_565 16_665 102.482(10)
Zn15 Zn18 Zn16 . 16_665 64.094(10)
Zn40 Zn18 Zn16 17_665 20_565 123.46(2)
Zn40 Zn18 Zn16 1_565 20_565 108.32(2)
Zn20 Zn18 Zn16 16_665 20_565 151.571(17)
Zn20 Zn18 Zn16 12_565 20_565 61.682(11)
Zn13 Zn18 Zn16 1_565 20_565 102.482(10)
Zn15 Zn18 Zn16 . 20_565 64.094(10)
Zn16 Zn18 Zn16 16_665 20_565 128.17(2)
Zn40 Zn18 Zn22 17_665 16_665 113.41(2)
Zn40 Zn18 Zn22 1_565 16_665 121.41(2)
Zn20 Zn18 Zn22 16_665 16_665 59.098(12)
Zn20 Zn18 Zn22 12_565 16_665 101.164(14)
Zn13 Zn18 Zn22 1_565 16_665 151.974(8)
Zn15 Zn18 Zn22 . 16_665 65.719(16)
Zn16 Zn18 Zn22 16_665 16_665 52.307(10)
Zn16 Zn18 Zn22 20_565 16_665 103.520(14)
Zn40 Zn18 Zn22 17_665 20_565 121.41(2)
Zn40 Zn18 Zn22 1_565 20_565 113.41(2)
Zn20 Zn18 Zn22 16_665 20_565 101.164(14)
Zn20 Zn18 Zn22 12_565 20_565 59.098(12)
Zn13 Zn18 Zn22 1_565 20_565 151.973(8)
Zn15 Zn18 Zn22 . 20_565 65.719(16)
Zn16 Zn18 Zn22 16_665 20_565 103.520(14)
Zn16 Zn18 Zn22 20_565 20_565 52.307(10)
Zn22 Zn18 Zn22 16_665 20_565 56.049(16)
Zn40 Zn18 Zn11 17_665 16_665 106.09(2)
Zn40 Zn18 Zn11 1_565 16_665 112.90(2)
Zn20 Zn18 Zn11 16_665 16_665 103.776(9)
Zn20 Zn18 Zn11 12_565 16_665 151.395(13)
Zn13 Zn18 Zn11 1_565 16_665 57.671(11)
Zn15 Zn18 Zn11 . 16_665 66.902(15)
Zn16 Zn18 Zn11 16_665 16_665 57.032(10)
Zn16 Zn18 Zn11 20_565 16_665 102.739(15)
Zn22 Zn18 Zn11 16_665 16_665 106.029(11)
Zn22 Zn18 Zn11 20_565 16_665 132.499(16)
Zn40 Zn18 Zn11 17_665 12_565 112.90(2)
Zn40 Zn18 Zn11 1_565 12_565 106.09(2)
Zn20 Zn18 Zn11 16_665 12_565 151.395(13)
Zn20 Zn18 Zn11 12_565 12_565 103.776(9)
Zn13 Zn18 Zn11 1_565 12_565 57.671(11)
Zn15 Zn18 Zn11 . 12_565 66.902(15)
Zn16 Zn18 Zn11 16_665 12_565 102.739(15)
Zn16 Zn18 Zn11 20_565 12_565 57.032(10)
Zn22 Zn18 Zn11 16_665 12_565 132.499(16)
Zn22 Zn18 Zn11 20_565 12_565 106.029(11)
Zn11 Zn18 Zn11 16_665 12_565 50.313(11)
Zn41 Zn19 Zn20 . 9_665 69.186(13)
Zn41 Zn19 Zn20 . 20_665 69.186(13)
Zn20 Zn19 Zn20 9_665 20_665 133.28(2)
Zn41 Zn19 Zn21 . 1_665 174.02(5)
Zn20 Zn19 Zn21 9_665 1_665 111.822(12)
Zn20 Zn19 Zn21 20_665 1_665 111.822(12)
Zn41 Zn19 Zn43 . 12_665 45.03(4)
Zn20 Zn19 Zn43 9_665 12_665 63.417(19)
Zn20 Zn19 Zn43 20_665 12_665 72.41(2)
Zn21 Zn19 Zn43 1_665 12_665 140.90(3)
Zn41 Zn19 Zn43 . 16_665 45.03(4)
Zn20 Zn19 Zn43 9_665 16_665 72.41(2)
Zn20 Zn19 Zn43 20_665 16_665 63.417(19)
Zn21 Zn19 Zn43 1_665 16_665 140.90(3)
Zn43 Zn19 Zn43 12_665 16_665 9.08(3)
Zn41 Zn19 Zn17 . 20_665 118.86(3)
Zn20 Zn19 Zn17 9_665 20_665 145.42(2)
Zn20 Zn19 Zn17 20_665 20_665 75.466(13)
Zn21 Zn19 Zn17 1_665 20_665 56.776(13)
Zn43 Zn19 Zn17 12_665 20_665 147.74(2)
Zn43 Zn19 Zn17 16_665 20_665 138.85(2)
Zn41 Zn19 Zn17 . 16_665 118.86(3)
Zn20 Zn19 Zn17 9_665 16_665 75.466(13)
Zn20 Zn19 Zn17 20_665 16_665 145.42(2)
Zn21 Zn19 Zn17 1_665 16_665 56.776(13)
Zn43 Zn19 Zn17 12_665 16_665 138.85(2)
Zn43 Zn19 Zn17 16_665 16_665 147.74(2)
Zn17 Zn19 Zn17 20_665 16_665 71.62(2)
Zn41 Zn19 Zn25 . . 126.34(4)
Zn20 Zn19 Zn25 9_665 . 93.949(14)
Zn20 Zn19 Zn25 20_665 . 93.949(14)
Zn21 Zn19 Zn25 1_665 . 59.631(16)
Zn43 Zn19 Zn25 12_665 . 81.52(2)
Zn43 Zn19 Zn25 16_665 . 81.52(2)
Zn17 Zn19 Zn25 20_665 . 103.819(15)
Zn17 Zn19 Zn25 16_665 . 103.819(15)
Zn41 Zn19 Zn23 . 20_665 124.284(19)
Zn20 Zn19 Zn23 9_665 20_665 147.29(2)
Zn20 Zn19 Zn23 20_665 20_665 56.302(10)
Zn21 Zn19 Zn23 1_665 20_665 58.224(11)
Zn43 Zn19 Zn23 12_665 20_665 103.36(2)
Zn43 Zn19 Zn23 16_665 20_665 96.36(2)
Zn17 Zn19 Zn23 20_665 20_665 59.585(12)
Zn17 Zn19 Zn23 16_665 20_665 112.558(16)
Zn25 Zn19 Zn23 . 20_665 53.552(11)
Zn41 Zn19 Zn23 . 16_665 124.284(19)
Zn20 Zn19 Zn23 9_665 16_665 56.302(10)
Zn20 Zn19 Zn23 20_665 16_665 147.29(2)
Zn21 Zn19 Zn23 1_665 16_665 58.225(11)
Zn43 Zn19 Zn23 12_665 16_665 96.36(2)
Zn43 Zn19 Zn23 16_665 16_665 103.36(2)
Zn17 Zn19 Zn23 20_665 16_665 112.558(16)
Zn17 Zn19 Zn23 16_665 16_665 59.585(12)
Zn25 Zn19 Zn23 . 16_665 53.552(11)
Zn23 Zn19 Zn23 20_665 16_665 99.01(2)
Zn41 Zn19 Zn14 . 12_665 61.01(3)
Zn20 Zn19 Zn14 9_665 12_665 58.320(10)
Zn20 Zn19 Zn14 20_665 12_665 115.364(18)
Zn21 Zn19 Zn14 1_665 12_665 114.130(17)
Zn43 Zn19 Zn14 12_665 12_665 96.38(2)
Zn43 Zn19 Zn14 16_665 12_665 101.15(2)
Zn17 Zn19 Zn14 20_665 12_665 94.541(18)
Zn17 Zn19 Zn14 16_665 12_665 58.093(12)
Zn25 Zn19 Zn14 . 12_665 148.666(8)
Zn23 Zn19 Zn14 20_665 12_665 153.558(18)
Zn23 Zn19 Zn14 16_665 12_665 96.057(10)
Zn40 Zn20 Zn23 9 . 160.50(2)
Zn40 Zn20 Zn19 9 20_455 95.08(2)
Zn23 Zn20 Zn19 . 20_455 66.928(14)
Zn40 Zn20 Zn18 9 16_665 60.47(2)
Zn23 Zn20 Zn18 . 16_665 138.154(16)
Zn19 Zn20 Zn18 20_455 16_665 137.332(18)
Zn40 Zn20 Zn26 9 9 108.00(2)
Zn23 Zn20 Zn26 . 9 63.158(11)
Zn19 Zn20 Zn26 20_455 9 80.470(15)
Zn18 Zn20 Zn26 16_665 9 137.901(14)
Zn40 Zn20 Zn39 9 9 27.82(3)
Zn23 Zn20 Zn39 . 9 135.12(3)
Zn19 Zn20 Zn39 20_455 9 68.20(3)
Zn18 Zn20 Zn39 16_665 9 79.38(3)
Zn26 Zn20 Zn39 9 9 108.76(2)
Zn40 Zn20 Zn42 9 16_565 44.47(4)
Zn23 Zn20 Zn42 . 16_565 131.36(4)
Zn19 Zn20 Zn42 20_455 16_565 106.90(2)
Zn18 Zn20 Zn42 16_665 16_565 80.62(3)
Zn26 Zn20 Zn42 9 16_565 68.23(3)
Zn39 Zn20 Zn42 9 16_565 63.27(4)
Zn40 Zn20 Zn22 9 . 121.11(2)
Zn23 Zn20 Zn22 . . 78.257(13)
Zn19 Zn20 Zn22 20_455 . 141.147(17)
Zn18 Zn20 Zn22 16_665 . 64.229(13)
Zn26 Zn20 Zn22 9 . 99.258(14)
Zn39 Zn20 Zn22 9 . 143.61(3)
Zn42 Zn20 Zn22 16_565 . 108.93(2)
Zn40 Zn20 Zn14 9 9 68.36(2)
Zn23 Zn20 Zn14 . 9 108.356(14)
Zn19 Zn20 Zn14 20_455 9 66.320(15)
Zn18 Zn20 Zn14 16_665 9 71.974(11)
Zn26 Zn20 Zn14 9 9 145.677(15)
Zn39 Zn20 Zn14 9 9 51.70(2)
Zn42 Zn20 Zn14 16_565 9 112.35(3)
Zn22 Zn20 Zn14 . 9 111.835(14)
Zn40 Zn20 Zn24 9 16_665 86.81(2)
Zn23 Zn20 Zn24 . 16_665 103.172(14)
Zn19 Zn20 Zn24 20_455 16_665 143.748(17)
Zn18 Zn20 Zn24 16_665 16_665 73.968(12)
Zn26 Zn20 Zn24 9 16_665 64.700(11)
Zn39 Zn20 Zn24 9 16_665 112.58(3)
Zn42 Zn20 Zn24 16_565 16_665 52.05(3)
Zn22 Zn20 Zn24 . 16_665 59.462(11)
Zn14 Zn20 Zn24 9 16_665 144.647(14)
Zn40 Zn20 Zn16 9 . 110.37(2)
Zn23 Zn20 Zn16 . . 82.264(14)
Zn19 Zn20 Zn16 20_455 . 103.335(15)
Zn18 Zn20 Zn16 16_665 . 61.140(11)
Zn26 Zn20 Zn16 9 . 140.864(15)
Zn39 Zn20 Zn16 9 . 108.67(2)
Zn42 Zn20 Zn16 16_565 . 141.67(3)
Zn22 Zn20 Zn16 . . 53.567(11)
Zn14 Zn20 Zn16 9 . 60.260(10)
Zn24 Zn20 Zn16 16_665 . 109.885(14)
Zn40 Zn20 Zn43 9 9 62.11(2)
Zn23 Zn20 Zn43 . 9 100.631(17)
Zn19 Zn20 Zn43 20_455 9 59.590(19)
Zn18 Zn20 Zn43 16_665 9 120.94(2)
Zn26 Zn20 Zn43 9 9 54.350(16)
Zn39 Zn20 Zn43 9 9 54.53(2)
Zn42 Zn20 Zn43 16_565 9 48.20(3)
Zn22 Zn20 Zn43 . 9 148.01(2)
Zn14 Zn20 Zn43 9 9 98.971(19)
Zn24 Zn20 Zn43 16_665 9 90.42(2)
Zn16 Zn20 Zn43 . 9 158.43(2)
Zn17 Zn21 Zn17 16 20 77.03(2)
Zn17 Zn21 Zn17 16 . 77.03(2)
Zn17 Zn21 Zn17 20 . 77.03(2)
Zn17 Zn21 Zn19 16 1_445 62.918(10)
Zn17 Zn21 Zn19 20 1_445 62.918(10)
Zn17 Zn21 Zn19 . 1_445 127.75(2)
Zn17 Zn21 Zn19 16 20_455 62.918(10)
Zn17 Zn21 Zn19 20 20_455 127.75(2)
Zn17 Zn21 Zn19 . 20_455 62.918(10)
Zn19 Zn21 Zn19 1_445 20_455 117.988(8)
Zn17 Zn21 Zn19 16 16_665 127.75(2)
Zn17 Zn21 Zn19 20 16_665 62.918(10)
Zn17 Zn21 Zn19 . 16_665 62.918(10)
Zn19 Zn21 Zn19 1_445 16_665 117.988(8)
Zn19 Zn21 Zn19 20_455 16_665 117.988(8)
Zn17 Zn21 Zn23 16 . 125.170(9)
Zn17 Zn21 Zn23 20 . 125.170(9)
Zn17 Zn21 Zn23 . . 64.074(13)
Zn19 Zn21 Zn23 1_445 . 168.18(2)
Zn19 Zn21 Zn23 20_455 . 65.430(6)
Zn19 Zn21 Zn23 16_665 . 65.430(6)
Zn17 Zn21 Zn23 16 16 64.074(13)
Zn17 Zn21 Zn23 20 16 125.170(9)
Zn17 Zn21 Zn23 . 16 125.170(9)
Zn19 Zn21 Zn23 1_445 16 65.430(6)
Zn19 Zn21 Zn23 20_455 16 65.430(6)
Zn19 Zn21 Zn23 16_665 16 168.18(2)
Zn23 Zn21 Zn23 . 16 108.886(13)
Zn17 Zn21 Zn23 16 20 125.170(9)
Zn17 Zn21 Zn23 20 20 64.074(13)
Zn17 Zn21 Zn23 . 20 125.170(9)
Zn19 Zn21 Zn23 1_445 20 65.430(6)
Zn19 Zn21 Zn23 20_455 20 168.18(2)
Zn19 Zn21 Zn23 16_665 20 65.430(6)
Zn23 Zn21 Zn23 . 20 108.886(13)
Zn23 Zn21 Zn23 16 20 108.886(13)
Zn17 Zn21 Zn25 16 16_665 168.497(19)
Zn17 Zn21 Zn25 20 16_665 111.678(11)
Zn17 Zn21 Zn25 . 16_665 111.678(11)
Zn19 Zn21 Zn25 1_445 16_665 113.457(15)
Zn19 Zn21 Zn25 20_455 16_665 113.457(15)
Zn19 Zn21 Zn25 16_665 16_665 63.752(14)
Zn23 Zn21 Zn25 . 16_665 56.736(9)
Zn23 Zn21 Zn25 16 16_665 104.424(19)
Zn23 Zn21 Zn25 20 16_665 56.736(9)
Zn17 Zn21 Zn25 16 20_455 111.678(11)
Zn17 Zn21 Zn25 20 20_455 168.497(19)
Zn17 Zn21 Zn25 . 20_455 111.678(11)
Zn19 Zn21 Zn25 1_445 20_455 113.457(15)
Zn19 Zn21 Zn25 20_455 20_455 63.752(14)
Zn19 Zn21 Zn25 16_665 20_455 113.457(15)
Zn23 Zn21 Zn25 . 20_455 56.736(9)
Zn23 Zn21 Zn25 16 20_455 56.736(9)
Zn23 Zn21 Zn25 20 20_455 104.424(19)
Zn25 Zn21 Zn25 16_665 20_455 58.708(16)
Zn17 Zn21 Zn25 16 1_445 111.678(11)
Zn17 Zn21 Zn25 20 1_445 111.678(11)
Zn17 Zn21 Zn25 . 1_445 168.497(19)
Zn19 Zn21 Zn25 1_445 1_445 63.752(14)
Zn19 Zn21 Zn25 20_455 1_445 113.457(15)
Zn19 Zn21 Zn25 16_665 1_445 113.457(15)
Zn23 Zn21 Zn25 . 1_445 104.424(19)
Zn23 Zn21 Zn25 16 1_445 56.736(9)
Zn23 Zn21 Zn25 20 1_445 56.736(9)
Zn25 Zn21 Zn25 16_665 1_445 58.708(16)
Zn25 Zn21 Zn25 20_455 1_445 58.708(16)
Zn16 Zn22 Fe5 . . 174.59(2)
Zn16 Zn22 Zn22 . 16_665 117.448(12)
Fe5 Zn22 Zn22 . 16_665 58.129(10)
Zn16 Zn22 Zn22 . 20_565 117.448(12)
Fe5 Zn22 Zn22 . 20_565 58.129(10)
Zn22 Zn22 Zn22 16_665 20_565 60.0
Zn16 Zn22 Zn27 . . 126.09(2)
Fe5 Zn22 Zn27 . . 59.314(12)
Zn22 Zn22 Zn27 16_665 . 108.716(9)
Zn22 Zn22 Zn27 20_565 . 108.716(9)
Zn16 Zn22 Zn24 . 16_665 121.151(10)
Fe5 Zn22 Zn24 . 16_665 60.351(9)
Zn22 Zn22 Zn24 16_665 16_665 109.488(10)
Zn22 Zn22 Zn24 20_565 16_665 60.353(10)
Zn27 Zn22 Zn24 . 16_665 61.393(10)
Zn16 Zn22 Zn24 . 20_565 121.151(10)
Fe5 Zn22 Zn24 . 20_565 60.351(9)
Zn22 Zn22 Zn24 16_665 20_565 60.353(10)
Zn22 Zn22 Zn24 20_565 20_565 109.487(10)
Zn27 Zn22 Zn24 . 20_565 61.393(10)
Zn24 Zn22 Zn24 16_665 20_565 111.841(19)
Zn16 Zn22 Zn20 . . 64.346(11)
Fe5 Zn22 Zn20 . . 118.839(12)
Zn22 Zn22 Zn20 16_665 . 163.337(10)
Zn22 Zn22 Zn20 20_565 . 103.870(9)
Zn27 Zn22 Zn20 . . 79.337(13)
Zn24 Zn22 Zn20 16_665 . 60.772(10)
Zn24 Zn22 Zn20 20_565 . 134.554(19)
Zn16 Zn22 Zn20 . 17 64.346(11)
Fe5 Zn22 Zn20 . 17 118.839(12)
Zn22 Zn22 Zn20 16_665 17 103.870(9)
Zn22 Zn22 Zn20 20_565 17 163.337(10)
Zn27 Zn22 Zn20 . 17 79.337(13)
Zn24 Zn22 Zn20 16_665 17 134.554(19)
Zn24 Zn22 Zn20 20_565 17 60.772(10)
Zn20 Zn22 Zn20 . 17 91.827(18)
Zn16 Zn22 Zn18 . 16_665 61.888(9)
Fe5 Zn22 Zn18 . 16_665 115.547(11)
Zn22 Zn22 Zn18 16_665 16_665 108.390(10)
Zn22 Zn22 Zn18 20_565 16_665 61.975(8)
Zn27 Zn22 Zn18 . 16_665 127.017(11)
Zn24 Zn22 Zn18 16_665 16_665 71.324(10)
Zn24 Zn22 Zn18 20_565 16_665 168.723(19)
Zn20 Zn22 Zn18 . 16_665 56.673(9)
Zn20 Zn22 Zn18 17 16_665 125.365(14)
Zn16 Zn22 Zn18 . 20_565 61.888(9)
Fe5 Zn22 Zn18 . 20_565 115.547(11)
Zn22 Zn22 Zn18 16_665 20_565 61.975(8)
Zn22 Zn22 Zn18 20_565 20_565 108.390(10)
Zn27 Zn22 Zn18 . 20_565 127.017(11)
Zn24 Zn22 Zn18 16_665 20_565 168.723(19)
Zn24 Zn22 Zn18 20_565 20_565 71.324(10)
Zn20 Zn22 Zn18 . 20_565 125.365(14)
Zn20 Zn22 Zn18 17 20_565 56.673(9)
Zn18 Zn22 Zn18 16_665 20_565 103.502(19)
Zn16 Zn22 Zn15 . . 62.897(15)
Fe5 Zn22 Zn15 . . 111.694(17)
Zn22 Zn22 Zn15 16_665 . 63.727(8)
Zn22 Zn22 Zn15 20_565 . 63.727(8)
Zn27 Zn22 Zn15 . . 171.008(17)
Zn24 Zn22 Zn15 16_665 . 115.303(12)
Zn24 Zn22 Zn15 20_565 . 115.303(12)
Zn20 Zn22 Zn15 . . 106.713(12)
Zn20 Zn22 Zn15 17 . 106.713(12)
Zn18 Zn22 Zn15 16_665 . 55.102(10)
Zn18 Zn22 Zn15 20_565 . 55.102(10)
Zn25 Zn23 Zn25 20_455 16_665 62.509(18)
Zn25 Zn23 Zn20 20_455 17 163.185(14)
Zn25 Zn23 Zn20 16_665 17 100.702(10)
Zn25 Zn23 Zn20 20_455 . 100.702(10)
Zn25 Zn23 Zn20 16_665 . 163.185(14)
Zn20 Zn23 Zn20 17 . 96.066(17)
Zn25 Zn23 Fe6 20_455 . 58.074(11)
Zn25 Zn23 Fe6 16_665 . 58.074(11)
Zn20 Zn23 Fe6 17 . 115.267(12)
Zn20 Zn23 Fe6 . . 115.267(12)
Zn25 Zn23 Zn21 20_455 . 62.251(13)
Zn25 Zn23 Zn21 16_665 . 62.251(13)
Zn20 Zn23 Zn21 17 . 110.479(13)
Zn20 Zn23 Zn21 . . 110.479(13)
Fe6 Zn23 Zn21 . . 108.786(16)
Zn25 Zn23 Zn26 20_455 20 108.786(16)
Zn25 Zn23 Zn26 16_665 20 59.494(11)
Zn20 Zn23 Zn26 17 20 59.209(9)
Zn20 Zn23 Zn26 . 20 132.614(16)
Fe6 Zn23 Zn26 . 20 57.907(9)
Zn21 Zn23 Zn26 . 20 115.869(11)
Zn25 Zn23 Zn26 20_455 9 59.494(11)
Zn25 Zn23 Zn26 16_665 9 108.786(16)
Zn20 Zn23 Zn26 17 9 132.614(16)
Zn20 Zn23 Zn26 . 9 59.209(9)
Fe6 Zn23 Zn26 . 9 57.907(9)
Zn21 Zn23 Zn26 . 9 115.869(11)
Zn26 Zn23 Zn26 20 9 106.171(17)
Zn25 Zn23 Zn27 20_455 . 104.782(15)
Zn25 Zn23 Zn27 16_665 . 104.782(15)
Zn20 Zn23 Zn27 17 . 79.435(11)
Zn20 Zn23 Zn27 . . 79.436(11)
Fe6 Zn23 Zn27 . . 55.579(12)
Zn21 Zn23 Zn27 . . 164.365(19)
Zn26 Zn23 Zn27 20 . 57.899(9)
Zn26 Zn23 Zn27 9 . 57.899(9)
Zn25 Zn23 Zn17 20_455 . 108.908(15)
Zn25 Zn23 Zn17 16_665 . 108.908(15)
Zn20 Zn23 Zn17 17 . 74.391(12)
Zn20 Zn23 Zn17 . . 74.391(12)
Fe6 Zn23 Zn17 . . 164.061(18)
Zn21 Zn23 Zn17 . . 55.275(15)
Zn26 Zn23 Zn17 20 . 126.001(9)
Zn26 Zn23 Zn17 9 . 126.001(9)
Zn27 Zn23 Zn17 . . 140.360(18)
Zn25 Zn23 Zn19 20_455 20_455 62.257(12)
Zn25 Zn23 Zn19 16_665 20_455 110.398(16)
Zn20 Zn23 Zn19 17 20_455 128.212(18)
Zn20 Zn23 Zn19 . 20_455 56.770(10)
Fe6 Zn23 Zn19 . 20_455 116.229(13)
Zn21 Zn23 Zn19 . 20_455 56.345(10)
Zn26 Zn23 Zn19 20 20_455 169.705(17)
Zn26 Zn23 Zn19 9 20_455 74.303(10)
Zn27 Zn23 Zn19 . 20_455 127.495(9)
Zn17 Zn23 Zn19 . 20_455 57.014(12)
Zn25 Zn23 Zn19 20_455 16_665 110.398(15)
Zn25 Zn23 Zn19 16_665 16_665 62.257(12)
Zn20 Zn23 Zn19 17 16_665 56.770(10)
Zn20 Zn23 Zn19 . 16_665 128.212(18)
Fe6 Zn23 Zn19 . 16_665 116.229(13)
Zn21 Zn23 Zn19 . 16_665 56.345(9)
Zn26 Zn23 Zn19 20 16_665 74.303(10)
Zn26 Zn23 Zn19 9 16_665 169.705(17)
Zn27 Zn23 Zn19 . 16_665 127.495(9)
Zn17 Zn23 Zn19 . 16_665 57.014(12)
Zn19 Zn23 Zn19 20_455 16_665 103.35(2)
Zn42 Zn24 Fe5 1_565 . 175.02(5)
Zn42 Zn24 Zn30 1_565 . 127.76(5)
Fe5 Zn24 Zn30 . . 57.219(13)
Zn42 Zn24 Zn22 1_565 16_665 119.33(4)
Fe5 Zn24 Zn22 . 16_665 56.615(12)
Zn30 Zn24 Zn22 . 16_665 105.523(14)
Zn42 Zn24 Zn22 1_565 20_565 119.33(4)
Fe5 Zn24 Zn22 . 20_565 56.615(12)
Zn30 Zn24 Zn22 . 20_565 105.523(14)
Zn22 Zn24 Zn22 16_665 20_565 59.29(2)
Zn42 Zn24 Zn20 1_565 16_665 62.75(3)
Fe5 Zn24 Zn20 . 16_665 114.298(14)
Zn30 Zn24 Zn20 . 16_665 133.359(8)
Zn22 Zn24 Zn20 16_665 16_665 59.766(11)
Zn22 Zn24 Zn20 20_565 16_665 102.371(16)
Zn42 Zn24 Zn20 1_565 12_565 62.75(3)
Fe5 Zn24 Zn20 . 12_565 114.298(14)
Zn30 Zn24 Zn20 . 12_565 133.359(8)
Zn22 Zn24 Zn20 16_665 12_565 102.371(16)
Zn22 Zn24 Zn20 20_565 12_565 59.766(11)
Zn20 Zn24 Zn20 16_665 12_565 93.026(17)
Zn42 Zn24 Zn27 1_565 16_665 124.099(14)
Fe5 Zn24 Zn27 . 16_665 57.337(9)
Zn30 Zn24 Zn27 . 16_665 59.027(10)
Zn22 Zn24 Zn27 16_665 16_665 59.046(12)
Zn22 Zn24 Zn27 20_565 16_665 106.041(15)
Zn20 Zn24 Zn27 16_665 16_665 77.770(10)
Zn20 Zn24 Zn27 12_565 16_665 161.417(18)
Zn42 Zn24 Zn27 1_565 20_565 124.099(14)
Fe5 Zn24 Zn27 . 20_565 57.337(9)
Zn30 Zn24 Zn27 . 20_565 59.027(10)
Zn22 Zn24 Zn27 16_665 20_565 106.041(15)
Zn22 Zn24 Zn27 20_565 20_565 59.046(12)
Zn20 Zn24 Zn27 16_665 20_565 161.417(18)
Zn20 Zn24 Zn27 12_565 20_565 77.770(10)
Zn27 Zn24 Zn27 16_665 20_565 106.110(18)
Zn42 Zn24 Zn44 1_565 17_665 18.36(3)
Fe5 Zn24 Zn44 . 17_665 164.74(2)
Zn30 Zn24 Zn44 . 17_665 113.95(2)
Zn22 Zn24 Zn44 16_665 17_665 120.88(3)
Zn22 Zn24 Zn44 20_565 17_665 137.28(2)
Zn20 Zn24 Zn44 16_665 17_665 61.12(3)
Zn20 Zn24 Zn44 12_565 17_665 80.90(2)
Zn27 Zn24 Zn44 16_665 17_665 107.77(2)
Zn27 Zn24 Zn44 20_565 17_665 131.52(3)
Zn42 Zn24 Zn44 1_565 1_565 18.36(3)
Fe5 Zn24 Zn44 . 1_565 164.74(2)
Zn30 Zn24 Zn44 . 1_565 113.95(2)
Zn22 Zn24 Zn44 16_665 1_565 137.28(2)
Zn22 Zn24 Zn44 20_565 1_565 120.88(3)
Zn20 Zn24 Zn44 16_665 1_565 80.90(2)
Zn20 Zn24 Zn44 12_565 1_565 61.12(3)
Zn27 Zn24 Zn44 16_665 1_565 131.52(3)
Zn27 Zn24 Zn44 20_565 1_565 107.77(2)
Zn44 Zn24 Zn44 17_665 1_565 25.87(5)
Zn42 Zn24 Zn26 1_565 17_665 68.55(2)
Fe5 Zn24 Zn26 . 17_665 113.632(10)
Zn30 Zn24 Zn26 . 17_665 83.751(10)
Zn22 Zn24 Zn26 16_665 17_665 94.055(11)
Zn22 Zn24 Zn26 20_565 17_665 153.118(15)
Zn20 Zn24 Zn26 16_665 17_665 56.400(8)
Zn20 Zn24 Zn26 12_565 17_665 130.627(15)
Zn27 Zn24 Zn26 16_665 17_665 56.658(8)
Zn27 Zn24 Zn26 20_565 17_665 141.007(17)
Zn44 Zn24 Zn26 17_665 17_665 51.23(2)
Zn44 Zn24 Zn26 1_565 17_665 75.25(3)
Fe6 Zn25 Fe6 16_665 20_665 114.855(19)
Fe6 Zn25 Zn23 16_665 16_665 62.573(10)
Fe6 Zn25 Zn23 20_665 16_665 166.857(17)
Fe6 Zn25 Zn23 16_665 20_665 166.857(17)
Fe6 Zn25 Zn23 20_665 20_665 62.573(10)
Zn23 Zn25 Zn23 16_665 20_665 116.66(2)
Fe6 Zn25 Zn26 16_665 12_665 60.621(8)
Fe6 Zn25 Zn26 20_665 12_665 127.659(16)
Zn23 Zn25 Zn26 16_665 12_665 63.599(9)
Zn23 Zn25 Zn26 20_665 12_665 131.899(16)
Fe6 Zn25 Zn26 16_665 16_665 127.659(16)
Fe6 Zn25 Zn26 20_665 16_665 60.621(8)
Zn23 Zn25 Zn26 16_665 16_665 131.899(16)
Zn23 Zn25 Zn26 20_665 16_665 63.599(9)
Zn26 Zn25 Zn26 12_665 16_665 81.623(15)
Fe6 Zn25 Zn25 16_665 16_775 108.469(9)
Fe6 Zn25 Zn25 20_665 16_775 58.269(9)
Zn23 Zn25 Zn25 16_665 16_775 109.405(10)
Zn23 Zn25 Zn25 20_665 16_775 58.745(9)
Zn26 Zn25 Zn25 12_665 16_775 168.596(8)
Zn26 Zn25 Zn25 16_665 16_775 109.068(8)
Fe6 Zn25 Zn25 16_665 20_565 58.269(9)
Fe6 Zn25 Zn25 20_665 20_565 108.469(9)
Zn23 Zn25 Zn25 16_665 20_565 58.746(9)
Zn23 Zn25 Zn25 20_665 20_565 109.404(10)
Zn26 Zn25 Zn25 12_665 20_565 109.068(7)
Zn26 Zn25 Zn25 16_665 20_565 168.596(8)
Zn25 Zn25 Zn25 16_775 20_565 60.0
Fe6 Zn25 Zn32 16_665 . 63.909(9)
Fe6 Zn25 Zn32 20_665 . 63.909(9)
Zn23 Zn25 Zn32 16_665 . 121.090(11)
Zn23 Zn25 Zn32 20_665 . 121.090(11)
Zn26 Zn25 Zn32 12_665 . 70.097(12)
Zn26 Zn25 Zn32 16_665 . 70.097(12)
Zn25 Zn25 Zn32 16_775 . 109.154(10)
Zn25 Zn25 Zn32 20_565 . 109.154(10)
Fe6 Zn25 Zn31 16_665 1_665 60.010(9)
Fe6 Zn25 Zn31 20_665 1_665 60.010(9)
Zn23 Zn25 Zn31 16_665 1_665 111.143(11)
Zn23 Zn25 Zn31 20_665 1_665 111.143(11)
Zn26 Zn25 Zn31 12_665 1_665 112.448(12)
Zn26 Zn25 Zn31 16_665 1_665 112.448(12)
Zn25 Zn25 Zn31 16_775 1_665 60.407(8)
Zn25 Zn25 Zn31 20_565 1_665 60.407(8)
Zn32 Zn25 Zn31 . 1_665 57.029(13)
Fe6 Zn25 Zn21 16_665 1_665 111.356(10)
Fe6 Zn25 Zn21 20_665 1_665 111.356(10)
Zn23 Zn25 Zn21 16_665 1_665 61.013(11)
Zn23 Zn25 Zn21 20_665 1_665 61.013(11)
Zn26 Zn25 Zn21 12_665 1_665 118.405(12)
Zn26 Zn25 Zn21 16_665 1_665 118.405(12)
Zn25 Zn25 Zn21 16_775 1_665 60.646(8)
Zn25 Zn25 Zn21 20_565 1_665 60.646(8)
Zn32 Zn25 Zn21 . 1_665 167.789(19)
Zn31 Zn25 Zn21 1_665 1_665 110.759(16)
Fe6 Zn25 Zn19 16_665 . 122.105(9)
Fe6 Zn25 Zn19 20_665 . 122.105(9)
Zn23 Zn25 Zn19 16_665 . 64.191(10)
Zn23 Zn25 Zn19 20_665 . 64.191(10)
Zn26 Zn25 Zn19 12_665 . 76.715(12)
Zn26 Zn25 Zn19 16_665 . 76.715(12)
Zn25 Zn25 Zn19 16_775 . 109.051(9)
Zn25 Zn25 Zn19 20_565 . 109.051(9)
Zn32 Zn25 Zn19 . . 135.595(19)
Zn31 Zn25 Zn19 1_665 . 167.376(18)
Zn21 Zn25 Zn19 1_665 . 56.616(12)
Zn44 Zn26 Zn43 . . 36.16(4)
Zn44 Zn26 Zn28 . 16_665 69.11(3)
Zn43 Zn26 Zn28 . 16_665 65.41(2)
Zn44 Zn26 Fe6 . 20 176.78(3)
Zn43 Zn26 Fe6 . 20 146.89(2)
Zn28 Zn26 Fe6 16_665 20 110.604(15)
Zn44 Zn26 Zn33 . 12 121.35(3)
Zn43 Zn26 Zn33 . 12 143.34(2)
Zn28 Zn26 Zn33 16_665 12 79.665(12)
Fe6 Zn26 Zn33 20 12 55.690(9)
Zn44 Zn26 Zn25 . 16_665 125.38(3)
Zn43 Zn26 Zn25 . 16_665 89.24(2)
Zn28 Zn26 Zn25 16_665 16_665 90.321(13)
Fe6 Zn26 Zn25 20 16_665 57.654(10)
Zn33 Zn26 Zn25 12 16_665 102.243(13)
Zn44 Zn26 Zn20 . 12 66.45(2)
Zn43 Zn26 Zn20 . 12 65.767(19)
Zn28 Zn26 Zn20 16_665 12 130.318(16)
Fe6 Zn26 Zn20 20 12 114.996(13)
Zn33 Zn26 Zn20 12 12 143.876(14)
Zn25 Zn26 Zn20 16_665 12 97.683(13)
Zn44 Zn26 Zn27 . 20 121.17(3)
Zn43 Zn26 Zn27 . 20 144.71(2)
Zn28 Zn26 Zn27 16_665 20 143.996(16)
Fe6 Zn26 Zn27 20 20 57.064(10)
Zn33 Zn26 Zn27 12 20 65.546(12)
Zn25 Zn26 Zn27 16_665 20 105.319(11)
Zn20 Zn26 Zn27 12 20 80.316(13)
Zn44 Zn26 Zn23 . 20 122.88(3)
Zn43 Zn26 Zn23 . 20 104.82(2)
Zn28 Zn26 Zn23 16_665 20 146.697(15)
Fe6 Zn26 Zn23 20 20 59.202(10)
Zn33 Zn26 Zn23 12 20 110.637(12)
Zn25 Zn26 Zn23 16_665 20 56.907(11)
Zn20 Zn26 Zn23 12 20 57.633(11)
Zn27 Zn26 Zn23 20 20 61.143(11)
Zn44 Zn26 Zn43 . 20 41.94(3)
Zn43 Zn26 Zn43 . 20 7.01(3)
Zn28 Zn26 Zn43 16_665 20 61.551(19)
Fe6 Zn26 Zn43 20 20 140.974(19)
Zn33 Zn26 Zn43 12 20 140.93(2)
Zn25 Zn26 Zn43 16_665 20 83.535(17)
Zn20 Zn26 Zn43 12 20 70.751(19)
Zn27 Zn26 Zn43 20 20 150.70(2)
Zn23 Zn26 Zn43 20 20 104.814(19)
Zn44 Zn26 Zn29 . . 62.10(3)
Zn43 Zn26 Zn29 . . 92.03(2)
Zn28 Zn26 Zn29 16_665 . 59.701(10)
Fe6 Zn26 Zn29 20 . 114.863(13)
Zn33 Zn26 Zn29 12 . 59.322(10)
Zn25 Zn26 Zn29 16_665 . 145.843(14)
Zn20 Zn26 Zn29 12 . 113.887(13)
Zn27 Zn26 Zn29 20 . 93.029(13)
Zn23 Zn26 Zn29 20 . 153.071(15)
Zn43 Zn26 Zn29 20 . 94.449(18)
Zn44 Zn26 Zn24 . 1_545 62.27(3)
Zn43 Zn26 Zn24 . 1_545 93.47(2)
Zn28 Zn26 Zn24 16_665 1_545 115.939(14)
Fe6 Zn26 Zn24 20 1_545 115.686(13)
Zn33 Zn26 Zn24 12 1_545 91.974(12)
Zn25 Zn26 Zn24 16_665 1_545 152.174(14)
Zn20 Zn26 Zn24 12 1_545 58.900(11)
Zn27 Zn26 Zn24 20 1_545 59.050(10)
Zn23 Zn26 Zn24 20 1_545 95.785(12)
Zn43 Zn26 Zn24 20 1_545 100.413(18)
Zn29 Zn26 Zn24 . 1_545 61.797(11)
Fe6 Zn27 Fe5 . . 166.43(2)
Fe6 Zn27 Zn30 . 16_665 111.220(14)
Fe5 Zn27 Zn30 . 16_665 57.760(11)
Fe6 Zn27 Zn30 . 20_565 111.220(14)
Fe5 Zn27 Zn30 . 20_565 57.760(11)
Zn30 Zn27 Zn30 16_665 20_565 62.621(15)
Fe6 Zn27 Zn26 . 9 60.525(9)
Fe5 Zn27 Zn26 . 9 122.917(9)
Zn30 Zn27 Zn26 16_665 9 87.939(9)
Zn30 Zn27 Zn26 20_565 9 145.252(16)
Fe6 Zn27 Zn26 . 20 60.525(9)
Fe5 Zn27 Zn26 . 20 122.917(9)
Zn30 Zn27 Zn26 16_665 20 145.252(16)
Zn30 Zn27 Zn26 20_565 20 87.939(9)
Zn26 Zn27 Zn26 9 20 111.209(16)
Fe6 Zn27 Zn22 . . 136.240(18)
Fe5 Zn27 Zn22 . . 57.333(14)
Zn30 Zn27 Zn22 16_665 . 105.893(13)
Zn30 Zn27 Zn22 20_565 . 105.893(13)
Zn26 Zn27 Zn22 9 . 99.407(12)
Zn26 Zn27 Zn22 20 . 99.407(12)
Fe6 Zn27 Zn24 . 16_665 124.307(9)
Fe5 Zn27 Zn24 . 16_665 59.062(9)
Zn30 Zn27 Zn24 16_665 16_665 58.981(10)
Zn30 Zn27 Zn24 20_565 16_665 109.274(13)
Zn26 Zn27 Zn24 9 16_665 64.292(9)
Zn26 Zn27 Zn24 20 16_665 155.308(18)
Zn22 Zn27 Zn24 . 16_665 59.561(11)
Fe6 Zn27 Zn24 . 20_565 124.307(9)
Fe5 Zn27 Zn24 . 20_565 59.062(9)
Zn30 Zn27 Zn24 16_665 20_565 109.274(13)
Zn30 Zn27 Zn24 20_565 20_565 58.981(10)
Zn26 Zn27 Zn24 9 20_565 155.308(18)
Zn26 Zn27 Zn24 20 20_565 64.292(9)
Zn22 Zn27 Zn24 . 20_565 59.561(11)
Zn24 Zn27 Zn24 16_665 20_565 108.858(19)
Fe6 Zn27 Zn23 . . 60.178(12)
Fe5 Zn27 Zn23 . . 133.39(2)
Zn30 Zn27 Zn23 16_665 . 148.367(7)
Zn30 Zn27 Zn23 20_565 . 148.367(7)
Zn26 Zn27 Zn23 9 . 60.958(9)
Zn26 Zn27 Zn23 20 . 60.958(9)
Zn22 Zn27 Zn23 . . 76.062(15)
Zn24 Zn27 Zn23 16_665 . 98.942(12)
Zn24 Zn27 Zn23 20_565 . 98.942(12)
Fe6 Zn27 Zn33 . . 53.638(9)
Fe5 Zn27 Zn33 . . 115.595(14)
Zn30 Zn27 Zn33 16_665 . 57.892(9)
Zn30 Zn27 Zn33 20_565 . 90.507(13)
Zn26 Zn27 Zn33 9 . 56.627(9)
Zn26 Zn27 Zn33 20 . 107.935(13)
Zn22 Zn27 Zn33 . . 148.599(6)
Zn24 Zn27 Zn33 16_665 . 89.987(10)
Zn24 Zn27 Zn33 20_565 . 147.733(16)
Zn23 Zn27 Zn33 . . 103.809(12)
Fe6 Zn27 Zn33 . 17 53.639(9)
Fe5 Zn27 Zn33 . 17 115.595(14)
Zn30 Zn27 Zn33 16_665 17 90.507(13)
Zn30 Zn27 Zn33 20_565 17 57.892(9)
Zn26 Zn27 Zn33 9 17 107.935(13)
Zn26 Zn27 Zn33 20 17 56.627(9)
Zn22 Zn27 Zn33 . 17 148.599(6)
Zn24 Zn27 Zn33 16_665 17 147.733(15)
Zn24 Zn27 Zn33 20_565 17 89.987(10)
Zn23 Zn27 Zn33 . 17 103.809(12)
Zn33 Zn27 Zn33 . 17 62.653(13)
Zn45 Zn28 Zn45 20 16_665 13.64(4)
Zn45 Zn28 Zn32 20 . 169.39(3)
Zn45 Zn28 Zn32 16_665 . 169.39(3)
Zn45 Zn28 Zn26 20 16_665 106.60(2)
Zn45 Zn28 Zn26 16_665 16_665 97.34(3)
Zn32 Zn28 Zn26 . 16_665 72.073(14)
Zn45 Zn28 Zn26 20 12_665 97.34(3)
Zn45 Zn28 Zn26 16_665 12_665 106.60(2)
Zn32 Zn28 Zn26 . 12_665 72.073(14)
Zn26 Zn28 Zn26 16_665 12_665 83.359(17)
Zn45 Zn28 Zn34 20 . 57.91(2)
Zn45 Zn28 Zn34 16_665 . 57.91(2)
Zn32 Zn28 Zn34 . . 130.50(2)
Zn26 Zn28 Zn34 16_665 . 135.837(11)
Zn26 Zn28 Zn34 12_665 . 135.837(11)
Zn45 Zn28 Zn29 20 20 69.33(2)
Zn45 Zn28 Zn29 16_665 20 82.66(3)
Zn32 Zn28 Zn29 . 20 105.620(12)
Zn26 Zn28 Zn29 16_665 20 146.135(16)
Zn26 Zn28 Zn29 12_665 20 64.549(10)
Zn34 Zn28 Zn29 . 20 72.176(11)
Zn45 Zn28 Zn29 20 16_665 82.66(3)
Zn45 Zn28 Zn29 16_665 16_665 69.33(2)
Zn32 Zn28 Zn29 . 16_665 105.620(12)
Zn26 Zn28 Zn29 16_665 16_665 64.549(9)
Zn26 Zn28 Zn29 12_665 16_665 146.135(16)
Zn34 Zn28 Zn29 . 16_665 72.176(10)
Zn29 Zn28 Zn29 20 16_665 142.70(2)
Zn45 Zn28 Zn37 20 3_665 118.81(3)
Zn45 Zn28 Zn37 16_665 3_665 112.01(2)
Zn32 Zn28 Zn37 . 3_665 71.561(17)
Zn26 Zn28 Zn37 16_665 3_665 99.841(12)
Zn26 Zn28 Zn37 12_665 3_665 140.39(2)
Zn34 Zn28 Zn37 . 3_665 64.576(15)
Zn29 Zn28 Zn37 20 3_665 111.607(15)
Zn29 Zn28 Zn37 16_665 3_665 60.922(11)
Zn45 Zn28 Zn37 20 23_666 112.01(2)
Zn45 Zn28 Zn37 16_665 23_666 118.81(3)
Zn32 Zn28 Zn37 . 23_666 71.561(17)
Zn26 Zn28 Zn37 16_665 23_666 140.39(2)
Zn26 Zn28 Zn37 12_665 23_666 99.841(12)
Zn34 Zn28 Zn37 . 23_666 64.576(15)
Zn29 Zn28 Zn37 20 23_666 60.922(11)
Zn29 Zn28 Zn37 16_665 23_666 111.607(15)
Zn37 Zn28 Zn37 3_665 23_666 53.589(14)
Zn45 Zn28 Zn43 20 12_665 59.94(3)
Zn45 Zn28 Zn43 16_665 12_665 61.15(2)
Zn32 Zn28 Zn43 . 12_665 111.57(2)
Zn26 Zn28 Zn43 16_665 12_665 62.23(2)
Zn26 Zn28 Zn43 12_665 12_665 55.320(17)
Zn34 Zn28 Zn43 . 12_665 117.77(2)
Zn29 Zn28 Zn43 20 12_665 89.29(2)
Zn29 Zn28 Zn43 16_665 12_665 97.72(2)
Zn37 Zn28 Zn43 3_665 12_665 157.632(18)
Zn37 Zn28 Zn43 23_666 12_665 148.751(18)
Zn45 Zn28 Zn43 20 16_665 61.15(2)
Zn45 Zn28 Zn43 16_665 16_665 59.94(3)
Zn32 Zn28 Zn43 . 16_665 111.57(2)
Zn26 Zn28 Zn43 16_665 16_665 55.320(17)
Zn26 Zn28 Zn43 12_665 16_665 62.227(19)
Zn34 Zn28 Zn43 . 16_665 117.77(2)
Zn29 Zn28 Zn43 20 16_665 97.72(2)
Zn29 Zn28 Zn43 16_665 16_665 89.29(2)
Zn37 Zn28 Zn43 3_665 16_665 148.751(18)
Zn37 Zn28 Zn43 23_666 16_665 157.632(18)
Zn43 Zn28 Zn43 12_665 16_665 8.89(3)
Fe7 Zn29 Zn33 1_545 12 55.960(8)
Fe7 Zn29 Zn33 1_545 16_655 55.960(8)
Zn33 Zn29 Zn33 12 16_655 104.680(15)
Fe7 Zn29 Zn28 1_545 20 113.242(14)
Zn33 Zn29 Zn28 12 20 160.546(17)
Zn33 Zn29 Zn28 16_655 20 76.196(11)
Fe7 Zn29 Zn28 1_545 16_665 113.242(14)
Zn33 Zn29 Zn28 12 16_665 76.196(11)
Zn33 Zn29 Zn28 16_655 16_665 160.546(17)
Zn28 Zn29 Zn28 20 16_665 96.53(2)
Fe7 Zn29 Zn30 1_545 1_545 56.187(11)
Zn33 Zn29 Zn30 12 1_545 59.007(8)
Zn33 Zn29 Zn30 16_655 1_545 59.007(8)
Zn28 Zn29 Zn30 20 1_545 131.685(11)
Zn28 Zn29 Zn30 16_665 1_545 131.685(11)
Fe7 Zn29 Zn44 1_545 17_655 163.22(2)
Zn33 Zn29 Zn44 12 17_655 132.15(3)
Zn33 Zn29 Zn44 16_655 17_655 108.24(2)
Zn28 Zn29 Zn44 20 17_655 63.23(3)
Zn28 Zn29 Zn44 16_665 17_655 83.52(2)
Zn30 Zn29 Zn44 1_545 17_655 112.57(2)
Fe7 Zn29 Zn44 1_545 . 163.22(2)
Zn33 Zn29 Zn44 12 . 108.24(2)
Zn33 Zn29 Zn44 16_655 . 132.15(3)
Zn28 Zn29 Zn44 20 . 83.52(2)
Zn28 Zn29 Zn44 16_665 . 63.23(3)
Zn30 Zn29 Zn44 1_545 . 112.57(2)
Zn44 Zn29 Zn44 17_655 . 26.13(5)
Fe7 Zn29 Zn37 1_545 17_655 55.956(10)
Zn33 Zn29 Zn37 12 17_655 103.771(14)
Zn33 Zn29 Zn37 16_655 17_655 57.482(11)
Zn28 Zn29 Zn37 20 17_655 59.807(12)
Zn28 Zn29 Zn37 16_665 17_655 103.190(16)
Zn30 Zn29 Zn37 1_545 17_655 104.106(13)
Zn44 Zn29 Zn37 17_655 17_655 123.03(3)
Zn44 Zn29 Zn37 . 17_655 140.05(2)
Fe7 Zn29 Zn37 1_545 . 55.956(10)
Zn33 Zn29 Zn37 12 . 57.482(11)
Zn33 Zn29 Zn37 16_655 . 103.771(14)
Zn28 Zn29 Zn37 20 . 103.190(16)
Zn28 Zn29 Zn37 16_665 . 59.807(12)
Zn30 Zn29 Zn37 1_545 . 104.106(13)
Zn44 Zn29 Zn37 17_655 . 140.05(2)
Zn44 Zn29 Zn37 . . 123.03(3)
Zn37 Zn29 Zn37 17_655 . 58.664(17)
Fe7 Zn29 Zn26 1_545 17_655 111.910(10)
Zn33 Zn29 Zn26 12 17_655 141.020(15)
Zn33 Zn29 Zn26 16_655 17_655 56.459(7)
Zn28 Zn29 Zn26 20 17_655 55.749(10)
Zn28 Zn29 Zn26 16_665 17_655 133.691(17)
Zn30 Zn29 Zn26 1_545 17_655 83.125(10)
Zn44 Zn29 Zn26 17_655 17_655 51.84(2)
Zn44 Zn29 Zn26 . 17_655 76.23(3)
Zn37 Zn29 Zn26 17_655 17_655 93.483(10)
Zn37 Zn29 Zn26 . 17_655 152.090(14)
Fe7 Zn29 Zn26 1_545 . 111.910(10)
Zn33 Zn29 Zn26 12 . 56.459(7)
Zn33 Zn29 Zn26 16_655 . 141.020(15)
Zn28 Zn29 Zn26 20 . 133.691(17)
Zn28 Zn29 Zn26 16_665 . 55.749(10)
Zn30 Zn29 Zn26 1_545 . 83.125(10)
Zn44 Zn29 Zn26 17_655 . 76.23(3)
Zn44 Zn29 Zn26 . . 51.84(2)
Zn37 Zn29 Zn26 17_655 . 152.090(14)
Zn37 Zn29 Zn26 . . 93.483(10)
Zn26 Zn29 Zn26 17_655 . 114.270(17)
Fe5 Zn30 Fe7 . . 172.423(16)
Fe5 Zn30 Zn24 . . 60.677(12)
Fe7 Zn30 Zn24 . . 126.900(16)
Fe5 Zn30 Zn27 . 16_665 59.420(9)
Fe7 Zn30 Zn27 . 16_665 122.523(9)
Zn24 Zn30 Zn27 . 16_665 61.991(9)
Fe5 Zn30 Zn27 . 20_565 59.420(9)
Fe7 Zn30 Zn27 . 20_565 122.523(9)
Zn24 Zn30 Zn27 . 20_565 61.991(9)
Zn27 Zn30 Zn27 16_665 20_565 110.762(18)
Fe5 Zn30 Zn33 . 16_665 124.322(7)
Fe7 Zn30 Zn33 . 16_665 57.811(7)
Zn24 Zn30 Zn33 . 16_665 95.907(10)
Zn27 Zn30 Zn33 16_665 16_665 64.970(8)
Zn27 Zn30 Zn33 20_565 16_665 153.678(14)
Fe5 Zn30 Zn33 . 12_565 124.322(7)
Fe7 Zn30 Zn33 . 12_565 57.811(7)
Zn24 Zn30 Zn33 . 12_565 95.907(10)
Zn27 Zn30 Zn33 16_665 12_565 153.678(14)
Zn27 Zn30 Zn33 20_565 12_565 64.970(8)
Zn33 Zn30 Zn33 16_665 12_565 106.573(14)
Fe5 Zn30 Zn35 . 3_665 115.846(11)
Fe7 Zn30 Zn35 . 3_665 57.974(8)
Zn24 Zn30 Zn35 . 3_665 149.604(9)
Zn27 Zn30 Zn35 16_665 3_665 89.646(10)
Zn27 Zn30 Zn35 20_565 3_665 145.712(15)
Zn33 Zn30 Zn35 16_665 3_665 59.780(11)
Zn33 Zn30 Zn35 12_565 3_665 107.909(11)
Fe5 Zn30 Zn35 . 7_565 115.846(11)
Fe7 Zn30 Zn35 . 7_565 57.974(8)
Zn24 Zn30 Zn35 . 7_565 149.604(9)
Zn27 Zn30 Zn35 16_665 7_565 145.712(15)
Zn27 Zn30 Zn35 20_565 7_565 89.646(10)
Zn33 Zn30 Zn35 16_665 7_565 107.909(11)
Zn33 Zn30 Zn35 12_565 7_565 59.780(11)
Zn35 Zn30 Zn35 3_665 7_565 60.760(18)
Fe5 Zn30 Zn29 . 1_565 126.740(15)
Fe7 Zn30 Zn29 . 1_565 60.837(12)
Zn24 Zn30 Zn29 . 1_565 66.063(13)
Zn27 Zn30 Zn29 16_665 1_565 95.837(9)
Zn27 Zn30 Zn29 20_565 1_565 95.837(9)
Zn33 Zn30 Zn29 16_665 1_565 60.232(8)
Zn33 Zn30 Zn29 12_565 1_565 60.232(8)
Zn35 Zn30 Zn29 3_665 1_565 109.620(12)
Zn35 Zn30 Zn29 7_565 1_565 109.620(12)
Fe5 Zn30 Zn30 . 16_665 56.869(7)
Fe7 Zn30 Zn30 . 16_665 116.950(8)
Zn24 Zn30 Zn30 . 16_665 108.544(9)
Zn27 Zn30 Zn30 16_665 16_665 107.654(7)
Zn27 Zn30 Zn30 20_565 16_665 58.690(7)
Zn33 Zn30 Zn30 16_665 16_665 147.400(8)
Zn33 Zn30 Zn30 12_565 16_665 92.339(8)
Zn35 Zn30 Zn30 3_665 16_665 89.487(10)
Zn35 Zn30 Zn30 7_565 16_665 59.024(6)
Zn29 Zn30 Zn30 1_565 16_665 149.9140(10)
Fe5 Zn30 Zn30 . 20_565 56.869(7)
Fe7 Zn30 Zn30 . 20_565 116.950(8)
Zn24 Zn30 Zn30 . 20_565 108.544(9)
Zn27 Zn30 Zn30 16_665 20_565 58.690(7)
Zn27 Zn30 Zn30 20_565 20_565 107.654(7)
Zn33 Zn30 Zn30 16_665 20_565 92.339(7)
Zn33 Zn30 Zn30 12_565 20_565 147.400(8)
Zn35 Zn30 Zn30 3_665 20_565 59.024(6)
Zn35 Zn30 Zn30 7_565 20_565 89.487(10)
Zn29 Zn30 Zn30 1_565 20_565 149.9140(10)
Zn30 Zn30 Zn30 16_665 20_565 60.0
Zn32 Zn31 Zn32 16_665 1_445 119.040(6)
Zn32 Zn31 Zn32 16_665 20_455 119.040(6)
Zn32 Zn31 Zn32 1_445 20_455 119.040(6)
Zn32 Zn31 Fe6 16_665 16 165.86(3)
Zn32 Zn31 Fe6 1_445 16 64.229(5)
Zn32 Zn31 Fe6 20_455 16 64.229(5)
Zn32 Zn31 Fe6 16_665 . 64.229(5)
Zn32 Zn31 Fe6 1_445 . 165.86(3)
Zn32 Zn31 Fe6 20_455 . 64.229(5)
Fe6 Zn31 Fe6 16 . 109.146(13)
Zn32 Zn31 Fe6 16_665 20 64.229(5)
Zn32 Zn31 Fe6 1_445 20 64.229(5)
Zn32 Zn31 Fe6 20_455 20 165.86(3)
Fe6 Zn31 Fe6 16 20 109.146(13)
Fe6 Zn31 Fe6 . 20 109.146(13)
Zn32 Zn31 Zn36 16_665 . 63.405(9)
Zn32 Zn31 Zn36 1_445 . 135.09(3)
Zn32 Zn31 Zn36 20_455 . 63.405(9)
Fe6 Zn31 Zn36 16 . 125.351(8)
Fe6 Zn31 Zn36 . . 59.045(9)
Fe6 Zn31 Zn36 20 . 125.351(8)
Zn32 Zn31 Zn36 16_665 7 63.405(9)
Zn32 Zn31 Zn36 1_445 7 63.405(9)
Zn32 Zn31 Zn36 20_455 7 135.09(3)
Fe6 Zn31 Zn36 16 7 125.351(8)
Fe6 Zn31 Zn36 . 7 125.351(8)
Fe6 Zn31 Zn36 20 7 59.045(9)
Zn36 Zn31 Zn36 . 7 84.232(17)
Zn32 Zn31 Zn36 16_665 3 135.09(3)
Zn32 Zn31 Zn36 1_445 3 63.405(9)
Zn32 Zn31 Zn36 20_455 3 63.405(9)
Fe6 Zn31 Zn36 16 3 59.045(9)
Fe6 Zn31 Zn36 . 3 125.351(8)
Fe6 Zn31 Zn36 20 3 125.351(8)
Zn36 Zn31 Zn36 . 3 84.232(17)
Zn36 Zn31 Zn36 7 3 84.232(17)
Zn32 Zn31 Zn25 16_665 1_445 111.390(16)
Zn32 Zn31 Zn25 1_445 1_445 60.891(14)
Zn32 Zn31 Zn25 20_455 1_445 111.390(16)
Fe6 Zn31 Zn25 16 1_445 56.875(9)
Fe6 Zn31 Zn25 . 1_445 104.97(2)
Fe6 Zn31 Zn25 20 1_445 56.875(9)
Zn36 Zn31 Zn25 . 1_445 164.017(19)
Zn36 Zn31 Zn25 7 1_445 107.396(8)
Zn36 Zn31 Zn25 3 1_445 107.396(8)
Zn32 Zn31 Zn25 16_665 20_455 111.390(16)
Zn32 Zn31 Zn25 1_445 20_455 111.390(16)
Zn32 Zn31 Zn25 20_455 20_455 60.891(14)
Fe6 Zn31 Zn25 16 20_455 56.875(9)
Fe6 Zn31 Zn25 . 20_455 56.876(9)
Fe6 Zn31 Zn25 20 20_455 104.97(2)
Zn36 Zn31 Zn25 . 20_455 107.396(8)
Zn36 Zn31 Zn25 7 20_455 164.017(19)
Zn36 Zn31 Zn25 3 20_455 107.396(8)
Zn25 Zn31 Zn25 1_445 20_455 59.186(17)
Zn32 Zn31 Zn25 16_665 16_665 60.891(14)
Zn32 Zn31 Zn25 1_445 16_665 111.390(16)
Zn32 Zn31 Zn25 20_455 16_665 111.390(16)
Fe6 Zn31 Zn25 16 16_665 104.97(2)
Fe6 Zn31 Zn25 . 16_665 56.876(9)
Fe6 Zn31 Zn25 20 16_665 56.875(9)
Zn36 Zn31 Zn25 . 16_665 107.396(8)
Zn36 Zn31 Zn25 7 16_665 107.396(8)
Zn36 Zn31 Zn25 3 16_665 164.017(19)
Zn25 Zn31 Zn25 1_445 16_665 59.186(17)
Zn25 Zn31 Zn25 20_455 16_665 59.186(17)
Zn31 Zn32 Zn28 1_665 . 152.00(3)
Zn31 Zn32 Zn25 1_665 . 62.079(18)
Zn28 Zn32 Zn25 . . 89.923(19)
Zn31 Zn32 Fe6 1_665 16_665 58.913(10)
Zn28 Zn32 Fe6 . 16_665 106.545(14)
Zn25 Zn32 Fe6 . 16_665 55.673(10)
Zn31 Zn32 Fe6 1_665 20_665 58.913(10)
Zn28 Zn32 Fe6 . 20_665 106.545(14)
Zn25 Zn32 Fe6 . 20_665 55.673(10)
Fe6 Zn32 Fe6 16_665 20_665 101.592(17)
Zn31 Zn32 Zn36 1_665 3_665 60.562(13)
Zn28 Zn32 Zn36 . 3_665 134.779(12)
Zn25 Zn32 Zn36 . 3_665 106.192(13)
Fe6 Zn32 Zn36 16_665 3_665 56.640(8)
Fe6 Zn32 Zn36 20_665 3_665 117.541(17)
Zn31 Zn32 Zn36 1_665 7_665 60.562(13)
Zn28 Zn32 Zn36 . 7_665 134.779(12)
Zn25 Zn32 Zn36 . 7_665 106.192(13)
Fe6 Zn32 Zn36 16_665 7_665 117.541(17)
Fe6 Zn32 Zn36 20_665 7_665 56.640(8)
Zn36 Zn32 Zn36 3_665 7_665 81.56(2)
Zn31 Zn32 Zn33 1_665 9_665 105.063(9)
Zn28 Zn32 Zn33 . 9_665 77.228(10)
Zn25 Zn32 Zn33 . 9_665 97.903(11)
Fe6 Zn32 Zn33 16_665 9_665 52.595(8)
Fe6 Zn32 Zn33 20_665 9_665 152.730(18)
Zn36 Zn32 Zn33 3_665 9_665 59.124(11)
Zn36 Zn32 Zn33 7_665 9_665 138.420(19)
Zn31 Zn32 Zn33 1_665 20_665 105.063(9)
Zn28 Zn32 Zn33 . 20_665 77.228(10)
Zn25 Zn32 Zn33 . 20_665 97.903(11)
Fe6 Zn32 Zn33 16_665 20_665 152.730(18)
Fe6 Zn32 Zn33 20_665 20_665 52.595(7)
Zn36 Zn32 Zn33 3_665 20_665 138.420(19)
Zn36 Zn32 Zn33 7_665 20_665 59.124(11)
Zn33 Zn32 Zn33 9_665 20_665 149.802(18)
Zn31 Zn32 Zn32 1_665 14_556 95.658(16)
Zn28 Zn32 Zn32 . 14_556 112.340(13)
Zn25 Zn32 Zn32 . 14_556 157.737(12)
Fe6 Zn32 Zn32 16_665 14_556 114.438(11)
Fe6 Zn32 Zn32 20_665 14_556 114.438(11)
Zn36 Zn32 Zn32 3_665 14_556 58.346(9)
Zn36 Zn32 Zn32 7_665 14_556 58.346(9)
Zn33 Zn32 Zn32 9_665 14_556 87.512(11)
Zn33 Zn32 Zn32 20_665 14_556 87.512(11)
Zn31 Zn32 Zn26 1_665 12_665 104.225(17)
Zn28 Zn32 Zn26 . 12_665 54.102(11)
Zn25 Zn32 Zn26 . 12_665 54.538(11)
Fe6 Zn32 Zn26 16_665 12_665 53.224(9)
Fe6 Zn32 Zn26 20_665 12_665 106.185(17)
Zn36 Zn32 Zn26 3_665 12_665 101.785(9)
Zn36 Zn32 Zn26 7_665 12_665 160.701(17)
Zn33 Zn32 Zn26 9_665 12_665 53.388(8)
Zn33 Zn32 Zn26 20_665 12_665 119.790(16)
Zn32 Zn32 Zn26 14_556 12_665 139.355(8)
Zn31 Zn32 Zn26 1_665 16_665 104.225(17)
Zn28 Zn32 Zn26 . 16_665 54.102(11)
Zn25 Zn32 Zn26 . 16_665 54.538(11)
Fe6 Zn32 Zn26 16_665 16_665 106.185(17)
Fe6 Zn32 Zn26 20_665 16_665 53.224(9)
Zn36 Zn32 Zn26 3_665 16_665 160.701(17)
Zn36 Zn32 Zn26 7_665 16_665 101.785(9)
Zn33 Zn32 Zn26 9_665 16_665 119.790(16)
Zn33 Zn32 Zn26 20_665 16_665 53.388(8)
Zn32 Zn32 Zn26 14_556 16_665 139.355(8)
Zn26 Zn32 Zn26 12_665 16_665 68.964(14)
Fe6 Zn33 Fe7 . 3_665 166.234(15)
Fe6 Zn33 Zn26 . 9 61.914(9)
Fe7 Zn33 Zn26 3_665 9 124.787(11)
Fe6 Zn33 Zn37 . 9 133.760(14)
Fe7 Zn33 Zn37 3_665 9 59.211(12)
Zn26 Zn33 Zn37 9 9 101.680(11)
Fe6 Zn33 Zn33 . 14_556 120.997(8)
Fe7 Zn33 Zn33 3_665 14_556 58.204(5)
Zn26 Zn33 Zn33 9 14_556 157.992(8)
Zn37 Zn33 Zn33 9 14_556 59.616(7)
Fe6 Zn33 Zn35 . . 108.585(11)
Fe7 Zn33 Zn35 3_665 . 58.297(10)
Zn26 Zn33 Zn35 9 . 141.736(12)
Zn37 Zn33 Zn35 9 . 108.481(9)
Zn33 Zn33 Zn35 14_556 . 60.108(6)
Fe6 Zn33 Zn30 . 16_665 112.835(12)
Fe7 Zn33 Zn30 3_665 16_665 58.403(8)
Zn26 Zn33 Zn30 9 16_665 88.211(11)
Zn37 Zn33 Zn30 9 16_665 109.136(12)
Zn33 Zn33 Zn30 14_556 16_665 108.179(8)
Zn35 Zn33 Zn30 . 16_665 60.173(11)
Fe6 Zn33 Zn29 . 16_565 125.946(13)
Fe7 Zn33 Zn29 3_665 16_565 61.226(9)
Zn26 Zn33 Zn29 9 16_565 64.219(10)
Zn37 Zn33 Zn29 9 16_565 62.184(12)
Zn33 Zn33 Zn29 14_556 16_565 110.491(9)
Zn35 Zn33 Zn29 . 16_565 110.373(11)
Zn30 Zn33 Zn29 16_665 16_565 60.760(10)
Fe6 Zn33 Zn36 . . 60.483(9)
Fe7 Zn33 Zn36 3_665 . 118.362(9)
Zn26 Zn33 Zn36 9 . 114.920(11)
Zn37 Zn33 Zn36 9 . 96.906(11)
Zn33 Zn33 Zn36 14_556 . 60.835(6)
Zn35 Zn33 Zn36 . . 84.593(12)
Zn30 Zn33 Zn36 16_665 . 141.002(14)
Zn29 Zn33 Zn36 16_565 . 156.888(13)
Fe6 Zn33 Zn32 . 20_455 63.454(11)
Fe7 Zn33 Zn32 3_665 20_455 129.197(15)
Zn26 Zn33 Zn32 9 20_455 68.810(13)
Zn37 Zn33 Zn32 9 20_455 70.307(13)
Zn33 Zn33 Zn32 14_556 20_455 92.489(11)
Zn35 Zn33 Zn32 . 20_455 143.812(15)
Zn30 Zn33 Zn32 16_665 20_455 155.873(15)
Zn29 Zn33 Zn32 16_565 20_455 100.875(13)
Zn36 Zn33 Zn32 . 20_455 60.347(12)
Fe6 Zn33 Zn27 . . 56.017(10)
Fe7 Zn33 Zn27 3_665 . 115.316(11)
Zn26 Zn33 Zn27 9 . 57.826(9)
Zn37 Zn33 Zn27 9 . 152.909(12)
Zn33 Zn33 Zn27 14_556 . 143.651(7)
Zn35 Zn33 Zn27 . . 85.559(10)
Zn30 Zn33 Zn27 16_665 . 57.138(9)
Zn29 Zn33 Zn27 16_565 . 91.459(11)
Zn36 Zn33 Zn27 . . 107.643(9)
Zn32 Zn33 Zn27 20_455 . 112.015(13)
Fe6 Zn33 Zn33 . 17 52.555(7)
Fe7 Zn33 Zn33 3_665 17 114.385(10)
Zn26 Zn33 Zn33 9 17 105.642(8)
Zn37 Zn33 Zn33 9 17 148.298(7)
Zn33 Zn33 Zn33 14_556 17 90.0
Zn35 Zn33 Zn33 . 17 56.106(6)
Zn30 Zn33 Zn33 16_665 17 87.661(7)
Zn29 Zn33 Zn33 16_565 17 146.046(9)
Zn36 Zn33 Zn33 . 17 56.955(7)
Zn32 Zn33 Zn33 20_455 17 105.088(9)
Zn27 Zn33 Zn33 . 17 58.674(6)
Zn34 Zn34 Zn45 14_556 . 172.02(2)
Zn34 Zn34 Zn45 14_556 16_665 172.02(3)
Zn45 Zn34 Zn45 . 16_665 13.82(4)
Zn34 Zn34 Zn45 14_556 20 172.02(2)
Zn45 Zn34 Zn45 . 20 13.82(4)
Zn45 Zn34 Zn45 16_665 20 13.82(4)
Zn34 Zn34 Zn28 14_556 20 117.160(14)
Zn45 Zn34 Zn28 . 20 59.080(17)
Zn45 Zn34 Zn28 16_665 20 59.080(17)
Zn45 Zn34 Zn28 20 20 70.82(3)
Zn34 Zn34 Zn28 14_556 16_665 117.160(14)
Zn45 Zn34 Zn28 . 16_665 59.080(17)
Zn45 Zn34 Zn28 16_665 16_665 70.82(3)
Zn45 Zn34 Zn28 20 16_665 59.080(17)
Zn28 Zn34 Zn28 20 16_665 100.803(18)
Zn34 Zn34 Zn28 14_556 . 117.160(14)
Zn45 Zn34 Zn28 . . 70.82(3)
Zn45 Zn34 Zn28 16_665 . 59.080(17)
Zn45 Zn34 Zn28 20 . 59.080(17)
Zn28 Zn34 Zn28 20 . 100.803(18)
Zn28 Zn34 Zn28 16_665 . 100.803(18)
Zn34 Zn34 Zn37 14_556 9_655 64.442(10)
Zn45 Zn34 Zn37 . 9_655 115.078(10)
Zn45 Zn34 Zn37 16_665 9_655 108.69(2)
Zn45 Zn34 Zn37 20 9_655 122.51(2)
Zn28 Zn34 Zn37 20 9_655 59.414(10)
Zn28 Zn34 Zn37 16_665 9_655 151.753(7)
Zn28 Zn34 Zn37 . 9_655 102.635(7)
Zn34 Zn34 Zn37 14_556 17_655 64.442(10)
Zn45 Zn34 Zn37 . 17_655 108.69(2)
Zn45 Zn34 Zn37 16_665 17_655 115.078(10)
Zn45 Zn34 Zn37 20 17_655 122.51(2)
Zn28 Zn34 Zn37 20 17_655 59.413(10)
Zn28 Zn34 Zn37 16_665 17_655 102.635(7)
Zn28 Zn34 Zn37 . 17_655 151.753(7)
Zn37 Zn34 Zn37 9_655 17_655 50.895(14)
Zn34 Zn34 Zn37 14_556 3_665 64.442(10)
Zn45 Zn34 Zn37 . 3_665 122.51(2)
Zn45 Zn34 Zn37 16_665 3_665 108.69(2)
Zn45 Zn34 Zn37 20 3_665 115.078(11)
Zn28 Zn34 Zn37 20 3_665 102.635(7)
Zn28 Zn34 Zn37 16_665 3_665 151.753(7)
Zn28 Zn34 Zn37 . 3_665 59.414(10)
Zn37 Zn34 Zn37 9_655 3_665 56.345(15)
Zn37 Zn34 Zn37 17_655 3_665 102.756(12)
Zn34 Zn34 Zn37 14_556 . 64.442(10)
Zn45 Zn34 Zn37 . . 108.69(2)
Zn45 Zn34 Zn37 16_665 . 122.51(2)
Zn45 Zn34 Zn37 20 . 115.078(11)
Zn28 Zn34 Zn37 20 . 102.635(7)
Zn28 Zn34 Zn37 16_665 . 59.413(10)
Zn28 Zn34 Zn37 . . 151.753(7)
Zn37 Zn34 Zn37 9_655 . 102.756(12)
Zn37 Zn34 Zn37 17_655 . 56.345(15)
Zn37 Zn34 Zn37 3_665 . 128.79(2)
Zn34 Zn34 Zn37 14_556 23_666 64.442(10)
Zn45 Zn34 Zn37 . 23_666 122.51(2)
Zn45 Zn34 Zn37 16_665 23_666 115.078(10)
Zn45 Zn34 Zn37 20 23_666 108.69(2)
Zn28 Zn34 Zn37 20 23_666 151.753(8)
Zn28 Zn34 Zn37 16_665 23_666 102.635(7)
Zn28 Zn34 Zn37 . 23_666 59.414(10)
Zn37 Zn34 Zn37 9_655 23_666 102.756(12)
Zn37 Zn34 Zn37 17_655 23_666 128.79(2)
Zn37 Zn34 Zn37 3_665 23_666 50.895(14)
Zn37 Zn34 Zn37 . 23_666 102.756(12)
Fe7 Zn35 Fe7 3_665 7_565 175.30(2)
Fe7 Zn35 Zn33 3_665 . 57.995(7)
Fe7 Zn35 Zn33 7_565 . 125.759(14)
Fe7 Zn35 Zn33 3_665 17 125.759(14)
Fe7 Zn35 Zn33 7_565 17 57.995(7)
Zn33 Zn35 Zn33 . 17 67.787(13)
Fe7 Zn35 Zn33 3_665 14_556 57.995(7)
Fe7 Zn35 Zn33 7_565 14_556 125.759(14)
Zn33 Zn35 Zn33 . 14_556 59.785(12)
Zn33 Zn35 Zn33 17 14_556 96.817(17)
Fe7 Zn35 Zn33 3_665 6 125.759(14)
Fe7 Zn35 Zn33 7_565 6 57.995(7)
Zn33 Zn35 Zn33 . 6 96.817(17)
Zn33 Zn35 Zn33 17 6 59.785(12)
Zn33 Zn35 Zn33 14_556 6 67.787(13)
Fe7 Zn35 Zn30 3_665 7_565 120.166(8)
Fe7 Zn35 Zn30 7_565 7_565 58.264(6)
Zn33 Zn35 Zn30 . 7_565 151.653(16)
Zn33 Zn35 Zn30 17 7_565 107.822(9)
Zn33 Zn35 Zn30 14_556 7_565 94.286(7)
Zn33 Zn35 Zn30 6 7_565 60.047(7)
Fe7 Zn35 Zn30 3_665 3_665 58.264(6)
Fe7 Zn35 Zn30 7_565 3_665 120.166(8)
Zn33 Zn35 Zn30 . 3_665 107.822(9)
Zn33 Zn35 Zn30 17 3_665 151.653(16)
Zn33 Zn35 Zn30 14_556 3_665 60.047(7)
Zn33 Zn35 Zn30 6 3_665 94.286(7)
Zn30 Zn35 Zn30 7_565 3_665 61.952(12)
Fe7 Zn35 Zn30 3_665 16_665 58.264(6)
Fe7 Zn35 Zn30 7_565 16_665 120.166(8)
Zn33 Zn35 Zn30 . 16_665 60.047(7)
Zn33 Zn35 Zn30 17 16_665 94.286(7)
Zn33 Zn35 Zn30 14_556 16_665 107.822(9)
Zn33 Zn35 Zn30 6 16_665 151.653(16)
Zn30 Zn35 Zn30 7_565 16_665 146.66(2)
Zn30 Zn35 Zn30 3_665 16_665 107.798(12)
Fe7 Zn35 Zn30 3_665 20_565 120.166(8)
Fe7 Zn35 Zn30 7_565 20_565 58.264(6)
Zn33 Zn35 Zn30 . 20_565 94.286(7)
Zn33 Zn35 Zn30 17 20_565 60.047(7)
Zn33 Zn35 Zn30 14_556 20_565 151.653(16)
Zn33 Zn35 Zn30 6 20_565 107.822(9)
Zn30 Zn35 Zn30 7_565 20_565 107.798(12)
Zn30 Zn35 Zn30 3_665 20_565 146.66(2)
Zn30 Zn35 Zn30 16_665 20_565 61.952(12)
Fe7 Zn35 Zn35 3_665 3_665 117.652(11)
Fe7 Zn35 Zn35 7_565 3_665 57.652(11)
Zn33 Zn35 Zn35 . 3_665 148.617(7)
Zn33 Zn35 Zn35 17 3_665 107.221(8)
Zn33 Zn35 Zn35 14_556 3_665 148.617(7)
Zn33 Zn35 Zn35 6 3_665 107.221(8)
Zn30 Zn35 Zn35 7_565 3_665 59.620(9)
Zn30 Zn35 Zn35 3_665 3_665 90.513(10)
Zn30 Zn35 Zn35 16_665 3_665 90.513(10)
Zn30 Zn35 Zn35 20_565 3_665 59.620(9)
Fe7 Zn35 Zn35 3_665 7_565 57.652(11)
Fe7 Zn35 Zn35 7_565 7_565 117.652(11)
Zn33 Zn35 Zn35 . 7_565 107.221(8)
Zn33 Zn35 Zn35 17 7_565 148.617(7)
Zn33 Zn35 Zn35 14_556 7_565 107.221(8)
Zn33 Zn35 Zn35 6 7_565 148.617(7)
Zn30 Zn35 Zn35 7_565 7_565 90.513(10)
Zn30 Zn35 Zn35 3_665 7_565 59.620(9)
Zn30 Zn35 Zn35 16_665 7_565 59.620(9)
Zn30 Zn35 Zn35 20_565 7_565 90.513(10)
Zn35 Zn35 Zn35 3_665 7_565 60.0
Fe6 Zn36 Fe6 14_556 . 163.21(2)
Fe6 Zn36 Zn31 14_556 . 137.646(19)
Fe6 Zn36 Zn31 . . 59.144(12)
Fe6 Zn36 Zn31 14_556 14_556 59.144(12)
Fe6 Zn36 Zn31 . 14_556 137.646(19)
Zn31 Zn36 Zn31 . 14_556 78.50(2)
Fe6 Zn36 Zn33 14_556 6 54.431(8)
Fe6 Zn36 Zn33 . 6 112.491(14)
Zn31 Zn36 Zn33 . 6 146.771(6)
Zn31 Zn36 Zn33 14_556 6 102.698(9)
Fe6 Zn36 Zn33 14_556 . 112.491(13)
Fe6 Zn36 Zn33 . . 54.431(8)
Zn31 Zn36 Zn33 . . 102.697(9)
Zn31 Zn36 Zn33 14_556 . 146.771(6)
Zn33 Zn36 Zn33 6 . 93.996(17)
Fe6 Zn36 Zn33 14_556 14_556 54.431(8)
Fe6 Zn36 Zn33 . 14_556 112.491(13)
Zn31 Zn36 Zn33 . 14_556 146.771(6)
Zn31 Zn36 Zn33 14_556 14_556 102.698(9)
Zn33 Zn36 Zn33 6 14_556 66.091(14)
Zn33 Zn36 Zn33 . 14_556 58.331(11)
Fe6 Zn36 Zn33 14_556 17 112.491(14)
Fe6 Zn36 Zn33 . 17 54.431(8)
Zn31 Zn36 Zn33 . 17 102.697(9)
Zn31 Zn36 Zn33 14_556 17 146.771(6)
Zn33 Zn36 Zn33 6 17 58.331(11)
Zn33 Zn36 Zn33 . 17 66.091(14)
Zn33 Zn36 Zn33 14_556 17 93.996(17)
Fe6 Zn36 Zn32 14_556 3_665 61.547(9)
Fe6 Zn36 Zn32 . 3_665 124.188(10)
Zn31 Zn36 Zn32 . 3_665 96.049(14)
Zn31 Zn36 Zn32 14_556 3_665 56.033(9)
Zn33 Zn36 Zn32 6 3_665 60.529(8)
Zn33 Zn36 Zn32 . 3_665 153.032(17)
Zn33 Zn36 Zn32 14_556 3_665 112.319(10)
Zn33 Zn36 Zn32 17 3_665 91.118(10)
Fe6 Zn36 Zn32 14_556 16_665 124.188(10)
Fe6 Zn36 Zn32 . 16_665 61.547(9)
Zn31 Zn36 Zn32 . 16_665 56.033(9)
Zn31 Zn36 Zn32 14_556 16_665 96.049(14)
Zn33 Zn36 Zn32 6 16_665 91.118(10)
Zn33 Zn36 Zn32 . 16_665 112.319(10)
Zn33 Zn36 Zn32 14_556 16_665 153.032(17)
Zn33 Zn36 Zn32 17 16_665 60.529(8)
Zn32 Zn36 Zn32 3_665 16_665 63.309(18)
Fe6 Zn36 Zn32 14_556 20_455 124.188(10)
Fe6 Zn36 Zn32 . 20_455 61.547(9)
Zn31 Zn36 Zn32 . 20_455 56.033(9)
Zn31 Zn36 Zn32 14_556 20_455 96.049(14)
Zn33 Zn36 Zn32 6 20_455 153.032(17)
Zn33 Zn36 Zn32 . 20_455 60.529(8)
Zn33 Zn36 Zn32 14_556 20_455 91.118(10)
Zn33 Zn36 Zn32 17 20_455 112.319(10)
Zn32 Zn36 Zn32 3_665 20_455 145.96(2)
Zn32 Zn36 Zn32 16_665 20_455 106.130(19)
Fe6 Zn36 Zn32 14_556 7_455 61.547(9)
Fe6 Zn36 Zn32 . 7_455 124.188(10)
Zn31 Zn36 Zn32 . 7_455 96.049(14)
Zn31 Zn36 Zn32 14_556 7_455 56.033(9)
Zn33 Zn36 Zn32 6 7_455 112.319(10)
Zn33 Zn36 Zn32 . 7_455 91.118(10)
Zn33 Zn36 Zn32 14_556 7_455 60.529(8)
Zn33 Zn36 Zn32 17 7_455 153.032(17)
Zn32 Zn36 Zn32 3_665 7_455 106.130(19)
Zn32 Zn36 Zn32 16_665 7_455 145.96(2)
Zn32 Zn36 Zn32 20_455 7_455 63.309(18)
Zn37 Zn37 Fe7 7 1_545 177.973(10)
Zn37 Zn37 Zn33 7 12 123.287(9)
Fe7 Zn37 Zn33 1_545 12 58.335(9)
Zn37 Zn37 Zn33 7 23_556 123.287(9)
Fe7 Zn37 Zn33 1_545 23_556 58.335(9)
Zn33 Zn37 Zn33 12 23_556 60.769(13)
Zn37 Zn37 Zn37 7 17_655 120.0
Fe7 Zn37 Zn37 1_545 17_655 57.973(10)
Zn33 Zn37 Zn37 12 17_655 107.575(9)
Zn33 Zn37 Zn37 23_556 17_655 107.575(9)
Zn37 Zn37 Zn28 7 3_665 63.205(7)
Fe7 Zn37 Zn28 1_545 3_665 116.833(7)
Zn33 Zn37 Zn28 12 3_665 133.021(18)
Zn33 Zn37 Zn28 23_556 3_665 77.270(10)
Zn37 Zn37 Zn28 17_655 3_665 104.289(13)
Zn37 Zn37 Zn28 7 16_665 63.205(7)
Fe7 Zn37 Zn28 1_545 16_665 116.833(7)
Zn33 Zn37 Zn28 12 16_665 77.270(10)
Zn33 Zn37 Zn28 23_556 16_665 133.021(18)
Zn37 Zn37 Zn28 17_655 16_665 104.289(13)
Zn28 Zn37 Zn28 3_665 16_665 126.324(14)
Zn37 Zn37 Zn29 7 14_556 119.083(9)
Fe7 Zn37 Zn29 1_545 14_556 60.274(9)
Zn33 Zn37 Zn29 12 14_556 109.924(14)
Zn33 Zn37 Zn29 23_556 14_556 60.334(9)
Zn37 Zn37 Zn29 17_655 14_556 60.668(9)
Zn28 Zn37 Zn29 3_665 14_556 59.271(8)
Zn28 Zn37 Zn29 16_665 14_556 164.43(2)
Zn37 Zn37 Zn29 7 . 119.083(9)
Fe7 Zn37 Zn29 1_545 . 60.274(9)
Zn33 Zn37 Zn29 12 . 60.334(9)
Zn33 Zn37 Zn29 23_556 . 109.924(14)
Zn37 Zn37 Zn29 17_655 . 60.668(9)
Zn28 Zn37 Zn29 3_665 . 164.43(2)
Zn28 Zn37 Zn29 16_665 . 59.271(8)
Zn29 Zn37 Zn29 14_556 . 111.407(16)
Zn37 Zn37 Zn34 7 14_556 64.553(7)
Fe7 Zn37 Zn34 1_545 14_556 113.663(14)
Zn33 Zn37 Zn34 12 14_556 169.107(16)
Zn33 Zn37 Zn34 23_556 14_556 123.062(11)
Zn37 Zn37 Zn34 17_655 14_556 61.827(8)
Zn28 Zn37 Zn34 3_665 14_556 56.011(13)
Zn28 Zn37 Zn34 16_665 14_556 102.174(16)
Zn29 Zn37 Zn34 14_556 14_556 68.059(12)
Zn29 Zn37 Zn34 . 14_556 109.828(16)
Zn37 Zn37 Zn34 7 . 64.553(7)
Fe7 Zn37 Zn34 1_545 . 113.663(14)
Zn33 Zn37 Zn34 12 . 123.062(11)
Zn33 Zn37 Zn34 23_556 . 169.107(16)
Zn37 Zn37 Zn34 17_655 . 61.827(8)
Zn28 Zn37 Zn34 3_665 . 102.174(16)
Zn28 Zn37 Zn34 16_665 . 56.011(13)
Zn29 Zn37 Zn34 14_556 . 109.828(16)
Zn29 Zn37 Zn34 . . 68.059(12)
Zn34 Zn37 Zn34 14_556 . 51.12(2)
Zn38 Zn38 Zn38 20 16_665 60.000(2)
Zn38 Zn38 Zn39 20 16_665 121.33(4)
Zn38 Zn38 Zn39 16_665 16_665 148.25(3)
Zn38 Zn38 Zn39 20 12_665 148.25(3)
Zn38 Zn38 Zn39 16_665 12_665 121.32(4)
Zn39 Zn38 Zn39 16_665 12_665 38.60(6)
Zn38 Zn38 Zn10 20 . 123.66(2)
Zn38 Zn38 Zn10 16_665 . 123.66(2)
Zn39 Zn38 Zn10 16_665 . 83.63(4)
Zn39 Zn38 Zn10 12_665 . 83.63(4)
Zn38 Zn38 Zn39 20 9_655 50.73(4)
Zn38 Zn38 Zn39 16_665 9_655 102.62(4)
Zn39 Zn38 Zn39 16_665 9_655 70.60(6)
Zn39 Zn38 Zn39 12_665 9_655 103.34(4)
Zn10 Zn38 Zn39 . 9_655 120.77(3)
Zn38 Zn38 Zn39 20 20 102.62(4)
Zn38 Zn38 Zn39 16_665 20 50.73(4)
Zn39 Zn38 Zn39 16_665 20 103.34(4)
Zn39 Zn38 Zn39 12_665 20 70.60(6)
Zn10 Zn38 Zn39 . 20 120.77(3)
Zn39 Zn38 Zn39 9_655 20 116.77(5)
Zn38 Zn38 Fe4 20 . 85.52(2)
Zn38 Zn38 Fe4 16_665 . 85.52(2)
Zn39 Zn38 Fe4 16_665 . 63.82(3)
Zn39 Zn38 Fe4 12_665 . 63.82(3)
Zn10 Zn38 Fe4 . . 145.38(5)
Zn39 Zn38 Fe4 9_655 . 60.91(3)
Zn39 Zn38 Fe4 20 . 60.91(3)
Zn38 Zn38 Zn39 20 . 68.70(3)
Zn38 Zn38 Zn39 16_665 . 27.08(3)
Zn39 Zn38 Zn39 16_665 . 121.17(5)
Zn39 Zn38 Zn39 12_665 . 99.74(4)
Zn10 Zn38 Zn39 . . 143.65(3)
Zn39 Zn38 Zn39 9_655 . 93.90(4)
Zn39 Zn38 Zn39 20 . 33.92(5)
Fe4 Zn38 Zn39 . . 59.41(3)
Zn38 Zn38 Zn39 20 17_655 27.08(3)
Zn38 Zn38 Zn39 16_665 17_655 68.70(3)
Zn39 Zn38 Zn39 16_665 17_655 99.74(4)
Zn39 Zn38 Zn39 12_665 17_655 121.17(5)
Zn10 Zn38 Zn39 . 17_655 143.65(3)
Zn39 Zn38 Zn39 9_655 17_655 33.92(5)
Zn39 Zn38 Zn39 20 17_655 93.90(4)
Fe4 Zn38 Zn39 . 17_655 59.41(3)
Zn39 Zn38 Zn39 . 17_655 63.62(6)
Zn38 Zn38 Zn40 20 16_665 93.02(3)
Zn38 Zn38 Zn40 16_665 16_665 136.67(3)
Zn39 Zn38 Zn40 16_665 16_665 28.32(4)
Zn39 Zn38 Zn40 12_665 16_665 64.26(4)
Zn10 Zn38 Zn40 . 16_665 99.27(4)
Zn39 Zn38 Zn40 9_655 16_665 42.31(4)
Zn39 Zn38 Zn40 20 16_665 114.18(4)
Fe4 Zn38 Zn40 . 16_665 57.20(2)
Zn39 Zn38 Zn40 . 16_665 114.91(4)
Zn39 Zn38 Zn40 17_655 16_665 73.14(3)
Zn38 Zn38 Zn40 20 12_665 136.67(3)
Zn38 Zn38 Zn40 16_665 12_665 93.02(3)
Zn39 Zn38 Zn40 16_665 12_665 64.26(4)
Zn39 Zn38 Zn40 12_665 12_665 28.33(4)
Zn10 Zn38 Zn40 . 12_665 99.27(4)
Zn39 Zn38 Zn40 9_655 12_665 114.18(4)
Zn39 Zn38 Zn40 20 12_665 42.31(4)
Fe4 Zn38 Zn40 . 12_665 57.20(2)
Zn39 Zn38 Zn40 . 12_665 73.14(3)
Zn39 Zn38 Zn40 17_655 12_665 114.91(4)
Zn40 Zn38 Zn40 16_665 12_665 84.85(5)
Zn41 Zn39 Zn40 16_665 . 132.81(14)
Zn41 Zn39 Zn39 16_665 20 37.23(10)
Zn40 Zn39 Zn39 . 20 145.41(5)
Zn41 Zn39 Zn40 16_665 17_655 135.88(12)
Zn40 Zn39 Zn40 . 17_655 11.88(4)
Zn39 Zn39 Zn40 20 17_655 137.63(3)
Zn41 Zn39 Zn38 16_665 16_665 105.69(10)
Zn40 Zn39 Zn38 . 16_665 92.66(6)
Zn39 Zn39 Zn38 20 16_665 70.70(3)
Zn40 Zn39 Zn38 17_655 16_665 80.81(5)
Zn41 Zn39 Zn14 16_665 . 104.84(10)
Zn40 Zn39 Zn14 . . 105.39(6)
Zn39 Zn39 Zn14 20 . 109.14(3)
Zn40 Zn39 Zn14 17_655 . 111.30(5)
Zn38 Zn39 Zn14 16_665 . 115.67(5)
Zn41 Zn39 Zn38 16_665 20 111.07(10)
Zn40 Zn39 Zn38 . 20 84.72(6)
Zn39 Zn39 Zn38 20 20 77.38(4)
Zn40 Zn39 Zn38 17_655 20 72.87(5)
Zn38 Zn39 Zn38 16_665 20 7.95(4)
Zn14 Zn39 Zn38 . 20 118.27(4)
Zn41 Zn39 Zn43 16_665 . 46.12(11)
Zn40 Zn39 Zn43 . . 87.29(6)
Zn39 Zn39 Zn43 20 . 77.68(3)
Zn40 Zn39 Zn43 17_655 . 93.01(5)
Zn38 Zn39 Zn43 16_665 . 122.64(4)
Zn14 Zn39 Zn43 . . 119.49(4)
Zn38 Zn39 Zn43 20 . 121.73(4)
Zn41 Zn39 Fe4 16_665 . 77.36(9)
Zn40 Zn39 Fe4 . . 72.32(5)
Zn39 Zn39 Fe4 20 . 73.13(3)
Zn40 Zn39 Fe4 17_655 . 66.34(4)
Zn38 Zn39 Fe4 16_665 . 64.19(3)
Zn14 Zn39 Fe4 . . 177.63(6)
Zn38 Zn39 Fe4 20 . 61.24(3)
Zn43 Zn39 Fe4 . . 61.36(3)
Zn41 Zn39 Zn38 16_665 . 102.72(10)
Zn40 Zn39 Zn38 . . 92.26(6)
Zn39 Zn39 Zn38 20 . 68.70(3)
Zn40 Zn39 Zn38 17_655 . 80.38(4)
Zn38 Zn39 Zn38 16_665 . 4.67(2)
Zn14 Zn39 Zn38 . . 120.19(4)
Zn38 Zn39 Zn38 20 . 8.68(4)
Zn43 Zn39 Zn38 . . 117.98(4)
Fe4 Zn39 Zn38 . . 59.72(3)
Zn41 Zn39 Zn40 16_665 20 40.98(8)
Zn40 Zn39 Zn40 . 20 129.69(7)
Zn39 Zn39 Zn40 20 20 15.72(3)
Zn40 Zn39 Zn40 17_655 20 122.31(5)
Zn38 Zn39 Zn40 16_665 20 64.80(3)
Zn14 Zn39 Zn40 . 20 124.82(5)
Zn38 Zn39 Zn40 20 20 70.12(4)
Zn43 Zn39 Zn40 . 20 71.84(4)
Fe4 Zn39 Zn40 . 20 57.44(2)
Zn38 Zn39 Zn40 . 20 61.74(3)
Zn41 Zn39 Zn43 16_665 20 37.85(11)
Zn40 Zn39 Zn43 . 20 95.09(6)
Zn39 Zn39 Zn43 20 20 68.55(3)
Zn40 Zn39 Zn43 17_655 20 99.79(5)
Zn38 Zn39 Zn43 16_665 20 117.40(4)
Zn14 Zn39 Zn43 . 20 121.48(4)
Zn38 Zn39 Zn43 20 20 117.75(4)
Zn43 Zn39 Zn43 . 20 9.13(3)
Fe4 Zn39 Zn43 . 20 59.75(2)
Zn38 Zn39 Zn43 . 20 112.83(4)
Zn40 Zn39 Zn43 20 20 63.05(3)
Zn40 Zn40 Zn39 17_655 . 145.93(6)
Zn40 Zn40 Zn39 17_655 17_655 22.20(4)
Zn39 Zn40 Zn39 . 17_655 123.73(9)
Zn40 Zn40 Zn42 17_655 . 80.00(3)
Zn39 Zn40 Zn42 . . 119.22(7)
Zn39 Zn40 Zn42 17_655 . 94.10(5)
Zn40 Zn40 Zn41 17_655 16_665 147.71(3)
Zn39 Zn40 Zn41 . 16_665 20.02(7)
Zn39 Zn40 Zn41 17_655 16_665 128.41(6)
Zn42 Zn40 Zn41 . 16_665 99.35(6)
Zn40 Zn40 Zn44 17_655 . 96.54(4)
Zn39 Zn40 Zn44 . . 99.24(7)
Zn39 Zn40 Zn44 17_655 . 106.10(5)
Zn42 Zn40 Zn44 . . 20.04(4)
Zn41 Zn40 Zn44 16_665 . 79.32(6)
Zn40 Zn40 Fe4 17_655 . 82.16(2)
Zn39 Zn40 Fe4 . . 79.18(5)
Zn39 Zn40 Fe4 17_655 . 70.78(3)
Zn42 Zn40 Fe4 . . 70.47(4)
Zn41 Zn40 Fe4 16_665 . 67.60(4)
Zn44 Zn40 Fe4 . . 61.61(3)
Zn40 Zn40 Zn20 17_655 12 130.83(2)
Zn39 Zn40 Zn20 . 12 83.16(6)
Zn39 Zn40 Zn20 17_655 12 152.92(5)
Zn42 Zn40 Zn20 . 12 72.26(3)
Zn41 Zn40 Zn20 16_665 12 77.78(4)
Zn44 Zn40 Zn20 . 12 68.55(3)
Fe4 Zn40 Zn20 . 12 122.91(3)
Zn40 Zn40 Zn13 17_655 . 82.36(2)
Zn39 Zn40 Zn13 . . 85.36(6)
Zn39 Zn40 Zn13 17_655 . 75.42(4)
Zn42 Zn40 Zn13 . . 154.49(5)
Zn41 Zn40 Zn13 16_665 . 105.39(6)
Zn44 Zn40 Zn13 . . 172.82(4)
Fe4 Zn40 Zn13 . . 125.01(3)
Zn20 Zn40 Zn13 12 . 106.80(3)
Zn40 Zn40 Zn18 17_655 1_545 82.427(19)
Zn39 Zn40 Zn18 . 1_545 119.24(6)
Zn39 Zn40 Zn18 17_655 1_545 97.68(4)
Zn42 Zn40 Zn18 . 1_545 96.79(5)
Zn41 Zn40 Zn18 16_665 1_545 129.26(5)
Zn44 Zn40 Zn18 . 1_545 110.27(4)
Fe4 Zn40 Zn18 . 1_545 161.50(4)
Zn20 Zn40 Zn18 12 1_545 62.148(18)
Zn13 Zn40 Zn18 . 1_545 62.56(2)
Zn40 Zn40 Zn41 17_655 20 24.28(3)
Zn39 Zn40 Zn41 . 20 124.81(6)
Zn39 Zn40 Zn41 17_655 20 14.48(4)
Zn42 Zn40 Zn41 . 20 81.60(5)
Zn41 Zn40 Zn41 16_665 20 123.43(6)
Zn44 Zn40 Zn41 . 20 92.03(5)
Fe4 Zn40 Zn41 . 20 59.57(3)
Zn20 Zn40 Zn41 12 20 149.16(5)
Zn13 Zn40 Zn41 . 20 89.81(4)
Zn18 Zn40 Zn41 1_545 20 106.33(4)
Zn40 Zn40 Zn39 17_655 20 132.85(3)
Zn39 Zn40 Zn39 . 20 18.87(4)
Zn39 Zn40 Zn39 17_655 20 111.81(5)
Zn42 Zn40 Zn39 . 20 109.50(5)
Zn41 Zn40 Zn39 16_665 20 17.82(4)
Zn44 Zn40 Zn39 . 20 89.95(5)
Fe4 Zn40 Zn39 . 20 60.33(3)
Zn20 Zn40 Zn39 12 20 94.96(4)
Zn13 Zn40 Zn39 . 20 96.00(4)
Zn18 Zn40 Zn39 1_545 20 138.11(4)
Zn41 Zn40 Zn39 20 20 109.26(4)
Zn39 Zn41 Zn39 12_665 16_665 105.5(2)
Zn39 Zn41 Zn43 12_665 16_665 125.17(12)
Zn39 Zn41 Zn43 16_665 16_665 113.81(12)
Zn39 Zn41 Zn43 12_665 12_665 113.81(12)
Zn39 Zn41 Zn43 16_665 12_665 125.17(12)
Zn43 Zn41 Zn43 16_665 12_665 12.42(5)
Zn39 Zn41 Zn40 12_665 12_665 27.17(8)
Zn39 Zn41 Zn40 16_665 12_665 121.19(12)
Zn43 Zn41 Zn40 16_665 12_665 98.11(6)
Zn43 Zn41 Zn40 12_665 12_665 87.13(6)
Zn39 Zn41 Zn40 12_665 16_665 121.19(12)
Zn39 Zn41 Zn40 16_665 16_665 27.17(8)
Zn43 Zn41 Zn40 16_665 16_665 87.13(6)
Zn43 Zn41 Zn40 12_665 16_665 98.11(6)
Zn40 Zn41 Zn40 12_665 16_665 124.25(7)
Zn39 Zn41 Zn19 12_665 . 117.73(8)
Zn39 Zn41 Zn19 16_665 . 117.73(8)
Zn43 Zn41 Zn19 16_665 . 75.27(5)
Zn43 Zn41 Zn19 12_665 . 75.27(5)
Zn40 Zn41 Zn19 12_665 . 117.49(4)
Zn40 Zn41 Zn19 16_665 . 117.49(4)
Zn39 Zn41 Fe4 12_665 . 81.51(8)
Zn39 Zn41 Fe4 16_665 . 81.51(8)
Zn43 Zn41 Fe4 16_665 . 68.79(5)
Zn43 Zn41 Fe4 12_665 . 68.79(5)
Zn40 Zn41 Fe4 12_665 . 65.37(4)
Zn40 Zn41 Fe4 16_665 . 65.37(4)
Zn19 Zn41 Fe4 . . 143.84(8)
Zn39 Zn41 Zn40 12_665 20 29.64(9)
Zn39 Zn41 Zn40 16_665 20 114.96(11)
Zn43 Zn41 Zn40 16_665 20 97.19(5)
Zn43 Zn41 Zn40 12_665 20 87.12(5)
Zn40 Zn41 Zn40 12_665 20 8.01(2)
Zn40 Zn41 Zn40 16_665 20 116.31(6)
Zn19 Zn41 Zn40 . 20 125.05(3)
Fe4 Zn41 Zn40 . 20 57.97(3)
Zn39 Zn41 Zn40 12_665 9_655 114.96(11)
Zn39 Zn41 Zn40 16_665 9_655 29.64(9)
Zn43 Zn41 Zn40 16_665 9_655 87.12(5)
Zn43 Zn41 Zn40 12_665 9_655 97.19(5)
Zn40 Zn41 Zn40 12_665 9_655 116.31(6)
Zn40 Zn41 Zn40 16_665 9_655 8.01(2)
Zn19 Zn41 Zn40 . 9_655 125.05(3)
Fe4 Zn41 Zn40 . 9_655 57.97(3)
Zn40 Zn41 Zn40 20 9_655 108.35(5)
Zn39 Zn41 Zn38 12_665 . 54.55(9)
Zn39 Zn41 Zn38 16_665 . 54.55(9)
Zn43 Zn41 Zn38 16_665 . 127.74(6)
Zn43 Zn41 Zn38 12_665 . 127.74(6)
Zn40 Zn41 Zn38 12_665 . 66.75(4)
Zn40 Zn41 Zn38 16_665 . 66.75(4)
Zn19 Zn41 Zn38 . . 156.81(7)
Fe4 Zn41 Zn38 . . 59.35(3)
Zn40 Zn41 Zn38 20 . 61.09(3)
Zn40 Zn41 Zn38 9_655 . 61.09(3)
Zn39 Zn41 Zn14 12_665 12_665 55.81(8)
Zn39 Zn41 Zn14 16_665 12_665 108.62(13)
Zn43 Zn41 Zn14 16_665 12_665 133.51(5)
Zn43 Zn41 Zn14 12_665 12_665 124.66(4)
Zn40 Zn41 Zn14 12_665 12_665 74.58(4)
Zn40 Zn41 Zn14 16_665 12_665 135.44(8)
Zn19 Zn41 Zn14 . 12_665 68.75(3)
Fe4 Zn41 Zn14 . 12_665 137.32(4)
Zn40 Zn41 Zn14 20 12_665 81.03(3)
Zn40 Zn41 Zn14 9_655 12_665 137.86(7)
Zn38 Zn41 Zn14 . 12_665 92.17(5)
Zn44 Zn42 Zn44 . 17_655 85.6(2)
Zn44 Zn42 Zn40 . . 112.66(12)
Zn44 Zn42 Zn40 17_655 . 128.39(12)
Zn44 Zn42 Zn40 . 17_655 128.39(12)
Zn44 Zn42 Zn40 17_655 17_655 112.66(12)
Zn40 Zn42 Zn40 . 17_655 19.99(5)
Zn44 Zn42 Zn43 . 17_655 109.64(11)
Zn44 Zn42 Zn43 17_655 17_655 31.72(9)
Zn40 Zn42 Zn43 . 17_655 98.82(6)
Zn40 Zn42 Zn43 17_655 17_655 81.38(5)
Zn44 Zn42 Zn43 . . 31.72(9)
Zn44 Zn42 Zn43 17_655 . 109.64(11)
Zn40 Zn42 Zn43 . . 81.38(5)
Zn40 Zn42 Zn43 17_655 . 98.82(6)
Zn43 Zn42 Zn43 17_655 . 121.77(6)
Zn44 Zn42 Zn24 . 1_545 107.07(10)
Zn44 Zn42 Zn24 17_655 1_545 107.07(10)
Zn40 Zn42 Zn24 . 1_545 111.95(7)
Zn40 Zn42 Zn24 17_655 1_545 111.95(7)
Zn43 Zn42 Zn24 17_655 1_545 116.71(3)
Zn43 Zn42 Zn24 . 1_545 116.71(3)
Zn44 Zn42 Zn43 . 9_655 106.07(10)
Zn44 Zn42 Zn43 17_655 9_655 31.72(9)
Zn40 Zn42 Zn43 . 9_655 97.51(5)
Zn40 Zn42 Zn43 17_655 9_655 80.95(4)
Zn43 Zn42 Zn43 17_655 9_655 4.856(18)
Zn43 Zn42 Zn43 . 9_655 116.99(5)
Zn24 Zn42 Zn43 1_545 9_655 121.40(3)
Zn44 Zn42 Zn43 . 20 31.72(9)
Zn44 Zn42 Zn43 17_655 20 106.07(10)
Zn40 Zn42 Zn43 . 20 80.95(4)
Zn40 Zn42 Zn43 17_655 20 97.51(5)
Zn43 Zn42 Zn43 17_655 20 116.99(5)
Zn43 Zn42 Zn43 . 20 4.856(18)
Zn24 Zn42 Zn43 1_545 20 121.40(3)
Zn43 Zn42 Zn43 9_655 20 112.20(5)
Zn44 Zn42 Fe4 . . 75.57(8)
Zn44 Zn42 Fe4 17_655 . 75.57(8)
Zn40 Zn42 Fe4 . . 64.39(4)
Zn40 Zn42 Fe4 17_655 . 64.38(4)
Zn43 Zn42 Fe4 17_655 . 64.13(3)
Zn43 Zn42 Fe4 . . 64.13(3)
Zn24 Zn42 Fe4 1_545 . 176.26(8)
Zn43 Zn42 Fe4 9_655 . 59.54(3)
Zn43 Zn42 Fe4 20 . 59.54(3)
Zn44 Zn42 Zn45 . . 44.39(9)
Zn44 Zn42 Zn45 17_655 . 44.39(9)
Zn40 Zn42 Zn45 . . 120.40(6)
Zn40 Zn42 Zn45 17_655 . 120.40(6)
Zn43 Zn42 Zn45 17_655 . 65.27(4)
Zn43 Zn42 Zn45 . . 65.27(4)
Zn24 Zn42 Zn45 1_545 . 126.78(7)
Zn43 Zn42 Zn45 9_655 . 61.88(3)
Zn43 Zn42 Zn45 20 . 61.88(3)
Fe4 Zn42 Zn45 . . 56.96(3)
Zn44 Zn42 Zn20 . 12 88.45(8)
Zn44 Zn42 Zn20 17_655 12 168.30(15)
Zn40 Zn42 Zn20 . 12 63.27(4)
Zn40 Zn42 Zn20 17_655 12 78.89(5)
Zn43 Zn42 Zn20 17_655 12 158.98(8)
Zn43 Zn42 Zn20 . 12 68.84(2)
Zn24 Zn42 Zn20 1_545 12 65.20(2)
Zn43 Zn42 Zn20 9_655 12 159.70(7)
Zn43 Zn42 Zn20 20 12 73.03(2)
Fe4 Zn42 Zn20 . 12 112.61(4)
Zn45 Zn42 Zn20 . 12 132.17(2)
Zn43 Zn43 Zn44 20 . 143.25(4)
Zn43 Zn43 Zn44 20 20 28.99(4)
Zn44 Zn43 Zn44 . 20 114.26(7)
Zn43 Zn43 Zn41 20 16_665 83.79(2)
Zn44 Zn43 Zn41 . 16_665 109.78(5)
Zn44 Zn43 Zn41 20 16_665 96.28(4)
Zn43 Zn43 Zn42 20 . 148.83(3)
Zn44 Zn43 Zn42 . . 18.30(6)
Zn44 Zn43 Zn42 20 . 122.32(5)
Zn41 Zn43 Zn42 16_665 . 91.95(6)
Zn43 Zn43 Zn26 20 . 127.549(19)
Zn44 Zn43 Zn26 . . 70.36(4)
Zn44 Zn43 Zn26 20 . 131.03(4)
Zn41 Zn43 Zn26 16_665 . 129.43(4)
Zn42 Zn43 Zn26 . . 78.12(4)
Zn43 Zn43 Zn39 20 . 102.32(3)
Zn44 Zn43 Zn39 . . 90.17(5)
Zn44 Zn43 Zn39 20 . 109.11(5)
Zn41 Zn43 Zn39 16_665 . 20.06(3)
Zn42 Zn43 Zn39 . . 72.11(6)
Zn26 Zn43 Zn39 . . 119.77(4)
Zn43 Zn43 Fe4 20 . 85.278(17)
Zn44 Zn43 Fe4 . . 70.87(4)
Zn44 Zn43 Fe4 20 . 66.99(3)
Zn41 Zn43 Fe4 16_665 . 66.04(4)
Zn42 Zn43 Fe4 . . 65.01(3)
Zn26 Zn43 Fe4 . . 141.23(4)
Zn39 Zn43 Fe4 . . 60.70(3)
Zn43 Zn43 Zn42 20 20 26.31(3)
Zn44 Zn43 Zn42 . 20 119.50(5)
Zn44 Zn43 Zn42 20 20 14.74(5)
Zn41 Zn43 Zn42 16_665 20 81.54(5)
Zn42 Zn43 Zn42 . 20 122.52(5)
Zn26 Zn43 Zn42 . 20 144.75(5)
Zn39 Zn43 Zn42 . 20 94.84(5)
Fe4 Zn43 Zn42 . 20 60.26(3)
Zn43 Zn43 Zn39 20 20 68.55(3)
Zn44 Zn43 Zn39 . 20 117.29(5)
Zn44 Zn43 Zn39 20 20 79.30(5)
Zn41 Zn43 Zn39 16_665 20 16.98(3)
Zn42 Zn43 Zn39 . 20 101.19(5)
Zn26 Zn43 Zn39 . 20 145.05(4)
Zn39 Zn43 Zn39 . 20 33.76(5)
Fe4 Zn43 Zn39 . 20 59.13(2)
Zn42 Zn43 Zn39 20 20 64.57(5)
Zn43 Zn43 Zn45 20 . 91.90(3)
Zn44 Zn43 Zn45 . . 51.78(5)
Zn44 Zn43 Zn45 20 . 63.21(4)
Zn41 Zn43 Zn45 16_665 . 123.07(5)
Zn42 Zn43 Zn45 . . 64.73(4)
Zn26 Zn43 Zn45 . . 97.29(3)
Zn39 Zn43 Zn45 . . 114.24(4)
Fe4 Zn43 Zn45 . . 57.04(3)
Zn42 Zn43 Zn45 20 . 71.84(4)
Zn39 Zn43 Zn45 20 . 114.21(4)
Zn43 Zn43 Zn44 20 17_655 133.57(3)
Zn44 Zn43 Zn44 . 17_655 13.32(3)
Zn44 Zn43 Zn44 20 17_655 105.19(5)
Zn41 Zn43 Zn44 16_665 17_655 102.36(4)
Zn42 Zn43 Zn44 . 17_655 18.74(4)
Zn26 Zn43 Zn44 . 17_655 83.65(3)
Zn39 Zn43 Zn44 . 17_655 83.99(4)
Fe4 Zn43 Zn44 . 17_655 57.58(3)
Zn42 Zn43 Zn44 20 17_655 108.18(4)
Zn39 Zn43 Zn44 20 17_655 107.00(4)
Zn45 Zn43 Zn44 . 17_655 46.00(3)
Zn42 Zn44 Zn44 . 17_655 47.22(10)
Zn42 Zn44 Zn43 . . 129.98(13)
Zn44 Zn44 Zn43 17_655 . 150.19(4)
Zn42 Zn44 Zn43 . 20 133.54(13)
Zn44 Zn44 Zn43 17_655 20 144.66(3)
Zn43 Zn44 Zn43 . 20 7.75(3)
Zn42 Zn44 Zn45 . . 117.71(11)
Zn44 Zn44 Zn45 17_655 . 72.64(4)
Zn43 Zn44 Zn45 . . 92.91(6)
Zn43 Zn44 Zn45 20 . 85.28(5)
Zn42 Zn44 Zn26 . . 117.66(9)
Zn44 Zn44 Zn26 17_655 . 136.24(3)
Zn43 Zn44 Zn26 . . 73.48(5)
Zn43 Zn44 Zn26 20 . 78.25(5)
Zn45 Zn44 Zn26 . . 116.59(5)
Zn42 Zn44 Zn40 . . 47.30(11)
Zn44 Zn44 Zn40 17_655 . 83.46(4)
Zn43 Zn44 Zn40 . . 83.19(5)
Zn43 Zn44 Zn40 20 . 86.25(5)
Zn45 Zn44 Zn40 . . 123.22(5)
Zn26 Zn44 Zn40 . . 116.22(4)
Zn42 Zn44 Zn45 . 20 125.13(10)
Zn44 Zn44 Zn45 17_655 20 82.53(4)
Zn43 Zn44 Zn45 . 20 81.21(6)
Zn43 Zn44 Zn45 20 20 73.55(5)
Zn45 Zn44 Zn45 . 20 11.80(4)
Zn26 Zn44 Zn45 . 20 114.03(4)
Zn40 Zn44 Zn45 . 20 119.76(4)
Zn42 Zn44 Fe4 . . 84.01(9)
Zn44 Zn44 Fe4 17_655 . 75.84(3)
Zn43 Zn44 Fe4 . . 74.40(4)
Zn43 Zn44 Fe4 20 . 69.77(4)
Zn45 Zn44 Fe4 . . 64.62(4)
Zn26 Zn44 Fe4 . . 147.87(6)
Zn40 Zn44 Fe4 . . 59.81(3)
Zn45 Zn44 Fe4 20 . 59.94(3)
Zn42 Zn44 Zn45 . 16_665 112.73(10)
Zn44 Zn44 Zn45 17_655 16_665 69.32(3)
Zn43 Zn44 Zn45 . 16_665 93.20(5)
Zn43 Zn44 Zn45 20 16_665 85.46(5)
Zn45 Zn44 Zn45 . 16_665 7.07(2)
Zn26 Zn44 Zn45 . 16_665 123.42(4)
Zn40 Zn44 Zn45 . 16_665 116.23(4)
Zn45 Zn44 Zn45 20 16_665 13.21(4)
Fe4 Zn44 Zn45 . 16_665 58.06(3)
Zn42 Zn44 Zn40 . 17_655 35.79(10)
Zn44 Zn44 Zn40 17_655 17_655 68.55(3)
Zn43 Zn44 Zn40 . 17_655 96.52(5)
Zn43 Zn44 Zn40 20 17_655 98.62(5)
Zn45 Zn44 Zn40 . 17_655 115.85(4)
Zn26 Zn44 Zn40 . 17_655 126.94(4)
Zn40 Zn44 Zn40 . 17_655 14.91(4)
Zn45 Zn44 Zn40 20 17_655 115.55(4)
Fe4 Zn44 Zn40 . 17_655 57.70(3)
Zn45 Zn44 Zn40 16_665 17_655 108.82(4)
Zn42 Zn44 Zn43 . 17_655 51.62(8)
Zn44 Zn44 Zn43 17_655 17_655 16.49(3)
Zn43 Zn44 Zn43 . 17_655 133.70(6)
Zn43 Zn44 Zn43 20 17_655 128.35(5)
Zn45 Zn44 Zn43 . 17_655 66.11(3)
Zn26 Zn44 Zn43 . 17_655 152.62(6)
Zn40 Zn44 Zn43 . 17_655 76.50(4)
Zn45 Zn44 Zn43 20 17_655 73.96(4)
Fe4 Zn44 Zn43 . 17_655 59.38(2)
Zn45 Zn44 Zn43 16_665 17_655 61.20(3)
Zn40 Zn44 Zn43 17_655 17_655 62.16(3)
Zn45 Zn45 Zn45 16_665 20 60.0000(10)
Zn45 Zn45 Zn44 16_665 17_655 123.18(4)
Zn45 Zn45 Zn44 20 17_655 147.74(3)
Zn45 Zn45 Zn44 16_665 . 147.74(3)
Zn45 Zn45 Zn44 20 . 123.18(4)
Zn44 Zn45 Zn44 17_655 . 34.72(8)
Zn45 Zn45 Zn44 16_665 9_655 45.02(4)
Zn45 Zn45 Zn44 20 9_655 97.47(4)
Zn44 Zn45 Zn44 17_655 9_655 78.16(7)
Zn44 Zn45 Zn44 . 9_655 107.11(5)
Zn45 Zn45 Zn44 16_665 20 97.47(4)
Zn45 Zn45 Zn44 20 20 45.02(4)
Zn44 Zn45 Zn44 17_655 20 107.11(5)
Zn44 Zn45 Zn44 . 20 78.16(7)
Zn44 Zn45 Zn44 9_655 20 113.62(6)
Zn45 Zn45 Fe4 16_665 . 83.09(2)
Zn45 Zn45 Fe4 20 . 83.09(2)
Zn44 Zn45 Fe4 17_655 . 66.59(4)
Zn44 Zn45 Fe4 . . 66.59(4)
Zn44 Zn45 Fe4 9_655 . 61.54(3)
Zn44 Zn45 Fe4 20 . 61.54(3)
Zn45 Zn45 Zn34 16_665 . 83.09(2)
Zn45 Zn45 Zn34 20 . 83.09(2)
Zn44 Zn45 Zn34 17_655 . 128.37(5)
Zn44 Zn45 Zn34 . . 128.37(5)
Zn44 Zn45 Zn34 9_655 . 112.58(3)
Zn44 Zn45 Zn34 20 . 112.58(3)
Fe4 Zn45 Zn34 . . 164.03(5)
Zn45 Zn45 Zn28 16_665 20 83.18(2)
Zn45 Zn45 Zn28 20 20 132.97(2)
Zn44 Zn45 Zn28 17_655 20 76.04(4)
Zn44 Zn45 Zn28 . 20 103.68(5)
Zn44 Zn45 Zn28 9_655 20 69.95(2)
Zn44 Zn45 Zn28 20 20 175.49(4)
Fe4 Zn45 Zn28 . 20 122.96(2)
Zn34 Zn45 Zn28 . 20 63.02(2)
Zn45 Zn45 Zn28 16_665 16_665 132.97(2)
Zn45 Zn45 Zn28 20 16_665 83.18(2)
Zn44 Zn45 Zn28 17_655 16_665 103.68(5)
Zn44 Zn45 Zn28 . 16_665 76.04(4)
Zn44 Zn45 Zn28 9_655 16_665 175.49(4)
Zn44 Zn45 Zn28 20 16_665 69.95(2)
Fe4 Zn45 Zn28 . 16_665 122.96(2)
Zn34 Zn45 Zn28 . 16_665 63.02(2)
Zn28 Zn45 Zn28 20 16_665 106.33(4)
Zn45 Zn45 Zn44 16_665 16_665 25.19(3)
Zn45 Zn45 Zn44 20 16_665 69.32(3)
Zn44 Zn45 Zn44 17_655 16_665 102.05(4)
Zn44 Zn45 Zn44 . 16_665 122.55(6)
Zn44 Zn45 Zn44 9_655 16_665 28.15(6)
Zn44 Zn45 Zn44 20 16_665 92.39(4)
Fe4 Zn45 Zn44 . 16_665 59.54(3)
Zn34 Zn45 Zn44 . 16_665 107.76(4)
Zn28 Zn45 Zn44 20 16_665 90.05(3)
Zn28 Zn45 Zn44 16_665 16_665 152.14(5)
Zn45 Zn45 Zn44 16_665 12_665 69.32(3)
Zn45 Zn45 Zn44 20 12_665 25.19(3)
Zn44 Zn45 Zn44 17_655 12_665 122.55(6)
Zn44 Zn45 Zn44 . 12_665 102.05(4)
Zn44 Zn45 Zn44 9_655 12_665 92.39(4)
Zn44 Zn45 Zn44 20 12_665 28.15(6)
Fe4 Zn45 Zn44 . 12_665 59.54(3)
Zn34 Zn45 Zn44 . 12_665 107.76(4)
Zn28 Zn45 Zn44 20 12_665 152.14(5)
Zn28 Zn45 Zn44 16_665 12_665 90.05(3)
Zn44 Zn45 Zn44 16_665 12_665 66.97(7)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Fe1 Zn7 . 2.5313(3)
Fe1 Zn7 16 2.5312(3)
Fe1 Zn7 20 2.5312(3)
Fe1 Zn7 13 2.5313(3)
Fe1 Zn7 4 2.5313(3)
Fe1 Zn7 8 2.5313(3)
Fe1 Zn2 4_445 2.5561(2)
Fe1 Zn2 13_665 2.5561(2)
Fe1 Zn2 16_665 2.5561(2)
Fe1 Zn2 8_655 2.5561(2)
Fe1 Zn2 1_445 2.5561(2)
Fe1 Zn2 20_455 2.5561(2)
Fe2 Zn2 . 2.4444(4)
Fe2 Zn4 . 2.5369(3)
Fe2 Zn5 13_665 2.5871(4)
Fe2 Zn8 16_665 2.6130(3)
Fe2 Zn8 12_665 2.6130(3)
Fe2 Zn1 8_665 2.65869(15)
Fe2 Zn1 16_665 2.65869(15)
Fe2 Zn10 . 2.6630(5)
Fe2 Zn6 16_665 2.7161(3)
Fe2 Zn6 20 2.7161(3)
Fe2 Zn3 4 2.7821(4)
Fe2 Zn3 8_655 2.7821(4)
Fe3 Zn7 . 2.4425(4)
Fe3 Zn16 . 2.5329(4)
Fe3 Zn11 17 2.5727(3)
Fe3 Zn11 . 2.5727(3)
Fe3 Zn17 . 2.5899(4)
Fe3 Zn12 16_665 2.6278(2)
Fe3 Zn12 20_455 2.6278(2)
Fe3 Zn14 20 2.6568(3)
Fe3 Zn14 9 2.6568(3)
Fe3 Zn8 9 2.6757(2)
Fe3 Zn8 20 2.6757(3)
Fe3 Zn5 . 2.7048(4)
Fe4 Zn40 17_655 2.5343(7)
Fe4 Zn40 . 2.5343(7)
Fe4 Zn40 9_655 2.5343(7)
Fe4 Zn40 16_665 2.5343(7)
Fe4 Zn40 20 2.5343(7)
Fe4 Zn40 12_665 2.5343(7)
Fe4 Zn45 16_665 2.5393(10)
Fe4 Zn45 . 2.5393(10)
Fe4 Zn45 20 2.5393(10)
Fe4 Zn41 20 2.5776(11)
Fe4 Zn41 16_665 2.5776(11)
Fe4 Zn41 . 2.5776(11)
Fe5 Zn22 20_565 2.5572(5)
Fe5 Zn22 . 2.5572(5)
Fe5 Zn22 16_665 2.5572(5)
Fe5 Zn30 . 2.5666(4)
Fe5 Zn30 16_665 2.5666(4)
Fe5 Zn30 20_565 2.5666(4)
Fe5 Zn27 20_565 2.6124(3)
Fe5 Zn27 16_665 2.6124(3)
Fe5 Zn27 . 2.6124(3)
Fe5 Zn24 16_665 2.6616(4)
Fe5 Zn24 . 2.6616(4)
Fe5 Zn24 20_565 2.6616(4)
Fe6 Zn33 17 2.4899(3)
Fe6 Zn33 . 2.4899(3)
Fe6 Zn27 . 2.5639(4)
Fe6 Zn25 16_665 2.5784(3)
Fe6 Zn25 20_455 2.5784(3)
Fe6 Zn26 20 2.6595(3)
Fe6 Zn26 9 2.6595(3)
Fe6 Zn36 . 2.6638(3)
Fe6 Zn31 . 2.6665(3)
Fe6 Zn23 . 2.6965(5)
Fe6 Zn32 16_665 2.8040(3)
Fe6 Zn32 20_455 2.8040(3)
Fe7 Zn33 12_565 2.5677(2)
Fe7 Zn33 23_566 2.5677(2)
Fe7 Zn33 3_665 2.5677(2)
Fe7 Zn33 16_665 2.5677(2)
Fe7 Zn35 7_565 2.5762(3)
Fe7 Zn35 3_665 2.5762(3)
Fe7 Zn30 14_556 2.5843(3)
Fe7 Zn30 . 2.5843(3)
Fe7 Zn37 17_665 2.5916(5)
Fe7 Zn37 1_565 2.5916(4)
Fe7 Zn29 14_566 2.7161(4)
Fe7 Zn29 1_565 2.7161(4)
Zn1 Fe2 16_665 2.65869(15)
Zn1 Fe2 8_655 2.65870(15)
Zn1 Zn6 . 2.7253(3)
Zn1 Zn6 13_655 2.7253(3)
Zn1 Zn3 13_665 2.7746(3)
Zn1 Zn3 1_545 2.7746(3)
Zn1 Zn8 . 2.7780(3)
Zn1 Zn8 5 2.7780(3)
Zn1 Zn2 8_655 2.8170(3)
Zn1 Zn2 16_665 2.8170(3)
Zn1 Zn5 20 2.8306(2)
Zn1 Zn5 4 2.8306(2)
Zn2 Fe1 1_665 2.5561(2)
Zn2 Zn7 13_665 2.6324(4)
Zn2 Zn7 20_665 2.6671(3)
Zn2 Zn7 16_665 2.6671(3)
Zn2 Zn2 4 2.6847(3)
Zn2 Zn2 8_765 2.6847(3)
Zn2 Zn8 12_665 2.7444(3)
Zn2 Zn8 16_665 2.7444(3)
Zn2 Zn5 13_665 2.7485(4)
Zn2 Zn1 8_665 2.8170(3)
Zn2 Zn1 16_665 2.8170(3)
Zn3 Zn9 . 2.6648(5)
Zn3 Zn6 13_665 2.7214(5)
Zn3 Zn4 13_665 2.7400(6)
Zn3 Zn1 13_665 2.7746(3)
Zn3 Zn1 1_565 2.7746(3)
Zn3 Fe2 4 2.7821(4)
Zn3 Fe2 8_665 2.7821(4)
Zn3 Zn5 16_665 2.7927(3)
Zn3 Zn5 20_565 2.7927(3)
Zn3 Zn3 20_565 2.9423(7)
Zn3 Zn3 16_665 2.9423(7)
Zn4 Fe2 20 2.5369(3)
Zn4 Fe2 16_665 2.5369(3)
Zn4 Zn6 16_665 2.6828(4)
Zn4 Zn6 . 2.6828(4)
Zn4 Zn6 20 2.6828(4)
Zn4 Zn3 13_665 2.7400(6)
Zn4 Zn3 4 2.7400(6)
Zn4 Zn3 8_655 2.7400(6)
Zn4 Zn10 20 2.7997(7)
Zn4 Zn10 . 2.7997(7)
Zn4 Zn10 16_665 2.7997(7)
Zn5 Fe2 13_665 2.5871(4)
Zn5 Zn11 17 2.6800(4)
Zn5 Zn11 . 2.6800(4)
Zn5 Zn2 13_665 2.7485(4)
Zn5 Zn7 . 2.7912(4)
Zn5 Zn3 16_665 2.7927(3)
Zn5 Zn3 20_565 2.7927(3)
Zn5 Zn1 20 2.8306(2)
Zn5 Zn1 4 2.8306(2)
Zn5 Zn8 20 2.8371(3)
Zn5 Zn8 9 2.8371(3)
Zn6 Zn13 . 2.6824(5)
Zn6 Fe2 16_665 2.7161(3)
Zn6 Fe2 20 2.7161(3)
Zn6 Zn3 13_665 2.7214(5)
Zn6 Zn1 13_655 2.7253(3)
Zn6 Zn8 . 2.8315(3)
Zn6 Zn8 17_655 2.8315(3)
Zn6 Zn10 20 2.9147(4)
Zn6 Zn10 16_665 2.9147(4)
Zn7 Zn2 13_665 2.6324(4)
Zn7 Zn2 20_455 2.6671(3)
Zn7 Zn2 16_665 2.6671(3)
Zn7 Zn12 16_665 2.6980(4)
Zn7 Zn12 20_455 2.6980(4)
Zn7 Zn7 16 2.7212(5)
Zn7 Zn7 20 2.7212(5)
Zn7 Zn8 9 2.7772(3)
Zn7 Zn8 20 2.7772(3)
Zn8 Fe2 16_665 2.6130(3)
Zn8 Zn11 12 2.6563(3)
Zn8 Fe3 20 2.6757(2)
Zn8 Zn10 16_665 2.7067(4)
Zn8 Zn14 . 2.7164(3)
Zn8 Zn2 16_665 2.7444(3)
Zn8 Zn7 20 2.7772(3)
Zn8 Zn12 16_665 2.8357(4)
Zn8 Zn5 20 2.8371(3)
Zn8 Zn8 20 2.9081(5)
Zn9 Zn3 16_665 2.6648(5)
Zn9 Zn3 20_565 2.6648(5)
Zn9 Zn15 . 2.6712(9)
Zn9 Zn11 20_565 2.7422(3)
Zn9 Zn11 12_565 2.7422(3)
Zn9 Zn11 16_665 2.7422(3)
Zn9 Zn11 . 2.7422(3)
Zn9 Zn11 9_665 2.7422(3)
Zn9 Zn11 17 2.7422(3)
Zn10 Zn38 . 2.4853(10)
Zn10 Zn13 20 2.6668(3)
Zn10 Zn13 16_665 2.6668(3)
Zn10 Zn8 12_665 2.7067(4)
Zn10 Zn8 16_665 2.7067(4)
Zn10 Zn38 16_665 2.7338(9)
Zn10 Zn38 20 2.7338(9)
Zn10 Zn6 20 2.9147(4)
Zn10 Zn6 16_665 2.9147(4)
Zn10 Zn14 12_665 3.1218(5)
Zn11 Zn11 20_565 2.4710(4)
Zn11 Zn8 9 2.6563(3)
Zn11 Zn11 17 2.6915(5)
Zn11 Zn13 16_565 2.7158(4)
Zn11 Zn16 . 2.7165(5)
Zn11 Zn14 9 2.7895(4)
Zn11 Zn18 16_665 2.9064(4)
Zn11 Zn15 . 3.1179(5)
Zn12 Fe3 16_665 2.6278(2)
Zn12 Fe3 20_665 2.6278(2)
Zn12 Zn14 12_665 2.6944(4)
Zn12 Zn14 16_665 2.6944(4)
Zn12 Zn7 16_665 2.6980(4)
Zn12 Zn7 20_665 2.6980(4)
Zn12 Zn17 16_665 2.7426(4)
Zn12 Zn17 20_665 2.7426(4)
Zn12 Zn12 20_565 2.8330(6)
Zn12 Zn12 16_775 2.8330(6)
Zn12 Zn8 12_665 2.8357(4)
Zn12 Zn8 16_665 2.8357(4)
Zn13 Zn40 17_655 2.6020(9)
Zn13 Zn40 . 2.6020(9)
Zn13 Zn10 20 2.6668(3)
Zn13 Zn10 16_665 2.6668(3)
Zn13 Zn18 1_545 2.7137(5)
Zn13 Zn11 16_655 2.7158(4)
Zn13 Zn11 12 2.7158(4)
Zn13 Zn14 17_655 2.7533(3)
Zn13 Zn14 . 2.7533(3)
Zn13 Zn39 17_655 2.8014(10)
Zn13 Zn39 . 2.8014(10)
Zn14 Zn39 . 2.3774(8)
Zn14 Fe3 20 2.6568(3)
Zn14 Zn12 16_665 2.6944(4)
Zn14 Zn20 12 2.7508(4)
Zn14 Zn17 20 2.7760(4)
Zn14 Zn41 16_665 2.7781(12)
Zn14 Zn16 20 2.7831(4)
Zn14 Zn11 12 2.7895(4)
Zn14 Zn19 16_665 2.9603(5)
Zn14 Zn40 . 2.9776(9)
Zn15 Zn18 . 2.7446(4)
Zn15 Zn18 16_665 2.7446(4)
Zn15 Zn18 20_565 2.7446(4)
Zn15 Zn16 20_565 2.9309(4)
Zn15 Zn16 16_665 2.9309(5)
Zn15 Zn16 . 2.9309(5)
Zn15 Zn22 20_565 3.0503(7)
Zn15 Zn22 16_665 3.0503(7)
Zn15 Zn22 . 3.0503(7)
Zn15 Zn11 20_565 3.1179(5)
Zn16 Zn22 . 2.4930(5)
Zn16 Zn17 . 2.6810(6)
Zn16 Zn11 17 2.7165(5)
Zn16 Zn18 16_665 2.7788(3)
Zn16 Zn18 20_565 2.7788(3)
Zn16 Zn14 9 2.7831(4)
Zn16 Zn14 20 2.7831(4)
Zn16 Zn20 . 2.7931(4)
Zn16 Zn20 17 2.7931(4)
Zn17 Zn21 . 2.5782(5)
Zn17 Zn12 16_665 2.7426(4)
Zn17 Zn12 20_455 2.7426(4)
Zn17 Zn19 20_455 2.7440(4)
Zn17 Zn19 16_665 2.7440(4)
Zn17 Zn14 20 2.7760(4)
Zn17 Zn14 9 2.7760(4)
Zn17 Zn23 . 2.8211(6)
Zn18 Zn40 17_665 2.6240(8)
Zn18 Zn40 1_565 2.6240(8)
Zn18 Zn20 16_665 2.6663(4)
Zn18 Zn20 12_565 2.6663(4)
Zn18 Zn13 1_565 2.7137(5)
Zn18 Zn16 16_665 2.7788(3)
Zn18 Zn16 20_565 2.7788(3)
Zn18 Zn22 16_665 2.8737(4)
Zn18 Zn22 20_565 2.8737(4)
Zn18 Zn11 16_665 2.9064(4)
Zn18 Zn11 12_565 2.9064(4)
Zn19 Zn41 . 2.4417(13)
Zn19 Zn20 9_665 2.6595(3)
Zn19 Zn20 20_665 2.6595(3)
Zn19 Zn21 1_665 2.6772(4)
Zn19 Zn43 12_665 2.7351(8)
Zn19 Zn43 16_665 2.7351(8)
Zn19 Zn17 20_665 2.7440(4)
Zn19 Zn17 16_665 2.7440(4)
Zn19 Zn25 . 2.8756(6)
Zn19 Zn23 20_665 2.9251(4)
Zn19 Zn23 16_665 2.9251(4)
Zn19 Zn14 12_665 2.9603(5)
Zn20 Zn40 9 2.5399(9)
Zn20 Zn23 . 2.6452(4)
Zn20 Zn19 20_455 2.6595(3)
Zn20 Zn18 16_665 2.6663(4)
Zn20 Zn26 9 2.6903(4)
Zn20 Zn39 9 2.7010(10)
Zn20 Zn42 16_565 2.7087(10)
Zn20 Zn22 . 2.7381(4)
Zn20 Zn14 9 2.7508(4)
Zn20 Zn24 16_665 2.7657(4)
Zn20 Zn43 9 2.8361(8)
Zn21 Zn17 16 2.5782(5)
Zn21 Zn17 20 2.5782(5)
Zn21 Zn19 1_445 2.6772(4)
Zn21 Zn19 20_455 2.6772(4)
Zn21 Zn19 16_665 2.6772(4)
Zn21 Zn23 . 2.7342(4)
Zn21 Zn23 16 2.7342(4)
Zn21 Zn23 20 2.7342(4)
Zn21 Zn25 16_665 2.7663(5)
Zn21 Zn25 20_455 2.7663(5)
Zn21 Zn25 1_445 2.7663(5)
Zn22 Zn22 16_665 2.7004(7)
Zn22 Zn22 20_565 2.7004(7)
Zn22 Zn27 . 2.7151(6)
Zn22 Zn24 16_665 2.7296(4)
Zn22 Zn24 20_565 2.7296(4)
Zn22 Zn20 17 2.7381(4)
Zn22 Zn18 16_665 2.8737(4)
Zn22 Zn18 20_565 2.8737(4)
Zn23 Zn25 20_455 2.6136(4)
Zn23 Zn25 16_665 2.6136(4)
Zn23 Zn20 17 2.6452(4)
Zn23 Zn26 20 2.7943(3)
Zn23 Zn26 9 2.7943(3)
Zn23 Zn27 . 2.7993(5)
Zn23 Zn19 20_455 2.9251(4)
Zn23 Zn19 16_665 2.9251(4)
Zn24 Zn42 1_565 2.4024(11)
Zn24 Zn30 . 2.6980(5)
Zn24 Zn22 16_665 2.7296(4)
Zn24 Zn22 20_565 2.7296(4)
Zn24 Zn20 16_665 2.7657(4)
Zn24 Zn20 12_565 2.7657(4)
Zn24 Zn27 16_665 2.7795(3)
Zn24 Zn27 20_565 2.7795(3)
Zn24 Zn44 17_665 2.8187(12)
Zn24 Zn44 1_565 2.8187(11)
Zn24 Zn26 17_665 2.9201(4)
Zn25 Fe6 16_665 2.5784(3)
Zn25 Fe6 20_665 2.5784(3)
Zn25 Zn23 16_665 2.6136(4)
Zn25 Zn23 20_665 2.6136(4)
Zn25 Zn26 12_665 2.6878(4)
Zn25 Zn26 16_665 2.6878(4)
Zn25 Zn25 16_775 2.7121(7)
Zn25 Zn25 20_565 2.7121(6)
Zn25 Zn32 . 2.7152(6)
Zn25 Zn31 1_665 2.7460(6)
Zn25 Zn21 1_665 2.7663(5)
Zn26 Zn44 . 2.4827(9)
Zn26 Zn43 . 2.5273(7)
Zn26 Zn28 16_665 2.6418(4)
Zn26 Fe6 20 2.6595(3)
Zn26 Zn33 12 2.6713(3)
Zn26 Zn25 16_665 2.6878(4)
Zn26 Zn20 12 2.6903(4)
Zn26 Zn27 20 2.7075(3)
Zn26 Zn23 20 2.7943(3)
Zn26 Zn43 20 2.8122(8)
Zn26 Zn29 . 2.8859(3)
Zn26 Zn24 1_545 2.9201(4)
Zn27 Zn30 16_665 2.6993(3)
Zn27 Zn30 20_565 2.6993(3)
Zn27 Zn26 9 2.7075(3)
Zn27 Zn26 20 2.7075(3)
Zn27 Zn24 16_665 2.7795(3)
Zn27 Zn24 20_565 2.7795(3)
Zn27 Zn33 . 2.9118(4)
Zn27 Zn33 17 2.9118(4)
Zn28 Zn45 20 2.5728(7)
Zn28 Zn45 16_665 2.5728(7)
Zn28 Zn32 . 2.6325(6)
Zn28 Zn26 16_665 2.6418(4)
Zn28 Zn26 12_665 2.6418(4)
Zn28 Zn34 . 2.6725(5)
Zn28 Zn29 20 2.7595(3)
Zn28 Zn29 16_665 2.7595(3)
Zn28 Zn37 3_665 2.7747(4)
Zn28 Zn37 23_666 2.7747(4)
Zn28 Zn43 12_665 2.7945(8)
Zn28 Zn43 16_665 2.7945(8)
Zn29 Fe7 1_545 2.7161(4)
Zn29 Zn33 12 2.7564(3)
Zn29 Zn33 16_655 2.7564(3)
Zn29 Zn28 20 2.7595(3)
Zn29 Zn28 16_665 2.7595(3)
Zn29 Zn30 1_545 2.7708(5)
Zn29 Zn44 17_655 2.7906(11)
Zn29 Zn44 . 2.7906(11)
Zn29 Zn37 17_655 2.8056(4)
Zn29 Zn37 . 2.8056(4)
Zn29 Zn26 17_655 2.8859(3)
Zn30 Zn27 16_665 2.6993(3)
Zn30 Zn27 20_565 2.6993(3)
Zn30 Zn33 16_665 2.7221(3)
Zn30 Zn33 12_565 2.7220(3)
Zn30 Zn35 3_665 2.7255(3)
Zn30 Zn35 7_565 2.7255(3)
Zn30 Zn29 1_565 2.7708(5)
Zn30 Zn30 16_665 2.8055(5)
Zn30 Zn30 20_565 2.8055(5)
Zn31 Zn32 16_665 2.6072(4)
Zn31 Zn32 1_445 2.6072(4)
Zn31 Zn32 20_455 2.6072(4)
Zn31 Fe6 16 2.6665(3)
Zn31 Fe6 20 2.6665(3)
Zn31 Zn36 . 2.7378(5)
Zn31 Zn36 7 2.7378(5)
Zn31 Zn36 3 2.7378(5)
Zn31 Zn25 1_445 2.7460(6)
Zn31 Zn25 20_455 2.7460(6)
Zn31 Zn25 16_665 2.7460(6)
Zn32 Zn31 1_665 2.6072(4)
Zn32 Fe6 16_665 2.8040(3)
Zn32 Fe6 20_665 2.8040(3)
Zn32 Zn36 3_665 2.8110(4)
Zn32 Zn36 7_665 2.8110(4)
Zn32 Zn33 9_665 2.8161(3)
Zn32 Zn33 20_665 2.8161(3)
Zn32 Zn32 14_556 2.9504(10)
Zn32 Zn26 12_665 3.1029(5)
Zn32 Zn26 16_665 3.1029(5)
Zn33 Fe7 3_665 2.5677(2)
Zn33 Zn26 9 2.6713(3)
Zn33 Zn37 9 2.6749(4)
Zn33 Zn33 14_556 2.7059(4)
Zn33 Zn35 . 2.7147(4)
Zn33 Zn30 16_665 2.7220(3)
Zn33 Zn29 16_565 2.7564(3)
Zn33 Zn36 . 2.7762(4)
Zn33 Zn32 20_455 2.8161(3)
Zn33 Zn33 17 3.0277(5)
Zn34 Zn34 14_556 2.5118(11)
Zn34 Zn45 . 2.5406(11)
Zn34 Zn45 16_665 2.5406(11)
Zn34 Zn45 20 2.5406(11)
Zn34 Zn28 20 2.6725(5)
Zn34 Zn28 16_665 2.6725(5)
Zn34 Zn37 9_655 2.9110(4)
Zn34 Zn37 17_655 2.9110(4)
Zn34 Zn37 3_665 2.9110(4)
Zn34 Zn37 . 2.9110(4)
Zn34 Zn37 23_666 2.9110(4)
Zn35 Fe7 3_665 2.5762(3)
Zn35 Fe7 7_565 2.5762(3)
Zn35 Zn33 17 2.7147(4)
Zn35 Zn33 14_556 2.7147(4)
Zn35 Zn33 6 2.7147(4)
Zn35 Zn30 7_565 2.7255(3)
Zn35 Zn30 3_665 2.7255(3)
Zn35 Zn30 16_665 2.7255(3)
Zn35 Zn30 20_565 2.7255(3)
Zn35 Zn35 3_665 2.7568(8)
Zn35 Zn35 7_565 2.7568(8)
Zn36 Fe6 14_556 2.6638(3)
Zn36 Zn31 14_556 2.7378(5)
Zn36 Zn33 6 2.7762(4)
Zn36 Zn33 14_556 2.7762(4)
Zn36 Zn33 17 2.7762(4)
Zn36 Zn32 3_665 2.8110(4)
Zn36 Zn32 16_665 2.8110(4)
Zn36 Zn32 20_455 2.8110(4)
Zn36 Zn32 7_455 2.8110(4)
Zn37 Zn37 7 2.5016(6)
Zn37 Fe7 1_545 2.5916(4)
Zn37 Zn33 12 2.6749(4)
Zn37 Zn33 23_556 2.6749(4)
Zn37 Zn37 17_655 2.7488(8)
Zn37 Zn28 3_665 2.7747(4)
Zn37 Zn28 16_665 2.7747(4)
Zn37 Zn29 14_556 2.8056(4)
Zn37 Zn34 14_556 2.9110(4)
Zn38 Zn38 20 0.4098(19)
Zn38 Zn38 16_665 0.4098(19)
Zn38 Zn39 16_665 2.2938(13)
Zn38 Zn39 12_665 2.2938(13)
Zn38 Zn39 9_655 2.5312(10)
Zn38 Zn39 20 2.5312(10)
Zn38 Zn39 . 2.6511(12)
Zn38 Zn39 17_655 2.6511(12)
Zn38 Zn40 16_665 2.6728(11)
Zn38 Zn40 12_665 2.6728(11)
Zn39 Zn41 16_665 0.9521(14)
Zn39 Zn40 . 1.2695(15)
Zn39 Zn39 20 1.516(2)
Zn39 Zn40 17_655 1.8827(15)
Zn39 Zn38 16_665 2.2938(13)
Zn39 Zn38 20 2.5312(10)
Zn39 Zn43 . 2.5393(11)
Zn39 Zn40 20 2.6607(14)
Zn39 Zn43 20 2.6654(12)
Zn40 Zn40 17_655 0.6916(18)
Zn40 Zn39 17_655 1.8827(15)
Zn40 Zn42 . 1.9924(19)
Zn40 Zn41 16_665 2.0399(10)
Zn40 Zn44 . 2.5018(12)
Zn40 Zn20 12 2.5399(9)
Zn40 Zn18 1_545 2.6240(8)
Zn40 Zn41 20 2.6505(11)
Zn40 Zn39 20 2.6607(14)
Zn41 Zn39 12_665 0.9521(14)
Zn41 Zn39 16_665 0.9521(14)
Zn41 Zn43 16_665 2.0007(19)
Zn41 Zn43 12_665 2.0007(19)
Zn41 Zn40 12_665 2.0399(10)
Zn41 Zn40 16_665 2.0399(10)
Zn41 Zn40 20 2.6505(11)
Zn41 Zn40 9_655 2.6505(11)
Zn41 Zn14 12_665 2.7781(12)
Zn42 Zn44 . 0.9289(16)
Zn42 Zn44 17_655 0.9289(16)
Zn42 Zn40 17_655 1.9924(19)
Zn42 Zn43 17_655 2.2670(10)
Zn42 Zn43 . 2.2670(10)
Zn42 Zn24 1_545 2.4024(11)
Zn42 Zn43 9_655 2.6469(10)
Zn42 Zn43 20 2.6469(10)
Zn42 Zn45 . 2.6760(18)
Zn42 Zn20 12 2.7087(10)
Zn43 Zn43 20 0.4329(16)
Zn43 Zn44 . 1.5554(17)
Zn43 Zn44 20 1.9199(16)
Zn43 Zn41 16_665 2.0007(19)
Zn43 Zn42 20 2.6469(10)
Zn43 Zn39 20 2.6654(12)
Zn43 Zn45 . 2.6879(10)
Zn43 Zn44 17_655 2.7235(14)
Zn44 Zn44 17_655 1.262(3)
Zn44 Zn43 20 1.9199(16)
Zn44 Zn45 . 2.1145(14)
Zn44 Zn45 20 2.5019(10)
Zn44 Zn45 16_665 2.6515(12)
Zn44 Zn40 17_655 2.6705(12)
Zn44 Zn43 17_655 2.7235(14)
Zn45 Zn45 16_665 0.6112(19)
Zn45 Zn45 20 0.6112(19)
Zn45 Zn44 17_655 2.1145(14)
Zn45 Zn44 9_655 2.5019(10)
Zn45 Zn44 20 2.5019(10)
Zn45 Zn28 20 2.5728(7)
Zn45 Zn28 16_665 2.5728(7)
Zn45 Zn44 16_665 2.6515(12)
Zn45 Zn44 12_665 2.6515(12)
